Embed Size (px)
Electrodeposition of CuInSe2 and doped ZnO thin films for solar cells
Laboratory of Inorganic ChemistryDepartment of Chemistry
Faculty of ScienceUniversity of Helsinki
To be presented, with the permission of the Faculty of Science of the University of Helsinki, forpublic criticism in Auditorium A129 of the Department of Chemistry, A. I. Virtasen aukio 1, onMay 9th, 2003 at 12 o’clock noon.
ISBN 952-91-5823-8 (print)ISBN 952-10-1081-9 (pdf)
Doc. Mikko Ritalaand
Prof. Markku LeskeläLaboratory of Inorganic Chemistry
Department of ChemistryUniversity of Helsinki
Prof. Jukka LukkariLaboratory of Physical Chemistry
University of TurkuFinland
Prof. Daniel LincotLaboratoire d’Electrochimie et de Chimie Analytique
Ecole Nationale Supérieure de Chimie de ParisFrance
Prof. Enn MellikovChair of Semiconductor Materials Technology
Institute of Materials Techology Tallinn Technical University
CuInSe2 is one of the most promising absorber materials for thin film solar cells. CuInSe2-basedsolar cells have shown long-term stability and the highest conversion efficiencies of all thin filmsolar cells, above 18 %. In this study, Cu2-xSe, CuInSe2, and doped ZnO thin films wereelectrodeposited potentiostatically from aqueous solutions. The films were studied by X-raydiffraction, scanning electron microscopy, energy dispersive X-ray analysis, ion beam analysismethods, and photoelectrochemical and capacitance-voltage measurements.
For the deposition of Cu2-xSe and CuInSe2 films, a new approach was developed that utilizesinduced co-deposition. Suitable conditions for induced co-deposition were achieved bycomplexing the Cu+ ions by thiocyanate ions that shifted the reduction potential of Cu+ to thenegative direction. Under these conditions, Se reduced at more positive potentials than Cu, andinduced the formation of Cu2-xSe at more positive potentials than where the deposition ofmetallic Cu began. Cu2-xSe, in turn, induced the formation of CuInSe2 at the same potentialrange, i.e., at more positive potentials than where metallic Cu or In deposited. Theelectrochemistry of the Cu-Se and Cu-In-Se systems was studied by cyclic voltammetry andelectrochemical quartz crystal microbalance measurements that verified the depositionmechanisms.
Induced co-deposition allowed the formation of almost stoichiometric CuInSe2 films(Cu1.30In1.00Se2.20) over wide potential and concentration ranges. The as-deposited CuInSe2 filmswere amorphous and contained hydrogen, oxygen, sulfur, carbon, and nitrogen as impurities.Hydrogen and oxygen originated apparently from the aqueous deposition solution and the otherimpurities from the thiocyanate ligands. Annealing at 400 or 500 EC under nitrogen made thefilms crystalline and decreased their impurity contents substantially. Etching in KCN solutionsand addition of an In2Se3 overlayer enhanced the photoactivities of the films and shifted theircompositions towards more stoichiometric values. Also the high carrier concentrations of theannealed films decreased to more favorable values upon these treatments.
Solar cells were prepared using the electrodeposited CuInSe2 films. The ZnO top electrodes wereprepared either electrochemically, by atomic layer deposition (ALD), or by sputtering. For thefirst time, Al and In doped ZnO films (ZnO:Al and ZnO:In) were prepared by electrodeposition.The cells with electrodeposited ZnO films showed good diode characteristics in the dark. Thephotoresponses were generally higher with ZnO:In than with ZnO:Al. The highest open circuitvoltage of 0.405 V was, however, measured for a device with an electrodeposited ZnO:Al film.The ALD-ZnO films resulted in higher photocurrents, up to 5.47 mA cm-2, than theelectrodeposited ZnO films. The best photoresponses, with a maximum conversion efficiencyof 1.3 %, were measured for the devices with sputtered ZnO films.
This thesis is based on experimental work carried out during the years 1998 - 2002 in theLaboratory of Inorganic Chemistry at the Department of Inorganic Chemistry at the Universityof Helsinki. I owe my deepest gratitude to my supervisors Prof. Markku Leskelä and Doc. MikkoRitala for the excellent guidance that I have received during this work. I am also thankful to Ms.Ada Chan for revising the English language of this thesis.
I am indebted to Dr. Heini Ritala for her valuable advice, support, and great company during theyears. Also my other coworkers Dr. Timo Sajavaara, Dr. Eero Rauhala, Mr. Frédéric Dartigues,as well as Mr. Antti Niskanen, Mr. Pierre Cowache and Dr. Steffen Schuler are gratefullyacknowledged for their contributions to this work. It has been a pleasure to work with you. I alsowish to thank Dr. Seppo Lindroos who shared the office with me until recently, and Mr. MikkoHeikkilä who has worked in the electrochemistry lab during the recent years, for good company.
I wish to thank the staff in the Laboratory of Inorganic Chemistry, especially the members of thethin film group, for the wonderful and inspiring working atmosphere, as well as for great timealso outside the laboratory. Above all, I am grateful to my dear Viljami, and to my dear friendsMarko, Antti R., and Petri, for their encouragement, help and friendship.
Special thanks to my long-time friends, especially Kaisa, Janne, Esko, Pirjo and Ismo, for manygreat moments during the years. I also want to express my gratitude to my parents Leena and Markku and to my brothers Harri-Heikki and Jari-Matti. Words cannot describe how important your continuous love and supporthave been to me.
Financial support from the Foundation for Technology, the Fortum Foundation, the EmilAaltonen Foundation and the Kemira Research Foundation is gratefully acknowledged.
Helsinki, April 2003
List of original publications
This work is based on the following original publications which are referred to in the text bytheir Roman numerals. Moreover, unpublished data, including results of capacitance-voltagemeasurements and of photovoltaic characterization, are presented and discussed.
I M. Kemell, M. Ritala, H. Saloniemi, M. Leskelä, T. Sajavaara, and E. Rauhala: One-stepelectrodeposition of Cu2-xSe and CuInSe2 thin films by the induced co-depositionmechanism, J. Electrochem. Soc., 147 (2000) 1080-1087.
II M. Kemell, H. Saloniemi, M. Ritala, and M. Leskelä: Electrochemical quartz crystalmicrobalance study of the electrodeposition mechanisms of Cu2-xSe thin films,Electrochim. Acta, 45 (2000) 3737-3748.
III M. Kemell, H. Saloniemi, M. Ritala, and M. Leskelä: Electrochemical quartz crystalmicrobalance study of the electrodeposition mechanisms of CuInSe2 thin films, J.Electrochem. Soc., 148 (2001) C110-C118.
IV M. Kemell, M. Ritala, and M. Leskelä: Effects of post-deposition treatments on thephotoactivity of CuInSe2 thin films deposited by the induced co-deposition mechanism,J. Mater. Chem., 11 (2001) 668-672.
V M. Kemell, F. Dartigues, M. Ritala, and M. Leskelä: Electrochemical preparation ofdoped ZnO thin films for CuInSe2 solar cells, Thin Solid Films, in press.
The author has written all the papers and done most of the experimental work, including thinfilm growth experiments and cyclic voltammetry, cyclic photovoltammetry and EQCMmeasurements as well as photoelectrochemical, XRD, SEM, and EDX studies. The author hasalso prepared most of the solar cells and done most of the electrical characterization.
Ion beam analyses were done in the Accelerator Laboratory at the Department of Physics at theUniversity of Helsinki. Most of the ZnO growth experiments and cyclic voltammetrymeasurements reported in Paper V were done by Frédéric Dartigues under supervision of theauthor. Some of the solar cells were completed and characterized in Ecole Nationale Supérieurede Chimie de Paris or in Hahn-Meitner-Institut in Berlin.
Abstract............................................................................................................................................4Preface..............................................................................................................................................5List of original publications............................................................................................................6Contents...........................................................................................................................................7Symbols and abbreviations...........................................................................................................9
2. Thin film solar cells...............................................................................................................14
2.1. CuInSe2 solar cells......................................................................................................182.1.1. Properties of the absorber material.............................................................182.1.2. Device structure..........................................................................................202.1.3. Stability and defect chemistry of CIS.......................................................212.1.4. Effects of sodium and oxygen......................................................................23
3. Thin film deposition methods for CuInSe2-based solar cells.....................................................263.1. Absorber layer.........................................................................................................26
3.1.1. Co-evaporation from elemental sources....................................................273.1.2. Selenization of metallic precursor layers.....................................................293.1.3. Evaporation from compound sources...........................................................323.1.4. Chemical vapor deposition...........................................................................343.1.5. Close-spaced vapor transport.......................................................................353.1.6. Low-temperature liquid phase methods.......................................................353.1.7. Spray pyrolysis.............................................................................................363.1.8. Particle deposition techniques......................................................................36
3.2. Buffer layer.............................................................................................................373.3. Oxide layer..................................................................................................................43
4. Cathodic one-step electrodeposition of CuInSe2 and Cu(In,Ga)Se2 thin films..........................46
5. Characterization of thin films and their growth processes by methods based on cyclic voltammetry..........................................................................................................................57
5.1. Cyclic voltammetry combined with electrochemical quartz crystal microbalance...................................................................................................................575.2 Cyclic photovoltammetry and photoelectrochemical characterization.......................60
6. Experimental..............................................................................................................................626.1. Deposition of films......................................................................................................626.2. Characterization of films.............................................................................................626.3. Characterization of film growth processes..................................................................636.4. Post-deposition treatments..........................................................................................646.5. Preparation of solar cells.............................................................................................656.6. Electrical characterization...........................................................................................66
7. Results and discussion...............................................................................................................677.1. Cu2-xSe films................................................................................................................67
7.1.1. Film growth..................................................................................................677.1.2. Growth processes studied by cyclic voltammetry and EQCM................68
7.2. CuInSe2 films..............................................................................................................707.2.1. Film growth and characterization...............................................................707.2.2. Growth processes studied by cyclic voltammetry and EQCM.................727.2.3. Photoelectrochemical characterization......................................................747.2.4. Capacitance-voltage measurements...........................................................75
7.3. Doped ZnO films........................................................................................................767.4. Solar cells...................................................................................................................78
7.4.1. Solar cells with electrodeposited ZnO........................................................797.4.2. Solar cells with ALD-ZnO...........................................................................807.4.3. Solar cells with sputtered ZnO.....................................................................81
Symbols and abbreviations
ε0 Permittivity of vacuumεσ Dielectric constantλ Wavelength η Efficiency µ Shear modulusρ Density
A Surface areaALD Atomic layer depositionC CapacitanceCBD Chemical bath depositionCVD Chemical vapor depositionDMZ Dimethylzinc e Elemental charge (1.602x10-19 C)E Potential EE Standard potentialEC Conduction bandEF Fermi levelEg Band gapEV Valence bandECALE Electrochemical atomic layer epitaxyEDTA Ethylenediamine tetraacetic acidEDX Energy dispersive X-ray analysisEQCM Electrochemical quartz crystal microbalancef Frequencyfo Fundamental resonant frequency F Faraday constant (96485.31 C mol-1)FF Fill factorhν Photon energyI CurrentIdark Dark currentImp Photocurrent at the maximum power pointIph PhotocurrentIsc Short circuit currentILGAR Ion layer gas reactionITO Indium doped tin oxide, SnO2:In
j Current densityjdark Dark current densityjmp Photocurrent density at the maximum power point jph Photocurrent densityjsc Short-circuit current densityKs Solubility productm MassM Molar massMBE Molecular beam epitaxyMLE Molecular layer electrodepositionMOCVD Metal organic chemical vapor depositionn Number of molesNA Acceptor concentrationODC Ordered defect compoundOVC Ordered vacancy compoundPmax Maximum power point PEC PhotoelectrochemicalPLD Pulsed laser depositionPVD Physical vapor depositionQ Charge (quantity of electricity)QCM Quartz crystal microbalanceRBS Rutherford backscattering spectrometryRT Room temperatureSEM Scanning electron microscopySCE Saturated calomel electrodeTCO Transparent conducting oxideTOF-ERDA Time-of-flight elastic recoil detection analysisUPD Underpotential depositionVf Forward biasVoc Open circuit voltageVr Reverse bias XRD X-ray diffractionz Number of electrons in an electrochemical reaction
Most of the present global energy production is accomplished by burning fossil fuels. However,the inherent problems associated with the use of fossil fuels such as their limited availability andthe environmental issues force the mankind to look for new, more sustainable long-term energysolutions to provide the future energy supply.
One of the most powerful alternatives for future large scale electricity production isphotovoltaics, i.e., the conversion of sunlight directly into electricity. Sunlight is available inmost locations, and it provides such an enormous supply of renewable energy that if the wholeglobal electricity demand would be covered exclusively by photovoltaics, the total land areaneeded for light collection would be only a few percent of the world’s desert area. [1, 2] Solarcells are easy to install and use, and their operational lifetimes are long, which eliminates theneed for continuous maintenance. Since photovoltaic systems are modular, they are equally wellsuited for both centralized and non-centralized electricity production. Therefore their potentialuses range from consumer electronics (pocket calculators, wristwatches etc.) to large powerplants.
Due to its reliability and stability, solar energy is a good choice in applications where poweroutages or shortages cannot be tolerated, for example in hospitals and certain production plants.Photovoltaic systems can be installed on rooftops and facades of buildings, and they can becombined with solar water heating systems. The power generated by rooftop solar cells can beused locally, and the surplus can be exported to the commercial grid if there is one in the region.[2, 3] The possibility for local electricity production offers consumers more freedom by reducingtheir dependence on the availability and price of commercial electricity. This is a crucial featureespecially in remote areas that lack the infrastructure of electrification. It is actually more cost-effective to install a photovoltaic system than to extend the grid if the power requirement liesmore than about half a kilometer away from the electrical line . Rooftop photovoltaicinstallations, both by public institutions and by individual citizens, are becoming more and morecommon worldwide. 
One of the main obstacles for photovoltaics to become more popular in the short term is the factthat the price of the electricity (cost per watt) produced by photovoltaics is in most cases not yetcompetitive with that produced by the conventional methods. Cost reduction can be achieved byeither improving the efficiencies or reducing the production costs of photovoltaic modules.
Among the most promising absorber materials for solar cells are CuInSe2-based chalcopyritematerials (copper indium selenide, CIS). The material properties can be varied by replacing partof the indium by gallium and/or part of the selenium by sulfur to form Cu(In,Ga)(S,Se)2. Highconversion efficiencies of almost 19 %  have been achieved using these materials. Moreover,
CIS-based solar cells are very stable, and thus their operational lifetimes are long. The favorableoptical properties of these materials (direct energy band gap and high absorption coefficient)allow the use of thin films (few micrometers) of material instead of thick slices of bulk silicon,reducing the consumption of materials. CIS-based thin films can be prepared both from gas andliquid phases by a variety of methods.
Electrodeposition is a liquid phase deposition method that can be used for the preparation ofmetal, semiconductor and conducting oxide thin films. Its advantages include the feasibility ofupscaling to large substrate areas and production volumes. Moreover, the deposition equipmentis relatively simple and the deposition temperatures are considerably lower than in many othermethods. These features make electrodeposition a low-cost deposition method. Thus the fact thatthe solar cell efficiencies achieved with electrodeposited films are generally somewhat lowerthan those achieved by the more expensive gas-phase methods is not necessarily a majordrawback, since it is compensated by the lower process costs.
The purpose of this study was to develop and study electrodeposition processes for thepreparation of thin films for CuInSe2 solar cells. Cu2-xSe, CuInSe2 and doped ZnO films weredeposited from aqueous solutions. Cu2-xSe and CIS films were deposited by the induced co-deposition method  where the compound formation occurs underpotentially, that is, at lessnegative potentials than where at least one of its component ions would reduce into its elementalstate. This positive potential shift is caused by the energy released in compound formation.Reproducible film growth is achieved since the film composition is not sensitive to smallvariations in growth conditions such as precursor concentrations and deposition potential but isautomatically directed toward being stoichiometric. The most well-known example of theutilization of the induced co-deposition mechanism is CdTe . The mechanism had not beenutilized for the deposition of ternary compounds prior to [I] where suitable conditions forinduced co-deposition were achieved by complexing Cu+ ions with thiocyanate ions to formstrong complexes, thereby shifting the deposition potential of metallic Cu to negative directionwhich enables the deposition of Se first.
The formation mechanisms of Cu2-xSe and CIS thin films were studied in detail by cyclicvoltammetry and electrochemical quartz crystal microbalance measurements. The properties ofthe CIS films and the effects of post-deposition treatments were studied by cyclicphotovoltammetry, photoelectrochemical measurements and capacitance-voltage measurements.
ZnO films doped with In and Al were prepared electrochemically for the first time. Finally, solarcell structures were prepared using the electrodeposited CIS and ZnO thin films. For comparison,for some devices the ZnO films were deposited by atomic layer deposition and sputtering.
The present thesis introduces first the concept and operation principle of thin film solar cells aswell as the most important thin film solar cell materials. Next, the methods used for thepreparation of thin films used in CuInSe2 solar cells are reviewed, with particular attention toelectrodeposition of CuInSe2-based absorber materials. Last part of the literature survey dealswith cyclic voltammetry and related methods used for the characterization of thin films andgrowth processes in this study. After the experimental details, the main results of this study willbe presented and discussed.
2. Thin film solar cells
Solar cells, or photovoltaic devices, are devices that convert sunlight directly into electricity. Thepower generating part of a solid-state solar cell consists of a semiconductor that forms arectifying junction either with another semiconductor or with a metal. Thus, the structure isbasically a pn-diode or a Schottky diode. In some junctions, a thin insulator film is placedbetween the two semiconductors or the semiconductor and the metal, thereby forming asemiconductor-insulator-semiconductor or a metal-insulator-semiconductor junction. Moreover,pn-junctions may be classified into homojunctions and heterojunctions according to whether thesemiconductor material on one side of the junction is the same as or different from that on theother side. Also liquid-junction solar cells exist where the junction is formed between asemiconductor and a liquid electrolyte. Thin film solar cells are usually pn- or pin-diodes, andtherefore only these types of devices are discussed here in more detail.
When the junction is illuminated, the semiconductor material absorbs the incoming photons iftheir energy hν is larger than that of the band gap of the semiconductor material. The absorbedphotons are converted into electron-hole pairs. These photogenerated electron-hole pairs areseparated by the internal electric field of the junction: holes drift to one electrode and electronsto the other one. [4, 8]. The electricity produced by a photovoltaic device is direct current andcan be used as such, converted into alternating current, or stored for later use.
Figure 1 presents a schematic energy band diagram of a pn-heterojunction solar cell (a) atthermal equilibrium in dark, (b) under a forward bias, (c) under a reverse bias, and (d) underillumination, open circuit conditions. Numbers 1 and 2 in Figure 1 refer to an n-type and a p-typesemiconductor, respectively, and ECi and EVi to their conduction and valence bands, respectively.Egi and EFi are the band gaps and Fermi levels, respectively. In the absence of an applied potential(Fig. 1a), the Fermi levels of the semiconductors coincide, and there is no current flow. Aforward bias Vf (Fig. 1b) shifts the Fermi level of the n-type semiconductor upwards and that ofthe p-type semiconductor downwards, thus lowering the potential energy barrier of the junction,and facilitating the current flow across it. The effect of a reverse bias Vr (Fig. 1c) is opposite: itincreases the potential barrier and thus impedes the current flow. Illumination of the junction(Fig. 1d) creates electron-hole pairs, causing an increase in the minority carrier concentration.The potential energy barrier decreases, allowing the current to flow, and a photovoltage VOC
(photovoltage under open circuit conditions, or open circuit voltage) is generated across thejunction. [4, 9]
Figure 1. A simplified energy band diagram of a pn-heterojunction solar cell (a) at thermal equilibriumin dark (b) under a forward bias (c) under a reverse bias and (d) under illumination, open circuitconditions.
Solar cells are characterized by current-voltage (I-V) measurements in the dark and understandardized illumination that simulates the sunlight [10, 11]. Figure 2 shows an example ofdiode characteristics of a solar cell in the dark and under illumination. The most importantparameters that describe the performance of a solar cell (open circuit voltage VOC, short circuitcurrent density jSC and fill factor FF) can be derived from the I-V curve measured underillumination.
Figure 2. Current-voltage characteristics of a solar cell in dark and under illumination
The open circuit voltage is limited by the band gap energy Eg of the absorber material, and itsmaximum value is calculated by dividing the band gap energy by the charge of an electron(Eg/e). Because of electron-hole pair recombination, the open circuit voltages of real solar cellsare considerably below their maximum limits. The maximum value of short circuit current
density, in turn, is the photogenerated current density jph  that depends on the amount ofabsorbed light. Fill factor, which describes the shape of the illuminated I-V curve, is expressedaccording to the following equation:
FFV jV j
where Vmp represents the photovoltage and jmp the photocurrent at the maximum power point Pmax.The conversion efficiency η of a solar cell is simply the ratio of the incoming power to themaximum power output Pmax = Vmpjmp that can be extracted from the device:
η =V j
Based on the above considerations, the band gap value is one of the most important propertiesof the absorber material of a solar cell. The optimum band gap value for the absorber materialof a single-junction solar cell is about 1.5 eV which results in a theoretical maximum efficiencyof 30 % . This is because VOC and FF increase, and jSC decreases with increasing band gap. Even higher efficiencies can be achieved with tandem solar cell structures or by using solarirradiation concentrators, but these are not included here.
Most commercial solar cells of today are made of mono- or polycrystalline silicon. Silicon is avery abundant and well-known material of which a lot of experience has been gained over thedecades - the first pn-junction solar cell based on crystalline silicon was made already in the1950's . Silicon photovoltaics owes a lot to the microelectronics industry that has gained theknowledge of the material properties as well as developed the manufacturing techniques.Additionally, rejects from microelectronics industry have served as a supply for high qualitysource material that has thus been available at a relatively low price. [8, 13]
However, owing to its indirect band gap, silicon is not an ideal absorber material for solar cells.Semiconductor materials with indirect band gaps do not absorb light as efficiently as those withdirect band gaps, and therefore a thick layer of material is needed to achieve sufficient lightabsorption. For example, 100 µm of crystalline silicon is needed for 90 % light absorption incomparison with 1 µm of GaAs that is a direct band gap semiconductor.  An inevitable resultof such a large thickness is that the silicon used in solar cells must be of very high quality inorder to allow for minority carrier lifetimes and diffusion lengths long enough so thatrecombination of the photogenerated charge carriers is minimized, and they are able to contribute
to the photocurrent. These strict material requirements increase the production costs. Moreover,due to the current production technologies, material losses during the fabrication of silicon solarcells are high.
The high production costs of crystalline silicon solar cells are compensated by their highefficiencies. Moreover since the 1950's, an important application of silicon solar cells has beenas power sources in space vehicles where reliability and high efficiency are far more importantissues than the cost. Also other expensive high-efficiency materials, such as GaAs and InP havebeen used in space applications. 
Due to the limitations of crystalline silicon, other absorber materials have been studiedextensively. These are semiconductors with direct band gaps and high absorption coefficients,and consequently they can be used in thin film form. Thin film solar cells have severaladvantages over crystalline silicon cells . The consumption of materials is less because thethicknesses of the active layers are only a few micrometers. Therefore, impurities and crystallineimperfections can be tolerated to a much higher extent as compared to crystalline silicon. Thinfilms can be deposited by a variety of vacuum and non-vacuum methods on inexpensivesubstrates such as glass. Also curved and/or flexible substrates such as polymeric sheets can beused, leading to lighter modules. Furthermore, composition gradients can be obtained in a moreeasily controllable manner.
The main candidates for low-cost thin film solar cell materials are amorphous hydrogenatedsilicon (a-Si:H), CdTe (cadmium telluride) and CuInSe2 and its alloys with Ga and/or S. [14, 15]Of these, amorphous silicon solar cells have currently the largest market share.  Theabsorption coefficient of amorphous silicon is higher than that of crystalline silicon whichenables its use in thin film form, and its band gap is closer to the ideal value of about 1.5 eV. Aserious disadvantage is the light-induced degradation of solar cells made of this material whichleads to a drop of conversion efficiency from the initial value.  This Staebler-Wronski effectresults from defects (dangling bonds) created by illumination that act as recombination centers.The stabilized efficiencies of amorphous silicon solar cells are quite low, about 13 % .
The polycrystalline compound semiconductor materials (CdTe and Cu(In,Ga)(S,Se)2) do notsuffer from light-induced degradation. In fact, the performances of CIS-based solar cells haveeven shown some improvement after illumination under normal operating conditions [16, 17].Another advantage is that they are direct band gap materials that have high absorptioncoefficients. The band gap of CdTe (1.4 eV) is very close to the ideal value. Despite that, therecord efficiency for CdTe solar cells is only 16.5 % .
2.1. CuInSe2 solar cells
2.1.1. Properties of the absorber material
The band gap of CuInSe2 is relatively low, 1.04 eV, but it can be adjusted to better match thesolar spectrum by substituting part of In by Ga or part of Se by S. The flexibility of the materialsystem allows in principle the band gap variation from 1.04 eV of CuInSe2 via 1.53 eV of CuInS2
and 1.7 eV of CuGaSe2 (CGS) to 2.5 eV of CuGaS2 . The ternary Cu-chalcogenidescrystallize in the tetragonal chalcopyrite structure . Sometimes, however, the cubicsphalerite phase , a disordered form of the chalcopyrite, is observed. The Cu-chalcopyritesexhibit the highest efficiencies among thin film solar cells – the present record efficiency is 18.8% for a device with a Cu(In,Ga)Se2 (CIGS) absorber . The Ga/(Ga+In) ratio in the absorberis about 25-30 %, and the resulting band gap is between 1.1 and 1.2 eV . An additionaladvantage of the Cu-based absorber materials is that they do not have the acceptability problemsassociated with CdTe since these materials are less toxic . Nevertheless, the Cd issue issomewhat shared also by the Cu(In,Ga)(Se,S)2 technology because a CdS buffer layer iscommonly used. The amount of Cd is, however, much less in the Cu(In,Ga)(Se,S)2 cells than inthe CdTe cells since the CdS layer is very thin.
One would expect that the higher band gap absorbers of the Cu(In,Ga)(S,Se)2 system wouldresult in devices with higher conversion efficiencies, but this is not the case – conversionefficiencies achieved by CuInS2 or CuGaSe2 absorbers lag far behind those achieved byCu(In,Ga)Se2 or even CuInSe2. This is partly due to the longer research history of CuInSe2 andCu(In,Ga)Se2 solar cells, but also due to some fundamental differences between the low bandgap (CuInSe2 and Cu(In,Ga)Se2 with a low Ga content) and wide band gap (CuInS2 andCuGaSe2) materials.  Of these, issues related to doping and recombination are describedbriefly in the following.
The overall composition of the photovoltaic-quality Cu(In,Ga)Se2 absorber film is slightly Cu-deficient, with a thin, even more Cu-deficient surface layer, the composition of whichcorresponds to the stable ordered vacancy or ordered defect compound (OVC/ODC)Cu(In,Ga)3Se5. [16, 23, 24]. The formation of this OVC layer occurs automatically on the topsurfaces of Cu-deficient Cu(In,Ga)Se2 thin films at high deposition temperatures , thusresulting in significant differences between the bulk and surface compositions of photovoltaic-quality Cu(In,Ga)Se2 films. The OVC surface layer is weakly n-type , and since the bulk ofthe absorber is p-type, they form a buried pn-junction [16, 23, 25]. The inverted surfaceminimizes the recombination at the CIGS/CdS interface . The thickness of the OVC layeris about 10 nm . Thicker, deliberately prepared OVC layers have been reported to result indeteriorated device performances  which was attributed to increased series resistancebecause of the low conductivity of the OVC and light absorption in the OVC instead of the
junction region. The band gap of the surface layer is direct and wider than that of the bulk, valuesbetween 1.23  and 1.3 eV  have been observed, in agreement with the predicted valueof 1.21 eV . The wide band gap of the surface layer increases further the barrier forrecombination at the CIGS/CdS interface. .
In agreement with the doping pinning rule of Zhang et al. , CuInSe2 and CuInS2 can be eitherp-type or n-type, depending on the composition. CuGaSe2, in contrast, is always p-type whichprevents the formation of the inverted surface. A factor that limits the use of CuInS2 is thatattempts to prepare Cu-poor CuInS2 lead often to the formation of n-type CuIn5S8. 
Recombination in the bulk of the absorber is the main loss mechanism in CuInSe2, Cu(In,Ga)Se2
and CuGaSe2 solar cells [31, 32]. Increased recombination losses observed in CuGaSe2 cells ascompared to CuInSe2 or Cu(In,Ga)Se2 cells are due to increased contribution of tunneling to therecombination in the bulk of the absorber.  Recombination mechanisms of CuInS2 cells, inturn, differ in the dark and under illumination: bulk recombination dominates in the dark andinterface recombination dominates under illumination . This is probably due to the difficultyof preparing CuInS2 absorbers with Cu-poor composition since according to Turcu et al. interface recombination dominates in all devices where the final absorber composition is Cu-rich. In all cases, the open circuit voltages of the cells correlate inversely with the defectdensities of the absorbers, measured by admittance spectroscopy. [22, 32] This is particularlymanifested by the fact that the open circuit voltages of CuInSe2 solar cells increase linearly withthe addition of Ga to the absorber, until a Ga/(Ga+In) ratio of about 30 % and a band gap ofabout 1.2 eV is reached. The increase of the open circuit voltages is faster than that of the bandgap, and is accompanied by a decreasing defect density. Beyond the Ga/(Ga+In) ratio of about30 %, the increase of VOC slows down [32, 34], accompanied by an increase of the defect density[32, 35]. Thus the optimum composition of a CIS-based absorber film seems to be Cu(In,Ga)Se2
with a Ga/(Ga+In) ratio of about 25-30 %. The Ga content and therefore the band gap of theabsorber is usually graded in such a way that the regions near the Mo back contact contain moreGa than those closer to the film surface . This grading enhances the separation of thephotogenerated charge carriers and reduces recombination at the back contact [36, 37].Moreover, as explained above, since the open circuit voltage increases and the short circuitcurrent decreases as a function of the band gap, careful design of the grading profile allows aseparate optimization of the open circuit voltage and short circuit current density: the higherband gap value of the graded material determines the open circuit voltage and the lower valuethe short circuit current density [36, 38].
2.1.2. Device structure
Figure 3 shows a schematic representation of a CIGS solar cell. Cell preparation starts by thedeposition of the Mo back contact on glass, followed by the p-type CIGS absorber, CdS or otherweakly n-type buffer layer, undoped ZnO, n-type transparent conductor (usually doped ZnO orIn2O3), metal grids and antireflection coating. Finally, the device is encapsulated to protect itagainst its surroundings.
Figure 3. A schematic view of the CIS solar cell structure
The structure of a CIGS cell is quite complex since it contains several compounds as stackedfilms that may react with each other. Fortunately, all detrimental interface reactions are eitherthermodynamically or kinetically inhibited at ambient temperatures. The formation of a thin p-type MoSe2 layer between the Mo and the absorber that occurs during the absorber preparationat sufficiently high temperatures under (In,Ga)xSey-rich growth conditions [39, 40] is beneficialfor the cell performance for several reasons: first, it forms a proper ohmic back contact. TheMo/CIGS contact without the MoSe2 layer is not an ohmic but a Schottky type contact whichcauses resistive losses. [39, 41] Another advantage is the improved adhesion of the absorber tothe Mo back contact. Further, since the band gap of MoSe2 is wider (about 1.4 eV ) than thatof a typical CIGS absorber, it forms a back surface field for the photogenerated electrons [29,39, 42], providing simultaneously a low-resistivity contact for holes . The back surface fieldreduces recombination at the back contact since the insertion of a wider band gap layer (of thesame conductivity type as the absorber) between the back contact and the absorber creates apotential barrier that confines minority carriers in the absorber . Finally, the MoSe2 layerprevents further reactions between CIGS and Mo .
A moderate interdiffusion of CdS and CIGS, that occurs to some extent in photovoltaic-qualitymaterial too [44, 45], is potentially beneficial to the cell performance.  Further, the reactionof CdS with CIGS to form detrimental Cu2S is inhibited as long as photovoltaic-quality (Cu-deficient) material is used. Similar stability is not present at a CIGS/ZnO interface since Cu-poorCIGS may react with ZnO to form ZnSe and In2O3 or Ga2O3 . This, in addition to the sputter-induced damage during ZnO deposition (see Chapter 3.3), may contribute to the lowerefficiencies of buffer-free devices. 
Figure 4 shows the structure of an alternative, inverted configuration. The preparation of this so-called superstrate cell starts with the deposition of the transparent conductor, followed by theabsorber deposition. The CdS layer is usually omitted in modern superstrate cells because thehigh absorber deposition temperatures would cause its intermixing with the CIGS layer. [46, 47]The advantages of the inverted configuration include lower cost, easier encapsulation and thepossible integration as the top cell in future tandem cells.  The conversion efficienciesachieved by superstrate cells are, at least so far, several percentage units lower than those of thesubstrate cells. This may be due to the fact that the substrate cells have been studied to a muchgreater extent than the superstrate cells. Because of these reasons, superstrate cells are notconsidered here in more detail.
Figure 4. A schematic view of a CIS superstrate solar cell structure
2.1.3. Stability and defect chemistry of CIGS
In addition to the conversion efficiency, another crucial issue of a solar cell is its stability sinceit affects directly the cost of the electricity produced, and thus the energy payback time. Despitethe complex solid state chemistry of the CIGS solar cell structure, they have shown exceptionallystable performances both under normal operating conditions [16, 17] as well as under harshconditions such as irradiation by X-rays , electrons [49-51], or protons [50, 52, 53].Radiation hardness demonstrates the suitability of CIGS cells to space applications.
Besides the interfacial stability discussed above, the most important factors that contribute to the
electrical and chemical stability of the CIS-based solar cells are the unique properties of theabsorber material, especially the wide single-phase domain and the fact that the doping levelremains non-degenerate (below 1018 cm-3) over a wide composition range. Both of these effectsresult from the strong self-compensation of the chalcopyrite compounds: defects that are causedby deviations from the stoichiometry are compensated by new defects that neutralize them, i. e.,formation energies of the compensating ionic defects are low. As a result, most of the defects ordefect complexes are electrically inactive with respect to the carrier recombination. 
According to Zhang et al. , the formation energies of defects and defect complexes inCuInSe2 are low. The energetically most favored isolated point defect is the shallow coppervacancy VCu that contributes to the very efficient p-type doping ability of CIS. The mostfavorable defect complex is (2VCu + InCu) that prevents degenerate doping in In-rich material.Because of the high concentration of (2VCu + InCu) complexes, they interact with each otherwhich lowers the formation energies further. The existence of the ordered defect compounds(ODC) CuIn3Se5, CuIn5Se8 etc. may be explained as periodically repeating (2VCu + InCu) units.Other defects may be present too but their formation energies are higher. 
CIGS solar cells exhibit electrical metastabilities that are manifested as the increase of the opencircuit voltage and improvement of fill factor upon illumination, and the effect of reverse biasingthe junction. Illumination-induced metastabilities may occur both in the absorber or at theCIGS/CdS interface, depending on the wavelength of illumination. [40, 54] Effects caused bylong-wavelength (red) illumination are related to the CIGS absorber since red light (lowenergies) is mostly absorbed in CIGS. Red illumination causes a metastable increase of netcarrier concentration, which decreases the width of the space charge layer. The open circuitvoltage increases due to the reduced recombination in the narrower space charge layer.  Thusthe increase of the open circuit voltage upon illumination is related to the CIGS absorber. [40,54]
Short-wavelength illumination (blue light), in turn, affects mostly the regions at or near theCdS/CIGS interface. Blue light is to a great extent absorbed into the buffer layer, and thephotogenerated holes are injected into the near-surface region of the CIGS absorber .Illumination by blue light has been reported to improve the fill factor which probably resultsfrom the ionization of deep donors in CdS. The positively charged fixed donors cause downwardband bending in the CdS and reduce the barrier height to electrons. [40, 55] The photogeneratedholes have also been suggested to neutralize the negative defect states that are present on theCIGS surface . The improvement of the FF upon illumination is therefore related to theCIGS/CdS interface.
Reverse bias has the opposite effect, and since it can be counterbalanced by blue illumination,it is reasonable to attribute also the effect of reverse bias to the interface region. Reverse bias
generates negative charge states to the buffer layer and to the surface defect layer of CIGS. These negative charges may be neutralized by blue illumination. 
Thus the illumination-induced defect reactions are beneficial to the device performance, andmoreover reversible. Self-annealing of the metastable states prevents accumulative long-termdamage since it occurs at ambient temperatures and with an adequate time scale. 
Radiation hardness has also been suggested to be due to the self-repair of the radiation-induceddamages rather than due to the resistance of the material to damage. The self-healing mechanismis a result of the mobility of Cu and reactions involving Cu-related defects or defect complexes. Thus the electrical stability of the CIGS material system seems to be of dynamic naturerather than static. The material is not resistant to changes but it is flexible because of inherentself-healing mechanisms. Particularly, the mobility of Cu, as well as the high defect density ofCIGS, are actually advantages in CIGS since they help in repairing damages, thus contributingto the unusual impurity tolerance and to the radiation hardness. Also the Cu-poor surfacecomposition of photovoltaic-quality CIGS films has been proposed to result from the migrationof Cu in the electric field of the space charge region.  The wide range of possible preparationtechniques and preparation conditions for Cu-chalcopyrites has been suggested to be anindication of a stable energetic minimum that can be reached via different routes .
2.1.4. Effects of sodium and oxygen
Yet another interesting feature is the beneficial effect of sodium on the structural and electricalproperties of Cu-chalcopyrite thin films. The phenomenon was discovered in 1993 [57, 58] whensolar cells prepared on soda lime glass substrates showed considerably higher efficiencies thanthose prepared on borosilicate glass. X-ray photoelectron spectroscopy and secondary ion massspectrometry studies revealed the presence of Na at relatively high concentrations both on thesurface and in the bulk of the CIGS films deposited on Mo/soda lime glass.  Sodium isnormally detrimental to semiconductors but its presence during the growth of CIS-based filmshas been reported to increase the grain size [57-60], smoothen the surface morphology [59, 60],enhance the crystallinity and (112) orientation [57-62], and increase the p-type conductivity(carrier concentration) [61-65]. Sodium has been suggested to aid the formation of the beneficialMoSe2 layer between Mo and CIGS . As a result, improved solar cell efficiencies have beenobtained in the presence of Na [59-64].
Sodium thus affects both the growth and the doping of Cu-chalcopyrite films. Na+ ions migratefrom the substrate to the CIGS film along grain boundaries , and their incorporation into aCIGS film occurs via interaction with Se [66, 67]. The Na contents in the CIGS films are quitehigh, typically about 0.1 at.% or higher [61, 65, 66, 68, 69]. According to Granata et al. , the
ideal Na content in CIS and CIGS films is between 0.05 and 0.5 at.%. Most of the sodium islocated at the film surface, near the Mo back contact, or at the grain boundaries [60, 62, 64-67,70].
In an attempt to explain the influence of Na on the structural properties of CIGS films preparedby co-evaporation, Braunger et al.  proposed a model according to which Na+ ions diffuseto the CIGS surface along grain boundaries and react subsequently with the elemental seleniumto form sodium polyselenides (Na2Sex, x = 1-6 …5). When the Se partial pressure is low, mainlyNa2Se is formed. Na2Se is a very stable compound which renders the release of Se from it highlyunlikely. Thus, no Se is available for the growth of the CIGS film. At higher Se pressures, theformation of polyselenides dominates. Because of the easier release of Se from them,polyselenides act as a Se source during the growth.
The increased p-type conductivity of Na-containing Cu-chalcopyrite films is generally attributedto the suppression of donor-type defects such as InCu [62, 63, 71, 72] that act as majority carriertraps. On the other hand, the removal of a minority-carrier trap state has also been reported .
As explained in Chapter 2.1.3, the concentration of InCu in photovoltaic-quality films is high.Sodium eliminates the InCu-related donor states or inhibits their formation by incorporating atthe Cu site which results in an increased hole concentration [62, 69]. The calculations of Wei etal.  support the conclusion that the main effect of sodium on the electronic properties of CISis to reduce the amount of intrinsic donor defects. When present at low concentrations, Naeliminates first the InCu defects which results in a higher p-type conductivity.  This removalof InCu antisites may lead to a more ordered structure which may explain also the enhanced (112)orientation.  Wei et al.  even propose the formation of layered NaInSe2 that directs theCIS film to the (112) orientation.
Overly high Na doses are detrimental to the electronic properties since they result in theelimination of VCu acceptor states and thereby reduce the carrier concentration.  On the otherhand, Na contents of higher than 1 at.% were reported to increase the carrier densities toexcessively high values (above 1018 cm-3) which reduced the cell performances. This may be dueto the formation of Na-containing compounds . The formation of additional phases at toohigh Na concentrations has in fact been observed , and it may result from the limited mutualsolubility of NaInSe2 and CuInSe2 .
In most cases, the diffusion of Na into the absorber film from the soda lime glass through the Moback contact at high deposition temperatures is considered to provide a sufficiently high Naconcentration, but deliberate incorporation of Na by introducing Na-containing precursors suchas NaF [59, 60, 63], Na2S [70, 71], Na2Se [64, 73], NaxO , NaHCO3  or elemental Na, has also been studied. The advantage of this approach is the possibility of a better control
over the sodium content and thus a better reproducibility since the Na supply from the glassdepends on the absorber deposition process as well as on the properties of the Mo back contact[59, 73] and the glass itself . Thus, the amount of Na diffusing from the substrate is difficultto estimate accurately. Moreover, since the diffusion of Na from the substrate slows down at lowtemperatures, the deliberate addition of Na allows one to use lower deposition temperatureswithout so much degradation of the cell efficiency [60, 61]. For instance, Bodegård et al. were able to decrease the CIGS deposition temperature from 510 to 425 EC with essentially nodegradation of the conversion efficiency. In another study , the conversion efficiencydecreased only 1.3 percentage units upon decreasing the deposition temperature from 550 EC to400 EC in the presence of additional sodium. In both cases, the efficiencies achieved underinsufficient supply of sodium were several percentage units lower. [60, 61] Furthermore,preparation of efficient superstrate cells may require the deliberate addition of Na since itsdiffusion from the glass is blocked by the transparent conductor  or the thin Al2O3 layer thatis often present under commercial conducting oxide thin films.
Effects of other alkali metal fluorides (LiF , KF  and CsF ) have also been studied.The addition of LiF was reported to cause an increased grain size and enhanced (112) orientationbut to a smaller extent than NaF. The grain sizes were comparable to those of the Na-containingfilms but the film surfaces were rougher.  The addition of KF increased the conductivitysomewhat, but CsF had in some cases the opposite effect since it decreased thephotoconductivity.  Thus, NaF had the highest influence on the film properties. In the caseof LiF, this may result from its higher chemical stability as compared to NaF which results in adifferent decomposition behavior . The smaller influence of KF and CsF was explained bythe differences in the ionic radii: the smaller ionic radius of Na helps its substitutionalincorporation into the chalcopyrite lattice .
In addition to the effects discussed above, Na also enhances the influence of oxygen in the CIS-based films [74-77]. The main role of oxygen is the passivation of positively charged Sevacancies (VSe) that are present on the surfaces and grain boundaries of the Cu-chalcopyrite thinfilms. [72, 76, 77]. The presence of Se vacancies at grain boundaries is especially detrimentalsince they decrease the effective p-type doping of the film. Additionally, they act asrecombination centers for the photogenerated electrons [75-78]. The passivation of Se vacanciesis therefore of significant importance to the performance of the solar cell. [75-77] Air-annealinghas in fact been used routinely to improve the photovoltaic properties of the CIGS solar cells. Physisorbed oxygen that is present on the surfaces and grain boundaries of oxygen-exposedCIGS films, chemisorbs as O2- which occupies the positively charged vacant Se sites, and thusobviates their disadvantageous effects. Sodium has been suggested to promote the formation ofchemisorbed O2- ions by weakening the O-O bond [72, 74, 75]. The correlated concentrationdistributions of these two elements in air-exposed CIGS films [62, 64, 66, 70, 74] support thisidea.
3. Thin film deposition methods for CuInSe2-based solar cells
A wide range of preparation methods exist for the thin film materials used in the CIS-basedsolar cells. The deposition method has generally a large impact on the resulting film propertiesas well as on the production cost. In this section, the most important deposition methods arereviewed, with the main focus on those used for the absorber deposition. Moreover, sinceCuInSe2 and Cu(In,Ga)Se2 are the most important Cu-chalcopyrite absorber materials, they areemphasized in this presentation. To some extent the deposition methods apply to CuGaSe2 andCuInS2 films as well.
The preparation of a standard CIS-based solar cell involves several steps every one of which isimportant. The preparation of a normal substrate configuration Cu-chalcopyrite solar cell startsfrom the deposition of the 1-2 µm thick Mo back contact that is most often sputtered. The qualityof the back contact and its adhesion to the underlying glass substrate are very important issues.After the deposition of absorber, buffer, and transparent conductor, metal grids (most often Alor Ni/Al) are deposited on the transparent conductor in order to enhance its conductivity. Finally,an antireflection coating (MgF2) is added in order to minimize reflection losses and thus increasethe efficiency.
3.1. Absorber layer
Although various techniques can be used to obtain stoichiometric CIS and CIGS films, only afew of them have resulted in high efficiency (over 15 %) solar cells so far. The absorber filmsfor the high efficiency solar cells are usually prepared either by co-evaporation from elementalsources or by reactive annealing of precursor films (elemental or compound layers) underselenium-containing atmospheres. 
Regardless of the deposition method, the absorber films of CIS-based high-efficiency deviceshave smooth surface morphologies and consist of large, densely packed grains. The films arecrystalline with the chalcopyrite structure , and their overall compositions are slightly Cu-deficient, in order to enable the formation of the Cu-poor ordered vacancy compound (OVC) onthe surface [23, 29]. Also, no additional phases are allowed in the films, copper selenide phasesespecially are detrimental to the solar cell performance since, being a degenerate semiconductor,Cu2-xSe is very conductive which results in high dark currents.
The formation of a photovoltaic-quality film requires generally a high temperature (400 EC orabove) during film growth or post-deposition annealing. The formation of Ga-containing phases(CGS and CIGS) requires generally higher temperatures or longer reaction times than for CIS[24, 79-82]. Higher temperatures also facilitate the formation of the MoSe2 interlayer . The
formation of a Cu-rich phase during the earlier stages of the growth enhances the formation ofsmooth, dense, and large-grained films. The presence of Na during the growth has a similareffect as well as other beneficial consequences, as reviewed in Chapter 2.1.4. As the high processtemperatures may cause the loss of Se, that must be compensated for, for instance by maintaininga Se-containing atmosphere.
3.1.1. Co-evaporation from elemental sources
The most successful absorber deposition method for high-efficiency small-area devices seemsto be the three-stage co-evaporation of CIGS from elemental sources in the presence of excessSe vapor [36, 83]. Deposition is often performed under ultra high vacuum conditions using amolecular beam epitaxy (MBE) system. The three-stage process, developed at the US NationalRenewable Energy Laboratory (NREL), is based on the bilayer process of Boeing  thatinvolves the co-evaporation of Cu-rich CIGS layer at a lower substrate temperature (450 EC),followed by In-rich layer at a higher temperature (550 EC). The layers intermix, forming ahomogeneous film with a slightly Cu-deficient overall composition. The three-stage processinvolves first the deposition of (In,Ga)2Se3 at a lower substrate temperature (about 300-350 EC)and then the evaporation of Cu and Se at a higher temperature (500-560 EC) to yield Cu-richCIGS. After adding some more (In,Ga)2Se3, a slightly Cu-deficient final film composition isachieved. A Se vapor treatment is carried out during the cooling step.  The Ga/(Ga+In) ratiois usually varied as a function of depth. Since the band gap of CGS is higher than that of CIS,the graded Ga content results in a graded band gap of about 1.1 to 1.2 eV which in turn improvesthe separation of the photogenerated charge carries and reduces recombination at the backcontact . For example, in the NREL world record cell the Ga/(Ga+In) ratio is about 30 %near the Mo back contact and about 25 % on the top surface .
CIGS films prepared by the three-stage co-evaporation process have resulted in solar cellefficiencies of around 18 % by many groups: world record 18.8 % of NREL , 18.5 % ofMatsushita , 18.0 % of Aoyama Gakuin University of Tokyo , 17.6 % of Tokyo Instituteof Technology , as well as the best Cd-free device with a CBD-ZnS buffer of 18.1 % .
A remarkable feature in  is that the CIGS films were (220/204) oriented – the typicalorientation of chalcopyrite CIGS films is either random or (112). The orientations of CuInSe2
and CIGS thin films were shown to depend on the orientation of the underlying (In,Ga)2Se3
precursor layer which in turn was a function of the properties of the Mo layer such asmorphology, grain size and stress. The (220/204) oriented CuInSe2 thin films were achieved onlyon dense, almost pinhole-free, large-grained Mo films with low tensile stress and a low Nacontent on the surface.  Under Na-free conditions , the film orientation was found todepend on the substrate orientation, i.e., (100) oriented Mo resulted in (112) oriented CIGS and
(110) oriented Mo in (220/204) oriented CIGS. The orientation of the (In,Ga)2Se3 precursor wasalso dependent on the Se/(In+Ga) flux ratio and substrate temperature during the evaporation.High flux ratios increased the (220/204) orientation of CIGS by increasing the (300) orientationof the (In,Ga)2Se3 precursor. Increasing substrate temperature was reported to have the oppositeeffect. 
The (220/204) oriented films were found to be more resistive than the (112) oriented films, andtheir apparent band gaps were lower than those of the (112) oriented films. The higherconversion efficiencies achieved with the (220/204) oriented absorbers were mainly due toincreased fill factors and lower series resistances, whereas the jSC and VOC were in most casesonly moderately higher.  The increase of the efficiency from 15.5 % with the (112) orientedabsorber to 17.6 % with the (220/204) oriented one may be explained by an easier diffusion ofCd atoms during the deposition of CdS into the (220/204) oriented films. Possible reasons area higher dissolution rate of Cu into an NH3 solution from the (220) surfaces and/or the fact thatthere are less atoms on the (220) surface as compared to the (112) surface. 
Co-evaporation can also be performed with a constant Cu/(In+Ga) flux ratio through the entireprocess. It was shown  that the flux ratio profile did not have a large impact on the deviceefficiency (best 16.4 %) when the co-evaporation was done at 550 EC. At 400 EC, in contrast,the presence of a Cu-rich growth stage improved the device efficiencies (best 14.1 %), whetherin the beginning or in the middle of deposition .
In order to gain information about the material properties such as defects, high-quality CIS andCGS films have been deposited on GaAs and InGaAs  and on Si  by MBE. The use ofepitaxial films in these studies eliminates the effects of grain boundaries and other non-idealities,and allows thus to get reliable and reproducible information of the intrinsic properties of thematerials. [91, 92]
Despite its unquestionable power in preparing high-quality material on small areas, co-evaporation exhibits some problems related to upscaling. This is due to the fact that co-evaporation requires a strict control of the evaporation fluxes to achieve the desired filmproperties such as composition, texture, and electrical properties. This is particularly difficultwith large substrate areas. As an inevitable consequence, the conversion efficiencies of large areacells and modules are considerably lower than those of the smaller-area devices , forexample the efficiency reported by Matsushita laboratories was 12.6 % for a 81.54 cm2
submodule  as compared to 18 % for a small-area cell . Moreover, in addition to thesophisticated and expensive equipment, the high deposition temperatures and incompleteutilization of source materials add to the complexity and cost of the co-evaporation method. 
According to ZSW/Würth Solar , the production of CIGS modules by co-evaporation should,
however, be possible well below the common market price of the crystalline Si solar celltechnology. Their in-line co-evaporation process [95, 96] is based on one-step co-evaporationof Cu, In, Ga, and Se from elemental sources onto moving substrates at high temperatures.Efficiencies of 30 cm x 30 cm CIGS modules average 11.3 %, with a maximum value of 12.7%. The maximum efficiency for a Cd-free module of the same size was 9.7 % .
3.1.2. Selenization of metallic precursor layers
Although the difficulties in upscaling are somewhat shared by all the deposition methods, thealternative multistep approach where the absorber is prepared by combination of simple, well-established deposition techniques for the more simple precursor layers offers certain advantages:compositional uniformity over large areas may be easier to achieve, and in many cases thethroughput is increased as compared to the co-evaporation. Moreover, the processes are oftenvery cost-effective because of the low deposition temperatures. This is important because apartfrom its efficiency and implementation, the energy payback time of a photovoltaic moduledepends on its production cost. For example, the energy payback time for CIS modules ofSiemens Solar Industries (SSI), manufactured by selenization of metals, has been calculated tobe 9 to 12 years at a pilot production rate and about 2 years in full production. Empiricalcalculations show that during its lifetime (estimated to be 30 years), a CIS panel generates upto 14 times the energy required to produce it. 
The most common multistep method is the selenization of stacked metal or alloy layers. Themetals or alloys can be deposited by a variety of methods, the most common of which aresputtering [80, 93, 98-102], evaporation [79, 101, 103-114], and electrodeposition [98, 102, 108,113, 115-122].
Selenization is most often carried out under a selenium-containing atmosphere at hightemperatures, typically above 400 EC. Selenium may be present either as H2Se [80, 101, 103,108, 109, 114, 116, 119, 122], most often diluted by Ar, or elemental Se [79, 98-100, 102, 105-107, 109, 113, 115, 120]. Selenization time depends on thickness, structure, and composition ofthe film, as well as on the reaction temperature and selenium source. Generally, the formationof CIS by selenization is faster and occurs at lower temperatures than for CGS [79, 81]. As aresult, CIGS films may contain CIS and CGS as separate phases if the reaction temperature istoo low or the time is too short . High reaction temperatures also facilitate the formation ofMoSe2. [39, 99, 109]. The chalcogenization method offers also a possibility of formingCuIn(S,Se)2 thin films by introducing both Se and S precursors into an annealing atmosphere.
Influence of the chalcogenide source in selenization of evaporated Cu-In alloys at different
temperatures (between 250 and 600 EC) has been studied in detail in . Three selenizationmethods were compared: (i) H2Se/Ar at atmospheric pressure, (ii) solid Se source under Ar flowat atmospheric pressure, (iii) elemental Se vapor in vacuum. In all cases the samples were heatedfor 10 min to the reaction temperature, and the reaction time was 40 min. At temperatures below500 EC, the H2Se method was found to be most efficient, resulting in films with about 50 at.%Se already at 400 EC. The Se vapor approach was the most inefficient. Above 500 EC, a Secontent of about 46-52 % was achieved by all methods. Single-phase CuInSe2 films wereobtained only by the H2Se method at 400 EC. Additional phases, Cu and In selenides and/or Cu-In alloys, were detected in all other samples. The H2Se method also resulted in the bestcompositional uniformity and the largest grain sizes. The formation of MoSe2 was detected onlyafter selenization by H2Se at 600 EC.  Thus, H2Se is the most efficient selenization sourcebut its toxicity is a serious drawback. Recently, diethylselenide was introduced as an alternative,less toxic selenium source. Promising results were obtained from the selenization experimentswith Cu-In and Cu-In-O precursors .
Chalcogenization can also be done by depositing the chalcogen film on or between the metalliclayers, again either by evaporation [93, 104, 105, 114, 117, 123] or electrodeposition [111, 112,118, 121] and annealing the stack under an inert atmosphere [104, 112, 114, 117, 118], thusforming the desired compound and avoiding the use of toxic vapors such as Se and especiallyH2Se. Sometimes, however, a chalcogen-containing annealing atmosphere [105, 114, 121, 123]is required in order to compensate for the chalcogen loss at high temperatures. Alberts et al. observed significant Se losses upon annealing of stacked In/Se/Cu/In/Se layers above 200EC, irrespective of whether the annealing was performed in vacuum with elemental Se vapor orunder an Ar flow at atmospheric pressure in the absence of Se. No In loss was detected untilabove 650 EC. 
The metal precursors are most often deposited at or near room temperature, but highertemperatures have been used as well. In order to facilitate the interdiffusion of the metalprecursors and alloy formation between them, the metal precursors can be pre-annealed at alower temperature [79, 101, 103, 107, 112, 118] prior to selenization. Another approach is thedeposition of Cu/In/Cu/In/Cu/In... multilayers instead of a bilayer [99, 105, 106]. The multilayerapproach has been reported to result in smoother surfaces and better crystallinity .
The process of Showa Shell [124, 125] involves sputtering of stacked precursor layers (Cu-Gaalloy and In) followed by selenization with dilute H2Se and surface sulfurization with dilute H2Sat high temperatures. The thin (about 50 nm) Cu(In,Ga)(S,Se)2 surface layer is thought toimprove the surface quality and thus the fill factor via the passivation of shallow defects suchas selenium vacancies and SeCu antisites . Module efficiency of 12.5 % was achieved foran area of 859.5 cm2 . A remarkable feature is that the device was Cd-free, withZn(O,S,OH)x as the buffer layer [124, 125].
The process of Siemens AG , in turn, eliminates the use of toxic H2Se gas since theabsorber is prepared by depositing the constituent elements at room temperature, followed byrapid annealing under a sulfur-containing atmosphere at 550 EC or lower temperatures to yieldCu(In,Ga)(S,Se)2. CuGa and In layers were sputtered, and Se was evaporated thermally. Theamount of Se exceeded the stoichiometric one by about 40 % in order to compensate for the Seloss that occurs during annealing. [123, 126] Moreover, the process involves a controlled Naincorporation as a Na compound deposited on Mo before the absorber deposition.  Moduleefficiency of 14.7 % (average 13.2 %) for 18.9 cm2 aperture area was achieved by this process,as compared to 11.8 % (average 11 %) when the annealing was performed without sulfur .This increase in efficiency was due to an increase of band gap and open circuit voltage of theabsorber material . The depth distributions of sulfur and gallium were nonuniform – theiramounts were highest close to the Mo back contact where the absorber consisted of smallergrains than closer to the top surface. Thus, sulfur was thought to incorporate preferentially atgrain boundaries .
Surface sulfurization is used also for co-evaporated absorbers, for example in  the CIGSfilms were soaked in a solution containing InCl3 and thioacetamide (CH3CSNH2) to sulfurize thesurface. The thin CuInS2 layer on the absorber surface increases the stability and conversionefficiency of the cell since it improves the quality of the pn-junction by passivating the surface.
The incorporation of sulfur in CIS and CIGS thin films prepared by selenization of evaporatedmetal precursors  or by co-evaporation  has been studied. The sulfur distribution inthe chalcopyrite films was found to depend strongly on the composition and microstructure ofthe original film. The distribution was nearly uniform in copper-rich films, whereas in near-stoichiometric and indium-rich films most of the sulfur was on the surface. In indium-rich films,sulfur was found also close to the Mo/absorber interface. The Ga content of the film affected thedistribution as well: more S was found close to the Mo/absorber interface when the Ga/(Ga+In)ratio in the near-stoichiometric film was increased. In that study, the H2S annealing time waslong, 20 min, and the temperature was 575 EC . Surface sulfurization (10-50 min by H2Sat 350-550 EC) of co-evaporated CIS and CIGS films was reported to result in surfaceroughening, i.e., nonuniform and porous surface layers. The sulfurization of CIS films resultedin the formation of sulfoselenides below the CuInS2 surface layer, and improved cellperformance. In CIGS films, a phase separation to Cu(In,Ga)Se2 and Cu(In,Ga)S2 occurred, andthe resulting cell performance was poor .
The in-line process of Lockheed Martin Astronautics involves sequential sputtering of Cu, Ga,and In from elemental targets at room temperature, followed by selenization in a Se vapor athigher temperatures [130, 131]. Compound formation occurs via reactions of binary selenides.[130, 131] Homogeneous CIS  and CIGS  films with uniform compositions are formed
over 900 cm2 substrates. Small-area efficiencies of over 10 % have been achieved on soda limeglass by using optimized post-annealing conditions .
3.1.3. Evaporation from compound sources
Binary [133-135], ternary [81, 107, 136-140], and even quaternary  compounds can be usedas evaporation sources too. This approach is potentially simpler and easier to control than theco-evaporation from elemental sources, provided that the compound does not decompose duringheating, thus resulting in a film composition that differs from the source material. Very often atleast Se is lost, in which case a Se atmosphere is required during deposition and/or post-deposition annealing. Decomposition may be avoided by a very fast heating to sufficiently hightemperatures so that the material evaporates before it decomposes . This approach isutilized for example in flash evaporation [136-140] and related methods  as well as inpulsed laser deposition [141, 142].
Park et al.  evaporated InxSe (x~1) / Cu2Se double layers from In2Se3 and Cu2Se sources atroom temperature and annealed them in a Se atmosphere at 550 EC to yield crystalline single-phase Cu- and Se-rich CuInSe2 films. After annealing, small amounts of In2Se3 and Se weredeposited on the film surface at the same temperature in order to form a thin CuIn3Se5 layer. Asolar cell efficiency of 5.4 % was achieved with the Ag/n-ZnO/i-ZnO/CdS/CuIn3Se5/CuInSe2/Mostructure.  The efficiency increased to 9.6 % when the process was slightly modified: Sewas co-evaporated with In2Se3 during the initial stage at substrate temperature of 150 EC, andin the Cu2Se evaporation stage, the substrate temperature was increased to 440 EC which wasalso used for the subsequent Se annealing (10 min). The Cu-poor surface layer was formed againby evaporating small amounts of In2Se3 and Se. An efficiency of 9.3 % was achieved with noOVC layer but a slightly Cu-poor surface. 
The sequential ''quasi-flash evaporation'' of In2Se3 and Cu2Se onto unheated substrates and asubsequent anneal at 500 EC under Ar for 1 h resulted in single-phase chalcopyrite CIS filmswith random orientation and p-type conductivity. The evaporation of In2Se3-Cu2Se mixtures bythe same method led to the formation of (112) oriented single-phase CIS after annealing at 400EC. The control of the film composition in the latter method was difficult, however, becauseIn2Se3 melted earlier than Cu2Se, and the evaporating In2Se3 vapor caused some loss of theunmelted Cu2Se powder. That is why the films evaporated from mixture of In2Se3 and Cu2Sewere very Cu-deficient and thus n-type. 
Thermal evaporation of p-type CuInSe2 thin films from a single CIS source at substratetemperatures ranging from 200 to 600 EC was reported by Sadigov et al. . Because ofdifficulties in achieving stoichiometric, crystalline and binary phase free films with good surface
morphology, additional Cu and In were evaporated on the films at room temperature, and thefilms were subsequently selenized in a Se containing atmosphere. 
Klenk et al. prepared CIS, CGS and CIGS films from CIS and CGS powders and their mixturesat substrate temperatures between room temperature and 350 EC both by thermal  and flash evaporation. In both cases, the resulting films were Se-deficient unless the evaporation wasdone in the presence of additional Se vapor [81, 136]. The films were annealed in the presenceof Se vapor at high temperatures of up to 550 EC [81, 136]. Thermal evaporation resulted inuniform and dense films when the substrate temperature was between 200 and 300 EC; filmthickness (1.5 µm) and composition were nearly constant over an area of 10 cm x 10 cm. Filmformation was found to proceed via the formation of binary selenides – probably because therelatively slow heating rate of the precursor powders caused their decomposition. A significantdifference between the formation kinetics of CIS and CGS was observed: the formation ofsingle-phase CuGaSe2 required reaction temperatures above 500 EC, whereas single-phasechalcopyrite CuInSe2 was obtained already at temperatures as low as 350 EC, with no significantimprovement of crystallinity at higher temperatures. Moreover, single-phase CIGS was obtainedonly when the Ga content of the film was below 6 at.%.  Solar cell efficiencies above 10 %were achieved with CIGS absorbers , whereas the efficiencies with the ternary absorberswere lower, between 3-4 % for CGS [81, 136] and 6 % for CIS . Substrate temperature didnot affect the composition of flash evaporated films significantly .
Often, however, the compositions of flash evaporated films have been found to depend onsubstrate temperature. Merino et al.  studied the flash evaporation of CIS and CIGS fromtwo types of crucibles and at different substrate temperatures. About 10 wt.% of Se powder wasadded to the crucible with the compound source, in order to prevent the formation of Se-poorfilms. The deviations of the film stoichiometry from the source material were minimized bycarefully choosing the temperatures of crucible and substrate and keeping the deposition rate lowenough. Most films were n-type but became p-type after annealing in Se vapor. Solar cells withstandard CdS and ZnO were made by co-evaporating a thin CuIn2Se3.5 layer on the absorber. Thebest efficiencies were 5.1 % for CIS and 6 % for CIGS. 
Amorphous CIS films have been deposited by flash evaporation onto unheated substrates [138,139]. XRD peaks of CIS and Cu7In4 together with some unidentified peaks appeared when thesubstrate temperature was 200 EC or above. Also post-annealing at 350 EC resulted in theformation of CIS, Cu7In4 and In2Se3. The optimum conditions for the formation of CIS weredetermined to be substrate temperature 250 EC and post-annealing at 350 EC for 3-4 h.  Onthe other hand, Joseph and Menon  prepared crystalline p-type CIS films by flashevaporation from a single CIS source onto unheated substrates. Single-phase chalcopyrite filmswere obtained after annealing in vacuum at 50 EC for 1 h. 
In pulsed laser deposition (PLD), a rotating target that consists of the source material is heatedby a pulsed laser beam. Victor et al.  prepared (112) oriented CIS thin films by PLD at asubstrate temperature of 150 EC. The chalcopyrite phase was present already in the as-depositedfilms, and the crystallinity was further increased by annealing in Ar at 500 EC for 10 or 20 s.Kuranouchi et al.  deposited CIS films on unheated substrates and at a substratetemperature of 500 EC. The films were post-annealed at 500 EC in vacuum. The films depositedat room temperature exhibited (112) orientation after annealing. 
3.1.4. Chemical vapor deposition
Chemical gas phase deposition techniques such as metal organic chemical vapor deposition(MOCVD) [143-146] and close-spaced vapor transport [147, 148] have also been used for thepreparation of CIS and CIGS thin films. A possible advantage is lower deposition temperaturesthan in evaporation processes.
McAleese et al.  deposited CIS thin films at 400-450 EC by thermal MOCVD at lowpressures from methyl-n-hexyldiselenocarbamate complexes of Cu(II) and In(III)(Cu(Se2CNCH3C6H13)2 and In(Se2CNCH3C6H13)3). The resulting films were close tostoichiometric, and their band gaps were estimated to be about 1.08 eV. XRD patterns of thefilms showed the main reflections of the chalcopyrite phase.
A plasma-enhanced CVD process was also reported  where hexafluoroacetylacetonatecomplexes Cu(hfac)2 and In(hfac)3 were used as the metal precursors and 4-methyl-1,2,3-selenadiazole as the Se source. H2 was used as the carrier gas for the metal precursors.Deposition temperatures ranged from 150 to 400 EC. The resulting films were Se deficientprobably due to a Se loss during post-deposition cool-down in vacuum. 
Cu(hfac)2 complexed with trimethylamine N(CH3)3  or diethylamine NH(C2H5)2  havebeen used as the Cu precursors in atmospheric pressure MOCVD of CIS films. TrimethylindiumIn(CH3)3 and triethylindium In(C2H5)3 were used as the In precursors and H2Se as the Seprecursor. H2 was used as the carrier gas. The depositions were carried out at 400 EC, and theresulting films exhibited strong (112) orientation regardless of the metal ratio. [145, 146]. Solarcells fabricated from the CVD-grown films were not very efficient; the maximum open circuitvoltage was 0.26 V . For comparison, the open circuit voltages of high-efficiency devicesare generally above 0.6 V [5, 84-87].
3.1.5. Close-spaced vapor transport
CIS , CGS , and CIGS [147, 148] thin films have been deposited by close-spacedvapor transport using iodine as a transport agent [147, 148]. The reactor is a vertical vacuum tubethat contains the desired compound as a powder, a substrate, and solid iodine. The tube is heated,and the reaction starts when iodine vaporizes and reacts with the source powder to form gaseousmetal iodides and Se2. The gaseous species then react on the substrate surface, forming thedesired compound and liberating iodine. Advantages of the method include low cost and thepossibility to deposit films on large substrate areas. CuIn1-xGaxSe2 films with compositionsidentical to those of the source materials were obtained within the whole composition range (xfrom 0 to 1). Moreover, the films exhibited chalcopyrite structure, good surface morphology andp-type conductivity.  The morphology of the deposit was found to depend on the grain sizeof the source powder: large-grained source powder resulted in a bilayer structure where theinitial (lower) layer consisted of considerably smaller grains than the upper one. The formationof the small-grained initial layer could be prevented using smaller-grained source powder whichresulted in the formation of large-grained, smooth films. 
3.1.6. Low-temperature liquid phase methods
Non-vacuum deposition methods, including electrodeposition, electroless deposition, chemicalbath deposition as well as spray pyrolysis and ''particle-based methods'' etc., have also been usedfor the preparation of CIS-based absorber films. These methods are inherently low-cost, sincethe deposition temperatures are generally low and the equipments are simple. Absorbersprepared by these methods need often at least a post-deposition treatment at high temperaturesunder selenium-containing atmospheres to obtain high-efficiency devices.
Bhattacharya et al. have studied extensively the preparation of CIGS solar cells from precursorsprepared by electrodeposition , electroless deposition  and chemical bath deposition[151, 152]. A feature common to all their non-vacuum processes is that the film stoichiometryhas to be adjusted after deposition by adding In, Ga and Se by physical vapor deposition at hightemperatures. Although this may be considered as a drawback, these are nevertheless promisingmethods for the preparation of precursor films.
The electrodeposited precursors were deposited at room temperature from aqueous solutionscontaining CuCl2, InCl3, H2SeO3, GaCl3 and LiCl. The resulting films were very Cu-rich butresulted in solar cell efficiencies of 15.4 % after the stoichiometry correction . It must benoted that electrodeposition of CIS-based materials has been studied extensively, and the processdescribed here uses the electrodeposited film only as a precursor layer. The numerous otherelectrodeposition processes will be described in more detail in Chapter 4.
Electroless deposition is based on redox reactions without an external current source. Cu-richCu-In-Ga-Se films were prepared from aqueous solutions containing CuCl2, InCl3, H2SeO3,GaCl3 and LiCl, using a Fe electrode as the reductant. After stoichiometry correction, the filmswere used for the preparation of solar cells and a conversion efficiency of 13.4 % was achieved.
CIS [151, 153] and CIGS  thin films have been prepared by chemical bath deposition usingsodium selenosulfate (Na2SeSO3) as the selenium precursor. In , the films were depositedat 40 EC using Cu(NH3)4
2+, and In3+ complexed by citrate as the metal precursors. After post-annealing at 520 EC in air, VOC about 0.3 V was measured for a n-Si/p-CIS heterojunction .Bhattacharya  used triethanolamine complexes of Cu+ and In3+ as the metal precursors. Cu-rich CIGS precursor films were deposited from solutions containing Cu(NO3)2, In(SO3NH2)3,Ga(NO3)3, Na2SeSO3, triethanolamine, NH4OH and/or NaOH. After stoichiometry correction,the films were used as absorbers of solar cells that exhibited an efficiency of 7.3 % .
3.1.7. Spray pyrolysis
Single-phase chalcopyrite CIS and CIGS thin films with strong (112) orientation and p-typeconductivity have been prepared by spray pyrolysis from acidic aqueous  and aqueous-ethanolic  solutions of CuCl2, InCl3, GaCl3 and N,N-dimethylselenourea. The [Cu2+]/([In3+]+ [Ga3+]) concentration ratios in the solutions were kept at 1, but an excess of selenium precursorwas needed in order to compensate for the Se loss during deposition [154, 155]. Films depositedfrom aqueous solutions at 400 EC  were reported to be uniform and adherent to thesubstrate, with compositions close to those of the deposition solutions, whereas films depositedfrom aqueous-ethanolic solutions  at the same temperature were slightly (In+Ga)-rich, witha higher Ga/(In+Ga) ratio than in the deposition solution. At slightly lower substratetemperatures (360 EC) the films were either Cu- or (In,Ga)-rich, depending on the In/Ga ratioin the deposition solution, and their Ga/(In+Ga) ratios were closer to those in the depositionsolutions.  Despite these promising results, the solar cell efficiencies reached with spray-pyrolysed absorbers were low.
3.1.8. Particle deposition techniques
The ''particle deposition techniques'' involve the deposition of particulate precursor materialsonto substrates at low temperatures, and subsequent sintering under a chalcogen overpressure.The precursors are typically sub-micron powders of metals, alloys, oxides or chalcogenides, andthey are deposited as inks, suspensions, or pastes by simple techniques such as printing, casting,
spraying, doctor-blading, spin-coating or dip-coating. The porous precursor layer then convertsinto a dense, large-grained film at the high (400 EC or above) sintering temperature. Animportant advantage of these methods is that since the metal ratio is fixed already in theprecursor material, the stoichiometry of the final film is independent of thickness. Consequently,compositionally uniform films can be prepared over large areas and relatively large thicknessvariations can be tolerated. [156, 157] Cell efficiencies between 10 and 13 % [156-158],submodule efficiencies between 7 and 8 % (area 50-150 cm2)  and module efficiency of 5%  have been achieved by these techniques. An example of an ink-coating process waspresented in . Metallic powder containing Cu-In alloys was spread over a substrate as anink and selenized under 5 % H2Se/N2 at 440 EC for 30 min to form CIS. Solar cells preparedusing the ink-coated absorber exhibited efficiencies of 10-11 %. 
3.2. Buffer layer
As was seen in Fig. 3, most high-efficiency CIGS solar cells of today have a thin (50 nm or less)CdS buffer layer and an undoped ZnO layer between the absorber and the transparent conductingoxide. The roles of CdS and undoped ZnO are related to some extent . Although the opencircuit voltages of high-efficiency CIGS devices are mostly determined by the electronic qualityof the bulk absorber material [31, 32], the cell performances are nevertheless heavily influencedby the formation of the ZnO/CdS/CIGS heterojunction.  The role of the buffer layer istwofold: it both affects the electrical properties of the junction and protects it against chemicalreactions and mechanical damage. From the electronic point of view, the CdS layer optimizesthe band alignment of the device [41, 160] and builds a sufficiently wide depletion width thatminimizes tunneling and establishes a higher contact potential that allows higher open circuitvoltage values . The buffer layer plays also a very important role as a ''mechanical buffer''since it protects the junction electronically and mechanically against the damage that mayotherwise be induced by the oxide deposition (especially sputtering, see next chapter). Moreover,in large-area devices the electronic quality of the CIGS film is not necessarily the same over theentire area, and recombination may be enhanced at grain boundaries or by local shunts. Togetherwith the undoped ZnO layer, CdS enables self-limitation of electrical losses by preventingelectrical inhomogeneities (defective parts of the CIGS film) from dominating the open circuitvoltage of the entire device. 
The thickness as well as the deposition method of the CdS layer have a large impact on deviceproperties. During the early days, the device structure consisted of a CuInSe2/CdS junction witha thick (about 1-3 µm) CdS layer [161-163]. The CdS layers of these devices were most oftenprepared by evaporation at substrate temperatures between RT and about 200 EC, or in somecases by sputtering , and the CdS film was often doped either with In  or Ga . Insome cases, a CdS bilayer was used [119, 164], consisting of a thinner high-resistivity layer,
prepared either by evaporation  or chemical bath deposition [57, 119, 164] and a thickerlow-resistivity layer, doped with 2 % In  or Ga . Evaporated CdS has been used alsoin combination with the transparent conducting oxide layer [23, 165, 166].
Nowadays chemical bath deposition (CBD) is used almost exclusively [16, 24], and thereforethis thesis focuses mainly on the effects caused by CBD-CdS. CBD is a liquid phase depositionmethod that is based on a spontaneous precipitation reaction between the constituent ions. Thedeposition is most often done in an aqueous solution. Precipitation occurs if the concentrationsof the ions in solution are high enough so that their ionic product exceeds the solubility product(Ks) of the compound to be deposited . The solubility product of CdS is about 10-28 ,and thus its formation in a 1 mM Cd2+ solution starts when free the sulfide ion concentrationexceeds 10-28 M2 / 10-3 M = 10-25 M.
Commonly used Cd-precursors include simple compounds as CdSO4 [86, 160], CdI2 [45, 168],Cd(CH3COO)2 [59, 159], and CdCl2 . In order to slow down the reaction and to avoid theformation of Cd(OH)2, the metal ion is usually heavily complexed by a ligand , most oftenNH3 [45, 59, 86, 159, 160, 168, 169].
The most common sulfur precursor is thiourea NH2CSNH2 [45, 59, 86, 159, 160, 168, 169], theamount of which in the deposition solution is usually much higher than that of the metalprecursor. The deposition is usually performed at an elevated temperature, and the solution isoften stirred during the deposition. After immersing the substrates in the deposition solution atroom temperature, the bath is heated to the desired temperature that is usually between 55 and90 EC [45, 86, 160, 168, 169]. Deposition temperature influences strongly the film morphologyand impurity content . The formation of CdS occurs according to the following net reaction:
[Cd(NH3)4]2+ + NH2CSNH2 + 2 OH– 6 CdS + 4 NH3 + CH2N2 + 2 H2O 
Intermediate steps of the reaction involve the release of Cd2+ ions from the ammonia complexand the decomposition of thiourea by OH- ions which releases S2- ions. The mechanisms of CBDreactions have been studied extensively, and will not be discussed here.
In contrast to evaporated films , CBD films contain high amounts of oxygen-relatedimpurities that originate from the deposition solution; the amount of oxygen in the films can beas high as 10-15 at.% [45, 170]. Most of the oxygen is present as OH- and H2O. [45, 170] Thus,the composition of CBD-CdS films is more accurately stated as Cd(S,O,OH) . Additionalimpurities such as C and N containing compounds result from side reactions of the chalcogenprecursor . The amount and identity of the impurities, and consequently the performanceof the solar cell depend strongly on the CdS deposition conditions [160, 168, 171, 172]. Forinstance in , the conversion efficiency increased from 17.6 % to 18.5 % when the CBD-CdS
process was improved.
In addition to the CdS film deposition, the chemical bath modifies the absorber surface. The bathhas been suggested to re-establish positively charged surface states and the surface typeinversion by removal of OSe acceptors and creation of CdCu donors at the surface region [16, 77].Thus the interface between CIGS and CBD-CdS is not abrupt but the layers are intermixed tosome extent [44, 45]. Both Cu-and Cd-diffusion play a role, and the intermixing is furtherenhanced during the post-deposition air-annealing . According to Nakada and Kunioka, Cu is substituted by Cd at the surface region of CIGS (depth about 10 nm). The diffusiondepth of Cd atoms may be related to the thickness of the Cu-deficient surface layer (CuIn3Se5)of CIGS . On the other hand, Heske et al.  have observed diffusion of Se and In fromCIGS into CdS and the diffusion of S from CdS into CIGS. The extent of interdiffusion dependson the structure of the absorber: (220/204) oriented CIGS films have been found to allow moreCd atoms to diffuse into the CIGS film .
One advantage of CBD as compared to evaporation is that a complete, conformal coverage ofthe CIGS surface can be obtained at very low thicknesses: already 10 nm has been reported tobe sufficient . The coverage depends on deposition conditions, particularly on themetal/chalcogen precursor ratio, being better with higher metal/chalcogen precursor ratios .
Absorption of light in the CdS layer, the band gap of which is 2.4 eV , decreases the shortcircuit current density. The absorption of light in the ZnO, in turn, is a less severe problem sinceits band gap is higher, 3.2 eV . Thus the reduced absorption in the thinner CdS layer resultsin a better device performance [57, 58]. The CdS layer must, however, be thick enough in orderto obtain high open circuit voltage and fill factor.  If the CdS layer is too thin or does notexist at all, recombination in the space-charge region of CIGS increases, causing losses in VOC,FF and spectral response . Although the collection at short wavelengths (<550 nm) isenhanced in buffer-free devices, the collection at the longer wavelengths is poor , andconsequently the conversion efficiencies are lower than those of standard devices. For instance,a conversion efficiency of 15 % was achieved without CdS, while the world record efficiencyof 18.8 % with CdS was announced in the same publication . Thus the optimum thickness ofthe CdS layer is a result of a compromise between increase in VOC and FF, and loss in jSC .
Performances of buffer-free devices have been found to improve upon dipping the absorbers insolutions containing only CdSO4 and ammonia but no thiourea at 60-80 EC before the depositionof the transparent conductor [160, 175, 176]. Further improvement of cell performances wereobserved upon applying a cathodic potential during the dip: Lincot et al.  achievedefficiencies of 11.3 % and 9.4 % with and without an applied potential during the dip,respectively. For comparison, an efficiency of 14.9 % was measured for a device with thestandard CdS and 5.9 % for a buffer-free device without the CdSO4-ammonia treatment .
These results support the idea of Cd incorporation and doping of CIGS . According toContreras et al. , their buffer-free device may, instead of being a buried junction, actually bea true heterojunction device. CdSO4-ammonia treatments in combination with a very thin CdSfilm provided enhanced spectral response in the blue part of the spectrum (short wavelengths) as compared to the world record device. Since the jSC values of the modified devices wereslightly higher and the VOC and FF similar to the high-efficiency devices with standard CdS, thisapproach may result in improved cell performances .
In order to decrease the optical absorption losses and to enhance the response in the short-wavelength region, alternative, more transparent buffer materials have been looked for. Forinstance, part of the Cd can be replaced by Zn to form (Cd,Zn)S, the band gap of which is higher[82, 174, 177]. Devaney et al  deposited conformal, uniform (Cd,Zn)S buffer layers by CBDfrom ZnCl2, CdCl2, NH4Cl, NH4OH and thiourea at 85 EC. The Zn content was varied, and theZn / (Zn+Cd) ratio in the best films was 15-20 %, resulting in a conversion efficiency of 12.5% with absorbers prepared by co-evaporation . Başol et al. , in turn, prepared (Cd,Zn)Sbuffers with about 10 % Zn by CBD from Zn-acetate, Cd-acetate, triethanolamine, NH4OH andthiourea at 55 EC, and achieved conversion efficiencies between 10 and 13 % with absorberfilms prepared by particle deposition and subsequent selenization [156, 158].
Due to the environmental concerns associated with Cd-containing materials, serious efforts havebeen directed towards completely Cd-free buffer materials. The materials studied include Zn-and In-based materials such as sulfides, selenides, hydroxysulfides and -selenides that can beprepared by CBD [87, 125, 178-180], ion layer gas reaction (ILGAR) , MOCVD ,atomic layer deposition (ALD) [183, 184], evaporation [26, 185-189] and sputtering .Analogously to the Cd-pretreatments described above, Zn- and In-pretreatments have led toimproved device performances as well, either with or without an additional buffer layer [150,175, 181, 183, 190].
The conversion efficiencies of Cd-free devices are approaching those of the standard devices.Recently, a conversion efficiency of 18.1 %, close to those of the best CdS containing devices,was achieved using a CBD-ZnS buffer layer in combination with a CIGS absorber prepared bythree-stage co-evaporation in a MBE system . ZnS layer was deposited by CBD from ZnSO4,NH3 and thiourea at 80EC . It contained a significant amount of Zn(OH)2 and ZnO phasesand C and S impurities . The band gap of the layer was, however, close to that of ZnS, 3.8eV. When the structure was annealed in air at 200EC for 10 min , the O-related impuritiesstudied by XPS were not affected but the cell performance improved markedly . Theimprovement was probably due to diffusion of Zn into CIGS and the formation of a buried pn-homojunction on the absorber surface. This intermixing explains why the conversion efficiencyis surprisingly high in spite of the large conduction band offset between CIGS and ZnS [87, 126,191].
The diffusion of evaporated Zn into CIGS has also been observed . Junction electron beam-induced current measurements revealed that the pn-junction of the Zn-diffused device is locatedin CIGS, in contrast to the devices with CdS and ZnO buffers where it is at the interface. TheZn-diffused buffer-free junction resulted in a conversion efficiency of 11.5 %. 
One of the Cd-free approaches of NREL  involved a Zn-diffused homojunction as well. Theabsorber was dipped in a ZnCl2 solution and annealed at 200EC in air. Then the ZnCl2 residuewas removed from the absorber surface by washing in water and etching in concentrated HCl,followed by deposition of the ZnO bilayer by sputtering. The conversion efficiency of this devicewas 14.2 %. 
The CBD-ZnS was found to be sensitive to oxygen-induced damage during sputter depositionof undoped ZnO, and thus the device was prepared without the undoped ZnO layer . Theoptimum thickness of the ZnS layer was 130 nm, indicating the need for reduction of shunt pathsbetween CIGS and ZnO:Al . As expected on basis of the higher band gap of the buffer, thecell exhibited higher quantum efficiency at short wavelengths than a CdS-containing cell [87,191]. This resulted in a higher jSC but the VOC was lower, resulting in a similar conversionefficiency as the standard cell with CdS .
Showa Shell [124, 125] likewise uses a ZnS-based CBD-buffer for their absorbers prepared byselenization of sputtered metal layers. A Zn(OH,S)x film is deposited from a solution containingZn-sulfate or acetate, NH3, and thiourea at a temperature above 80 EC, followed by annealingof the CIGS/buffer structure at 200 EC for 15 min, resulting in a buffer layer with a compositionof Zn(O,S,OH)x (oxyhydroxysulfide).  The efficiency of 12.5 % for a 30 cm x 30 cmmodule  demonstrates the suitability of this buffer deposition process to large substrateareas.
Kushiya et al.  studied also CBD-Zn(O,OH)x as buffer layers. The films were prepared bydepositing Zn(OH)2 at 60-80 EC from similar solutions as Zn(OH,S)x but without thiourea, andannealed to yield Zn(O,OH)x. The improved performance after annealing was attributed toconversion of hydroxide to oxide , and not to Zn diffusion as was done by Nakada andMizutani . The Zn(O,S,OH)x buffer of Kushiya et al.  suffered from sputter-induceddamage during the ZnO deposition too, indicating the need for optimization of buffer thickness(currently 50 nm) and the ZnO deposition method. Again, gain at shorter wavelengths and lossat longer wavelengths was observed as compared to CdS.  Light soaking, especially incombination with annealing, caused a remarkable improvement of the cell performance which was attributed to the release of H2O molecules from the hydroxide during light soaking.
Ennaoui et al.  deposited Zn(S,OH) and Zn(Se,OH) buffer layers on CIGSS absorbers of
Siemens by CBD at 50 and 70 EC, respectively. The deposition solutions contained ZnSO4,hydrazine hydrate, NH3 and thiourea or selenourea. The buffer deposition process was somewhatdifferent from those mentioned above since it involved a Zn pretreatment: the absorbers werefirst dipped for a few minutes into the heated solution that contained the metal precursor and theligands, and the chalcogenide precursor solution was added only thereafter. The growthmechanism was self-limiting, allowing the deposition of very thin buffer layers withhomogeneous surface coverages.  This approach led to total area efficiencies of 14.2 %both for Zn(S,OH) and for Zn(Se,OH) buffer layers.  Minimodule efficiencies (aperturearea 20 cm2) achieved by Zn(Se,OH) were between 10.7 and 11.7 %, comparable to thoseachieved by the standard CdS buffer (11.7-12.7 %) .
Indium-based materials have resulted in high conversion efficiencies too. Hariskos et al. ,for instance, deposited Inx(OH,S)y films on co-evaporated CIGS absorbers by CBD from InCl3
and CH3CSNH2 (thioacetamide) at 70 EC. Post-anneal at 200 EC and light soaking resulted inan active area efficiency of 15.7 %. Compared to the standard CdS buffer, the Inx(OH,S)y bufferresulted in improved VOC, comparable FF and slightly reduced jsc values. Again, gain in short-wavelength region and loss in long-wavelength region was observed. The former was due to theimproved transparency of the buffer layer, and the latter due to the modification of the electricalproperties of the absorber such as a reduced space-charge width .
Despite its above mentioned benefits, the CBD method has two disadvantages: first, thematerials yield is low which causes large volumes of Cd-containing waste. This problem can bepartially solved by recycling the deposition solution: the CdS-containing colloidal material isfiltered off after deposition, the concentrations of NH3 and thiourea are adjusted again to theinitial level, and Cd-precursor is added. The properties of the CdS layers deposited from therecycled solution do not differ significantly from those deposited from fresh solutions.  Thesecond problem is the difficulty of combining the CBD step as a part of an in-line vacuumprocess: if both the absorber and the ZnO bilayers are prepared by PVD methods in vacuum, theCBD step causes an undesirable interruption of the vacuum process.
Recently, a new deposition method called ion layer gas reaction (ILGAR) was developed for thedeposition of buffer layers. It is a cyclic method that consists of application of a metal precursoron a substrate by dipping or spraying, drying the substrate, and the reaction of the metalprecursor layer with gaseous hydrogen chalcogenide or water to form the corresponding metalchalcogenide or oxide. Thus, an evident advantage of ILGAR is that it produces less waste thanCBD does. The resulting films are conformal, and the film thickness is easily controlled by thenumber of deposition cycles. [176, 181] The application of a ILGAR-ZnS buffer to Siemensabsorbers resulted in total area conversion efficiency of 14.2 % when a Zn-pretreatment in aZnCl2-NH3 solution was performed before the deposition of the ILGAR-ZnS .
To avoid the second problem of CBD, i.e., its incompatibility with PVD processes, ''dry'',potentially more easily integrated, gas phase methods for buffer deposition have been studied.Siebentritt et al. , for instance, deposited ZnSe buffer layers on Siemens CIGSS absorbersby photoassisted MOCVD using ditertiarybutylselenide as the selenium source and dimethylzincor its adduct with triethylamine as the zinc sources. Hydrogen was used as the carrier gas, andUV illumination was used in order to enhance the decomposition of the Zn-precursor at lowdeposition temperatures. The highest total area efficiency, 11 %, was achieved with a 10 nmthick buffer layer deposited at 280 EC. This efficiency is the highest ever achieved with aMOCVD buffer. 
Lincot et al. [183, 184] deposited Zn(O,S), In2Se3 and Al2O3 buffer layers by ALD. Diethylzinc,indium acetylacetonate, and trimethylaluminum were used as the metal precursors, water as theoxygen precursor and H2S as the sulfur precursor. Efficiencies of 10.4 % for ZnO0.85S0.15, 13.5% for In2Se3, and 9 % for Al2O3 were achieved.
Konagai et al. used co-evaporation to prepare ZnSe  and ZnInxSey  buffer layers. Thebest conversion efficiencies achieved by these buffers were 9.1 %  and 15.1 % ,respectively, whereas the standard CdS resulted in 15.9 % . ZnSe buffers prepared bypulsed MBE resulted in conversion efficiency of 11.6 % after light soaking . In2Se3 (orInxSey) buffer layers prepared by co-evaporation, have resulted in conversion efficiencies of 8.5% on CIS  and 13 % on CIGS , whereas (In,Ga)ySe buffer layers prepared by the samemethod led to a conversion efficiency of almost 11 %. 
Delahoy et al.  prepared ZnIn2Se4 (ZIS) and ZnGaxSey (ZGS) by evaporation of bulkmaterial. The best efficiency achieved by ZIS was 11.6 %, and no light soaking effect wasobserved. For comparison, the standard CdS buffer resulted in efficiency of 16.3 %, whereas10.3 % was measured for a buffer-free device. 
3.3. Oxide layer
The requirements for the electrical top contact of a CIGS device are: sufficient transparency inorder to let enough light through to the underlying parts of the device, i.e., its band gap must behigh enough, and sufficient conductivity to be able to transport the photogenerated current to thecircuit without too much resistance losses. Nowadays, transparent conducting metal oxides(TCO) are used almost exclusively as the top contacts. Narrow lined metal grids (Ni-Al) areusually deposited on top of the TCO in order to reduce the series resistance. The quality of thefront contact is thus a function of the thickness, sheet resistance, absorption and reflection of theTCO as well as the spacing of the metal grids .
Referring to Fig. 3, most devices utilize nowadays an oxide bilayer that consists usually of a thin(50-100 nm) high-resistivity layer, and a thicker (100-1500 nm) low-resistivity layer. The high-resistivity layer is most often undoped ZnO. Its benefit to the device performance is the increaseof the VOC of the device by 20-40 mV . Its role is not completely understood yet, however.As was discussed in Chapter 3.2., the resistive oxide layer provides together with the buffer alocal series resistance that protects the device from electrical losses that may result fromelectronic inhomogeneities of the absorber.  Admittance spectroscopy and capacitance-voltage measurements  indicated that the presence of this resistive layer affects theelectronic properties of the heterojunction only to the extent that is expected on the basis of banddiagrams. The conducting part of the oxide bilayer is most often ZnO doped with either Al [5,36, 57, 59, 81, 85, 95, 126, 157, 182], B [85, 86, 123, 177, 190, 194], or Ga [125, 179, 195]. Alsotin doped In2O3 (In2O3:Sn, ITO) [26, 84, 94] is used commonly.
The oxide bilayer is most often deposited by sputtering [5, 26, 36, 57, 59, 81, 84, 85, 95, 97, 125,126, 157, 179, 182, 195] with no intentional heating of the substrate [36, 57, 85, 195]. Theresistive layer is sputtered in Ar/O2 (about 0.1-2 %) ambient [34, 36, 57, 82]. Besides sputteringintrinsic ZnO, the resistive layer may also be made from a doped target (ZnO:2 wt.% Al2O3) [34,57, 82], provided that the sputtering ambient contains enough oxygen. Oxygen is needed toprevent the formation of oxygen vacancies that might render even the undoped ZnO tooconductive.
The conductive layer (most often ZnO:Al) is usually deposited from a ZnO:2 wt.% Al2O3 targetin a pure Ar ambient. [36, 57, 82, 85] In some cases the sputtering ambient may contain a smallamount of O2 . The ZnO:Ga layers of HMI  and Showa  are sputtered in Ar fromZnO:Ga2O3 targets with Ga2O3 contents of 3.4 wt.%  or 5.7 wt.% . Doping of theoxide layer can be accomplished also by reactive sputtering as was done for instance byHagiwara et al.  who sputtered their ZnO:B electrodes from an undoped ZnO target in B2H6-Ar mixture.
Although sputtering is a fast and well-known deposition method for oxide thin films, itsdisadvantage is that it may damage the underlying layers [87, 178]. Damage occurs especiallyduring the deposition of the resistive layer that is done in an Ar/O2 ambient. Nakada et al. ,for instance, had to leave the resistive ZnO layer out and deposit a thicker ZnS buffer instead.
In order to reduce the damage caused by oxide deposition, softer, less damaging depositionmethods have been studied. The most important of these are MOCVD [98, 123, 177, 190, 194,196] and ALD [175, 183, 184, 197] since they can be used for the deposition of the wholebilayer. In some cases only the resistive part of the oxide bilayer is deposited by a softer method,for instance MOCVD , ALD , ILGAR , CBD  or electrodeposition and the conductive part by sputtering.
The less damaging oxide deposition methods are especially useful for the preparation of buffer-free devices where the protecting interlayer is absent. These buffer-free approaches have shownpromising results: a conversion efficiency of 12.7 % was measured for a device where theresistive ZnO layer was prepared by MOCVD and the conductive layer by sputtering . Forcomparison, a device with MOCVD-ZnO bilayer showed efficiency of 11.5 % . ALD-ZnObilayers have resulted in even higher efficiencies, up to 14.9 % with Cd pretreatment . Thecombination of the two methods has also proven to be successful: a conversion efficiency of 12.1% was measured for a device with ALD-grown resistive ZnO layer and MOCVD-grownconductive layer .
Bär et al.  measured a total area efficiency of 14.6 % for a device where part of the ZnOlayer was deposited by ILGAR and the rest was sputtered. Cell preparation involvedpretreatment in an aqueous CdSO4-NH3 solution. The success of the ILGAR method wasdemonstrated by the somewhat higher efficiency than for the standard device, 14.1 %.  Galet al.  measured a conversion efficiency of 11.4 % for a device with electrodepositedresistive ZnO layer and sputtered conductive ZnO layer. For comparison, the efficiency of astandard device with CdS and sputtered ZnO bilayer was 13.3 % .
4. Cathodic one-step electrodeposition of CuInSe2 and Cu(In,Ga)Se2 thinfilms
Electrochemical techniques for the preparation of CIS-based films include one-step deposition,sequential deposition of binary compounds, and deposition of elemental layers followed byannealing either under an inert or a reactive atmosphere. The sequential electrodepositiontechniques were discussed in Chapter 3.1. This chapter focuses on one-step electrodeposition ofCuInSe2 and Cu(In,Ga)Se2 thin films.
Electrodeposition is a liquid phase thin film deposition method that is based on electrochemicalreactions (reductions or oxidations) carried out using an external power supply. In addition tothe power supply, at least two electrodes are needed, between which the current flows in thedeposition solution. One of the electrodes is a working electrode, or substrate on which the filmgrows, and the other one is a counter electrode. The film growth occurs most often via reductionreactions, i.e., the working electrode is a cathode. Usually a three-electrode setup is used wherethe third electrode is a reference electrode with respect to which the electrochemical potentialof the working electrode is controlled or measured. If the potential of the working electrode iscontrolled, the resulting current may be measured, and vice versa. Deposition is often carried outat a constant potential (potentiostatically) or at a constant current (galvanostatically), but voltageand current waveforms or pulses can be used too.
In cathodic one-step electrodeposition of compound semiconductor thin films, simultaneousreduction of all the constituent ions at the same potential in suitable proportions is necessary inorder to achieve the desired film composition. This can be achieved by two ways: balancing thediffusion fluxes of the constituent ions to the cathode, or employing the induced co-depositionmechanism. The balancing of fluxes can be done by careful optimization of the depositionconditions, that is, adjusting the concentrations in the solution as well as the deposition potential.If the reduction potentials are far apart, they can be shifted closer to each other by complexingthe more noble ions with a ligand that forms strong complexes with them and thereby shifts theirreduction potentials towards more negative (less noble) values. The disadvantage of the fluxbalance approach is that the concentration and potential ranges for the formation ofstoichiometric product are often narrow, and thus small, unavoidable variations in concentrationsand potential may result in large changes in the film compositions. This deteriorates thereproducibility and may render upscaling to larger substrate areas problematic.
When induced co-deposition mechanism is exploited, the film composition is determined bythermodynamics [6, 7]. Using the most well-known system, CdTe, as an example, the morenoble ion (HTeO2
+ in the case of CdTe) that reduces at a less negative potential, deposits firston the electrode surface (Eq. 4) and induces the reduction of the less noble ion (Cd2+) and theformation of CdTe (Eq. 5) at less negative potentials than where the reduction of Cd2+ to metallic
Cd (Eq. 6) would take place.
HTeO2+(aq) + 3H+(aq) + 4 e- º Te(s) + 2H2O 
Te(s) + Cd2+(aq) + 2 e- º CdTe(s) 
Cd2+(aq) + 2 e- º Cd(s) 
The reason for the underpotential reduction of the less noble ion (Cd2+) is the energy released inthe compound formation. When the concentrations in the deposition solution are chosen so thatthe solution contains a large, 10-100 fold, excess of the less noble ion (Cd2+), the reaction (4) isalmost exclusively followed by the reaction (5) rather than by the reaction (4) itself. When thepotential is adjusted less negative than that required for the reaction (6), the deposition ofstoichiometric CdTe is ensured over a range of electrolyte compositions and electrode potentials.This kind of induced co-deposition process, employed most widely for CdTe but also for manyother binary compound semiconductors [200-202] is much less sensitive to the unavoidablevariations in the electrolyte compositions than processes which rely on balancing the diffusionfluxes. In addition, small potential drops across large substrates will have minimal effects. [6,7]
Electrodeposition of CIS-based thin films has been studied a lot by several groups since 1983.The majority of the existing electrodeposition processes for CIS thin films are based on the fluxbalance approach. Although the reaction mechanisms in the Cu-In-Se system have been studiedthoroughly [203-209], and the underpotential assimilation of In into the films has been frequentlynoticed and mentioned in the literature, the induced co-deposition approach had not been utilizedin the preparation of CIS thin films prior to [I]. This is illustrated by the fact that one-stepelectrodeposition of CIS has usually been carried out from solutions where the Cu and Seprecursor concentrations are of the same order of magnitude, and only In precursor is present inexcess. Under such conditions, film stoichiometry is determined by the deposition potential andthe ratio of diffusion fluxes of Se and Cu to the substrate surface. Electrodeposition processesbased on balancing the diffusion fluxes will be described in this chapter, and the only processthat utilizes induced co-deposition will be described in Chapter 7.
One reason for the lack of electrodeposition processes utilizing the induced co-deposition is thatthe electrodeposition of CIS occurs via the formation of copper selenide which does not followthe induced co-deposition mechanism [203, 204]. The complicated behavior of the Cu-Se systemmay be attributed to the following facts. First, the reduction of Se4+ to Se requires a largeoverpotential, i.e. its actual reduction potential is much more negative than the correspondingstandard reduction potential (EE = +0.556 V vs. Ag/AgCl ), and this potential is alsodependent on the electrode surface. Second, the standard reduction potentials of Cu+ and Cu2+
(EE = +0.298 V and +0.115 V vs. Ag/AgCl , respectively) are close to the observedreduction potential of Se4+ and, depending on the required Se overpotential, may be either morepositive or more negative than that of the Se4+ ions. As a consequence, independent co-depositionrather than induced co-deposition is observed in the Cu-Se system [203, 204]. Furthercomplications may arise from the passivating nature of Se deposited at room temperature .These issues can, however, be overcome [I] as will be described in Chapter 7.
One-step electrodeposition of CIS is usually carried out from an aqueous acidic solutioncontaining simple compounds of Cu2+ or Cu+ and In3+, most often sulfates [104, 203, 206-208,211-218] or chlorides [149, 150, 161, 163, 166, 209, 211, 216, 217, 219-224]. Because of thelimited solubility of Cu+ compounds and the instability of the free Cu+ ions in aqueous solutions,Cu2+ compounds are used considerably more frequently than Cu+ compounds. The most popularSe precursor is SeO2 which dissolves into mildly acidic solutions in the form of HSeO3
- ,but Na-selenosulfate  has been used too. Acidic solutions are used because the reductionof HSeO3
- is facilitated in acidic solutions .
The deposition solution contains often a complexing agent in order to shift the reductionpotentials of Cu and In closer together and/or to improve the film quality. The most popularcomplexing agent is citric acid [161, 203, 206-209, 212, 213, 215, 225] that acts also as a pHbuffer, but other ligands such as ammonia [151, 161], triethanolamine , ethylenediamine, ethylenediaminetetraacetic acid (EDTA) , and thiocyanate [211, 216, I-IV] can beused too. Sometimes a supporting electrolyte such as sulfate (K2SO4) [203, 206, 218] or chloride(LiCl [149, 150] or NaCl ) is added.
Electrodeposited CIS and CIGS films are usually amorphous or poorly crystalline and consistof small grains. They tend to be Cu-rich and contain frequently degenerate Cu2-xSe phases thatare detrimental to the device performance. Cu-rich films have generally larger grain sizes thanstoichiometric or In-rich films. The films may also contain impurities that originate from theaqueous deposition solution or from the complexing agents. For the above reasons, the filmsrequire at least annealing under an inert atmosphere prior to completing the device preparation.Very often the film stoichiometry needs to be corrected too, for instance by annealing under aSe-containing atmosphere and/or by selective etching in cyanide-containing solutions.
Bhattacharya  was the first one to electrodeposit CuInSe2 thin films. The depositionsolution contained 0.018 M In3+, 0.018 M Cu+ and 0.025 M SeO2 as well as 0.006 vol.%triethanolamine and 0.007 vol.% NH3 at pH of about 1. The films were deposited on SnO2:Fcoated glass substrates at -0.7 V vs. SCE at room temperature, and the solution was stirredduring the deposition. Film compositions were not analyzed, but X-ray diffractograms of thepost-annealed films (1 h at 600 EC under Ar) showed many of the reflections of the chalcopyritephase. 
Vedel et al. [203-205] have studied systematically the reaction mechanisms involved in theelectrodeposition of CuInSe2 thin films. The film formation reactions were studied on SnO2
electrodes, both by cyclic voltammetry and deposition experiments. Similar results wereobtained in sulfate and citrate solutions . Since the deposition of CIS proceeds via theformation of copper selenide, the binary Cu-Se system was studied first . The reductionpotential of Se4+ was found to shift to the positive direction in the presence of Cu2+ in thesolution. In fact, the deposition of Se in reasonable quantities was observed only in the presenceof Cu2+ in which case the formation of copper selenide enables the deposition of Se. Thus the Cu-Se system does not follow the induced co-deposition mechanism in the same way as the Cd-Tesystem does [6, 7].
In contrast, the behavior of the Cu-Se system in the presence of In3+ is analogous to that of Tein the presence of Cd2+, that is, copper selenide induces the formation of CIS. In the presence ofan excess of In3+ in the solution, the film composition is controlled by the Se4+/Cu2+ flux ratio (α)arriving at the electrode.  At low values of α, two co-deposition processes were observed,and the resulting films consisted of either CIS + Cu2Se or CIS + Cu. If the Se4+ flux is in excess(at high α), the two processes merge and only CIS + In2Se3 are obtained.  When In3+
concentration is not high enough, the electrodeposition process is limited by diffusion of all thethree ions. Consequently, the film composition is determined by both flux ratios α and β, whereβ is the In3+/Cu2+ flux ratio. 
Pottier and Maurin  studied the electrodeposition of Cu-In, Cu-Se and CIS thin films on Tiand Ni rotating disc electrodes from acidic sulphate and citrate solutions containing 5-10 mMCuSO4, 10-20 mM In2(SO4)3, 10-20 mM SeO2, 60-80 mM K2SO4, and 0-80 mM Na-citrate. Thepresence of citrate was found to decrease the plateau current of copper by modifying thediffusion coefficient of Cu2+ ions and slowing down its reduction rate. Small amounts of citratein the deposition solution resulted in the formation of smooth films, whereas large amountscaused powdery deposits. The formation of smooth layers of crystalline compounds (Cu9In4,Cu2Se or CIS) was correlated with a plateau on the polarization curves. The current in the plateauregion was found to be limited both by mass transport via convective diffusion and by a slowsurface process. The slow surface process was thought to suppress non-compact morphologiesand allow crystallization of a material with the desired composition. Films deposited outside thepotential range corresponding to the plateau had poor crystallinity, morphology, andcomposition. Thus the main function of the complexing agent was to promote the formation ofwell-defined crystallized compounds. 
Molin et al. [207, 208] studied the reactions in the citrate system on Ti electrodes. The depositionsolution consisted of 3 mM CuSO4, 6 mM In2(SO4)3, 5 mM SeO2, and 0.4 M citric acid at pH 1.7.By shifting the deposition potential to the negative direction, it was possible to obtain CuSe,
Cu3Se2, CuInSe2, and In-enriched CuInSe2 from the same deposition solution [207, 208]. Theformation of CIS was proposed to occur by the reaction of In3+ with Cu3Se2 . The potentialrange of CIS formation widened when the solution was stirred during the deposition. Moreover,the deposition rate as well as the current efficiency were found to increase but the filmmorphology did not change. The potential ranges for the formation of the various compoundsdepend on the total conductivity of the solution, cathode surface area (ohmic drops) andelectrolyte temperature . Therefore the addition of Na2SO4 as a supporting electrolyte wasfound to narrow the potential range of CIS formation due to increase of the solution conductivity. The kinetic study  revealed that in the citrate system, the rate of electrodepositionis determined by ion mass transfer and a chemical reaction at all potentials. The chemicalreaction determining the rate of electrodeposition was proposed to be the reduction of SeO3
2- bymetallic Cu , analogously to the mechanism proposed by Massaccesi et al. . Theaddition of Se4+ to Cu2+ solution was also found to shift the reduction potential of Cu2+ to morepositive values and increase the limiting current  which is in agreement with . Similarbehavior was observed also in solutions where thiocyanate ions were used as the complexingagents .
Oliveira et al.  studied the formation of CIS on Mo and on itself by cyclic voltammetry andgrowth experiments. Their electrolyte contained 0.4 M citric acid, 3 mM Cu(NO3)2, 3 mM InCl3,and 5 mM SeO2 at pH 2.0. In agreement with the other authors [203, 208], the formation ofCuxSe and its reaction with In3+ in the solution was observed which leads to assimilation of Ininto the film. In contrast to most of the other studies on CIS electrodeposition from citratesolutions, however, they observed the reduction of Se4+ at a more positive potential than that ofCu2+ and suggested therefore the formation of copper selenide via induced co-deposition,analogously to [I].  When the cyclic voltammograms were measured on a previouslydeposited CIS film, the currents corresponding to the reductions of Cu2+ and In3+ began to flowearlier and were stronger than on a Mo film. This suggests a surface-induced depositionmechanism. The current corresponding to the reduction of Se4+ to Se on CIS, in contrast, wassmaller than on Mo which was attributed to the formation of an insulating film.  Parallelto Vedel et al. , similar results were obtained in sulfate and citrate solutions . On theother hand, other authors  have observed cathodic shifts in the reduction potentials of bothCu2+ and HSeO2
+ on Ti substrates upon addition of citrate ions, whereas the reduction potentialof In3+ was unaffected. These differing results are an indication of the effect of the substrate onthe electrochemical reactions.
Herrero et al.  deposited CIS films on Mo substrates from solutions containing 3 mMCuSO4, 3 mM In2(SO4)3 and 5 mM SeO2 at pH 1.7 with 0.4 M citric acid as the complexingagent. CuxSe was found to be present also in the In-rich samples. They also studied the effectsof post-deposition treatments such as annealing for 15 min under Ar (at 200 to 600 EC) andetching in 0.5 M KCN at 40 EC for 2 min. The film characteristics were found to depend on the
sequence of post-deposition treatments. Etching of the as-deposited films resulted always in In-rich films, whereas etching after annealing resulted in more stoichiometric films since it removedsmaller amounts of Cu and Se. This is in agreement with other published data [226, IV]. The as-deposited films consisted of different components and the formation of CIS was observed onlyafter annealing. Only Cu-rich films could be identified as chalcopyrite, XRD patterns of In-richfilms did not show the characteristic chalcopyrite reflections but only those common tochalcopyrite and sphalerite. No evidence of secondary phases was seen when the depositionpotential was between -0.5 and -0.8 V vs. SCE, whereas films deposited at -0.4 V showed thepeaks of Cu2Se after annealing.  In a later publication , annealing was studied in moredetail. Annealing under a Se atmosphere was reported to result in a higher degree ofcrystallization than annealing in vacuum. Improved adhesion and film crystallinity wereobserved when a thin Cu layer was electrodeposited on Mo prior to the CIS deposition. Theimproved crystallinity was attributed to a small copper selenide excess that originated from theunderlying Cu layer when the structure was annealed in a Se atmosphere. The surfaces of theCIS films were found to be In-rich .
An In-rich surface layer was detected also on CIS films deposited from uncomplexed chloridesolutions [219, 220]. The films were deposited at -0.5 V vs. SCE, and the typical depositionsolution contained 0.004 M CuCl2, 0.008 M InCl3, and 0.008 M H2SeO3 at pH 1.5. The as-deposited semicrystalline films became polycrystalline after annealing at 500 EC under Ar for30 min. Also the grain size increased upon annealing. The bulk of the film was found to be Cu-rich which was attributed to the growth mechanism: Cu and Se deposit during the first seconds,forming a CuxSe layer which enables the assimilation of In3+ ions. At the beginning, more Cu isdeposited than In, but the amount of In increases as the deposition proceeds. That is why the filmsurface is poor in Cu.  This explains why photoelectrochemical (PEC) measurementsshowed p-type conductivity and C-V measurements n-type conductivity . PECmeasurements characterize mostly the bulk of the film where the light is mainly absorbed,whereas C-V measurements give information about the surface since the depletion region is onthe film surface .
On the other hand, C-V measurements performed by Xu et al.  on electrodeposited andvacuum-annealed CIS thin films showed p-type conductivity for films with In-rich bulkcompositions. Their CIS films were deposited from solutions containing 1 mM CuSO4, 10 mMIn2(SO4)3, 5 mM H2SeO3 and 25 mM Na-citrate at pH 3. 
Ueno et al.  deposited CIS films on Ti substrates from 10 mM CuSO4, 25 mM In2(SO4)3 and30 mM SeO2 at pH 1 at 50-55 EC. They observed that In can be co-deposited with Cu and Se at0.6 V more positive potentials than its equilibrium reduction potential. The as-deposited filmsdeposited between 0 and -0.6 V vs. SCE showed XRD reflections of CIS and Cu3Se2 whereasonly those of CIS were found for films deposited at -0.8 V. After annealing, the reflections
became stronger and the chalcopyrite phase could be identified. Films deposited at -1.0 Vshowed the reflections of metallic In in addition to those of CIS. The films were metal-rich, asevidenced by high dark currents observed during photoelectrochemical measurements. The filmswere compositionally nonuniform and exhibited poor surface morphologies. Moreover, thedeposition process was not very reproducible and was very sensitive to small changes inconditions since photoelectrochemical measurements showed different conductivity types forfilms deposited under nominally identical conditions. 
CIS thin films electrodeposited on SnO2 substrates from uncomplexed chloride solutionscontaining 5 mM of both CuCl2 and InCl3 and 10 mM SeO2 at pH 1.5 were reported to be In-richand Se-deficient in the beginning of the deposition. Cu/In ratio of 1 was obtained at -0.5 V vs.SCE. Poorly adherent films were deposited at -0.7 V or more negative potentials due to H2
evolution. The as-deposited films had XRD peaks of CIS and In2Se3, but only the characteristicchalcopyrite peaks were detected after annealing under N2 at 350 EC. The amount of Sedecreased during annealing, as did the Cu/In ratios of both Cu-rich and In-rich films. The Cu/Inratio for the stoichiometric films did not change. A low conversion efficiency of 1.5 % (activearea 0.01 cm2) was obtained for a film with Cu/In ratio of 0.95. 
CIS films deposited on rotating Ti electrodes at -0.8 V vs. SCE from 3.7 mM CuCl2, 22 mMInCl3 and 3.6 mM SeO2 at pH 1.5 were reported to contain small amounts of binary phases,possibly In6Se7 that is formed together with CIS. The broad and weak XRD peaks of the as-deposited films became sharper and more intense after annealing. The films were n-type and hadrough surface morphologies and were thus potentially suitable for photoelectrochemical (liquid-junction) solar cells. 
Raffaelle et al.  prepared all-electrodeposited CIS/CdS pn-junctions that showed good I-Vcharacteristics in the dark. The p-type CIS films of these structures were deposited fromsolutions containing 1 mM CuSO4, 10 mM In2(SO4)3, 5 mM SeO2, and 25 mM Na-citrate. They prepared also CIGS films by electrodepositing CIS films on previously electrodepositedCuGa2 layers .
Se-rich CIS films were deposited on Mo from ethylenediamine solutions containing Cu2+, In3+
and H2SeO3 at pH 1.7. The as-deposited films consisted of CIS, CuxSe, InySe and Se. Annealingdecreased the Se amount to 50 at.% but did not affect much the metal ratio. Cu-rich films wereconductive and showed the chalcopyrite reflections with preferred (112) orientation afterannealing at 350 EC or above whereas In-rich films were resistive and showed only thereflections of the sphalerite phase. Thus, the transition from chalcopyrite to sphalerite withcomposition was observed for the first time for electrodeposited CIS thin films. Chemicaltreatments in Br2 (0.05-0.1 vol.%) / MeOH and 0.1-0.5 M KCN solutions were studied too. TheBr2 treatment caused surface leveling but did not change the film composition whereas KCN was
found to dissolve selectively Cu and Se. The sequence of the post-deposition treatments wasagain found to be of importance and the results obtained were similar to those in . 
Ugarte et al.  used EDTA as the complexing agent. Their deposition solutions contained 10mM of both CuCl2 and SeO2, 15 mM InCl3, 10-20 mM EDTA, and 50 mM of glycine, NaCl andHCl each. The pH was 2. The films were deposited on SnO2 films and on Ti sheetspotentiostatically at -0.45 to -0.75 V vs. SCE. The as-deposited films showed some XRD peaksof CIS, and the crystallinity improved upon annealing. The films were etched in a cyanidesolution prior to the photoelectrochemical measurements that were performed in 0.5 M K2SO4
at pH 4.5. Despite the high dark currents (caused by the metal-rich film composition as statedearlier by Ueno et al. ), the measurements revealed that the films were p-type. The bestphotoresponses were achieved when the deposition solution contained EDTA. 
KSCN has been used as the complexing agent too [211, 216]. Due to its selectivity towards Cu+
ions it is a very promising ligand. The acidic deposition solution in  contained 2.75 mMCuCl, 2.55 mM In2(SO4)3, 3 mM SeO2 and 4 M KSCN. The deposition solution was modifiedlater by increasing the pH to 5, decreasing the KSCN concentration to 2 M and adding 0.4 Macetate buffer . The effect of electrolyte composition was studied by varying theconcentrations of the metal and selenium precursors. The In:Se ratio in the films was reportedto change with the deposition potential, while the Cu percentage in the films was approximatelyequal to its concentration percentage in the electrolyte. Annealing under a Se atmosphereincreased the crystal size more than annealing under Ar. In addition to the chalcopyrite phase,also binary Cu-Se and In-Se phases were detected in the annealed films. .
In addition to potentiostatic electrodeposition, CIS thin films have been preparedgalvanostatically. [104, 161, 163] Chowles et al.  electrodeposited near stoichiometric CISfilms at 7 mA on graphite from uncomplexed solutions containing CuSO4, In2(SO4)3 and SeO2
at pH 1. Annealing under Ar at or above 400 EC for 15 min caused the loss of excess Se andimproved the surface morphology.
The deposition solution of Sahu et al.  contained 0.73 mM CuCl, 5.27 mM InCl3 and 0.9mM SeO2 at pH 1.0. Upon scanning the potential to the negative direction during the cyclicvoltammetry measurement, Se was observed to deposit first, followed by copper and laterindium. Stoichiometric CIS films were reproducibly deposited on Mo sheets at 6 mA cm-2 fromstirred solutions at room temperature. The as-deposited films were amorphous, and XRD peaksof CIS as well as those of In2Se3 and CuSe were detected after annealing. Annealing resulted ina loss of excess Se already at 150 EC, and at 350 EC also In was lost. The as-deposited and theannealed films were p-type, with high carrier concentrations of 3.63x1020 cm-3, and resulted inlow open circuit voltages and short circuit current densities of 0.188 V and 0.056 mA cm-2,respectively.  For comparison, other devices with electrodeposited absorbers have shown
open circuit voltages of about 0.36 V, short circuit current densities between 25 and 35 mA cm-2,and conversion efficiencies between 4.8 and 7 % [164, 218].
The process of Garg et al.  was somewhat different since they used sodium selenosulfate(Na2SeSO3) as the Se source. Moreover, the deposition was carried out from basic solution (pH> 9). CuCl and InCl3, complexed with ammonia and citric acid, were used as the metalprecursors. The Cu/In ratio in the films was found to decrease with increasing deposition current.Stoichiometric, Cu-rich, or In-rich films were obtained by controlling two variables: depositioncurrent density and the solution composition. The as-deposited films showed the chalcopyriteXRD reflections which became more intense after annealing for 5 min at 400 EC. All films werep-type, but resulted in poor photoresponses (VOC 0.165 V, jSC < 1 mA cm-2). 
CIS thin films have been prepared by pulse plating too. [217, 223, 224]. The advantages of pulseplating over normal dc electrodeposition include high momentary current densities as well asimproved stoichiometry and smoother surface morphology, caused by rearrangement and partialdissolution of the film during the off-time. The duty cycle, or the ratio of the on-time to the totaltime (ton/(ton + toff)) is thus an important variable. Improved deposit distribution and adhesion anda lower impurity content have been reported for the pulse-plated films as compared to the dcelectrodeposited ones. [217, 223, 224]
Lokhande  deposited CIS thin films by pulse plating on various substrates (Ti, oxidized Ti,Mo, MoSe2, stainless steel and SnO2 film) from 0.1 M InCl3, 0.02 M CuCl and 0.05 M SeO2 atpH between 1 and 2. The depositions were carried out at room temperature with a duty cycle of33 % (5 ms on, 10 ms off). Stoichiometric CIS films were deposited when the pulse height wasbetween -0.8 and -0.9 V vs. SCE. The deposition process was poorly controlled since the firstfew films from a fresh solution were reported to be always Se-rich, and the Cu:In ratio increasedwhen the deposition time was longer than 30 min. Cu-rich films consisted of larger grains thanIn-rich films. The as-deposited films were poorly crystalline but the crystallinity improved uponannealing at 300 EC under Ar. On the other hand, Se loss was observed at temperatures higherthan 200 EC. 
Edamura and Muto  deposited CIS on ITO/glass from 2 mM CuSO4, 20 mM InCl3, 2 mMSeO2 at pH 1.5. The depositions were carried out at room temperature, and the optimumdeposition parameters were found to be: a duty cycle 33 % and a pulse height -0.8 V vs. SCE.The on- and off-times were 2 and 4 ms, respectively. Longer on-times resulted in nonuniformfilms, and shorter in scarce deposition. The as-deposited films had poor crystallinity, butchalcopyrite reflections with (112) preferred orientation were identified after annealing in air at300 EC for 1 h. The films had compact columnar structure and good adhesion. Hallmeasurements showed them to be n-type with a carrier concentration of 1.0x1017 cm-3. The bandgap was 0.99 eV, and the absorption coefficient was high, between 104 and 105 cm-1 at energies
above the band gap. 
Nomura et al.  deposited CIS thin films on Mo/glass from 1 mM CuCl2, 12 mM InCl3, and2 mM SeO2 at pH 1.8 and 40 EC. Nonpulse potential of 0.0 V vs. SCE, and pulse potentialsbetween -0.2 V and -0.9 V were used. The optimum pulse potential was found to be -0.7 V. Pulseduration was 1 ms, and the duty cycle was varied between 10 and 100 %. Se/metal ratio of about1 was maintained for a wide range of pulse potentials for duty cycles between 20-50 %.Smoothest surface was obtained for a duty cycle of 33 %. The as-deposited films were againpoorly crystalline, but annealing under N2 for 30 min improved the crystallinity, and preferred(112) orientation was observed with duty cycles of 33 % and higher. Composition of the almoststoichiometric films did not change upon annealing unless the temperature was very high.Annealing above 500 EC resulted in Se deficiency and decomposition into binary compounds.
Recently, an interesting new electrochemical technique, molecular layer electrodeposition (MLE), was introduced for the preparation of CuInSe2 thin films. The deposition solution thatcontains all the constituent ions flows over a horizontal cathode in a thin layer flow cell. Thecathode potential is controlled by a potentiostat. In addition to the advantages of normal orpulsed electrodeposition, this technique offers an additional controllable parameter, i.e., thevolume of the flowing solution. At low solution volumes, the amount of ions available forreactions is limited. Consequently, the film composition may differ from that obtained from alarger volume of solution that contains a relatively unlimited supply of ions.  Moreover,since the deposition is carried out from a single electrolyte that contains all the constituent ions,the method is simpler than electrochemical atomic layer epitaxy (ECALE)  that is based onalternating underpotential electrodeposition of the elements from separate solutions. Althoughthe formation of stoichiometric CIS films by MLE has not been reported yet, the techniquecertainly shows promise. 
Generally, the CIS-based absorbers prepared by one-step electrodeposition have not resulted inhigh-efficiency devices. Electrodeposited CIGS films can anyhow be used as precursors for thepreparation of high-efficiency devices (15.4 %) [149, 150], if the film composition is adjustedby evaporation of In, Ga and Se afterwards. The CIGS precursor films of [149, 150] weredeposited at room temperature from unstirred acidic solutions (pH about 2) containing 0.02-0.05M CuCl2, 0.04-0.06 M InCl3, 0.01-0.03 M H2SeO3, 0.08-0.1 M GaCl3 and 0.7-1 M LiCl. Thedeposition potential was -1.0 V vs. Pt, and the resulting film composition was CuIn0.32Ga0.01Se0.93
before and CuIn0.72Ga0.47Se2.05 after the PVD step [149, 150].
The highest conversion efficiencies achieved by one-step electrodeposited CuInSe2 absorberfilms without subsequent annealing under Se-containing atmospheres are those of Qiu and Shih[164, 169]. Their CIS films were deposited from a single solution that contained ''ions and
complexes of Cu, In, and Se''.  The films were post-deposition annealed at temperaturesbetween 300 and 420 EC for 20 min under Ar or in vacuum, and resulted in conversionefficiencies of 7 %  with a Mo/CIS/CdS structure and in 6.3 % with a Mo/CIS/CdS/ZnOstructure .
Kampmann et al.  electrodeposited CuInSe2 films on large substrate areas (80 cm2) fromsolutions containing 1.0 mM CuSO4, 3.0 mM In2(SO4)3 and 1.7 mM SeO2 at pH 2.4. 0.3 M K2SO4
was used as the supporting electrolyte. The as-deposited films were selenized at 500 EC underelemental selenium atmosphere, and resulted in conversion efficiency of 4.8 %.
Guillemoles et al.  obtained a conversion efficiency of 6.5 % using electrodeposited CISfilms. The films were deposited according to  and post-deposition annealed under elementalSe atmosphere for 20-30 min at 400-450 EC. The Cu/In ratio did not change upon annealing butthe Se content increased, partly due to the formation of MoSe2 between Mo and CIS. Afterannealing, the characteristic chalcopyrite reflections were observed also for the In-rich films, andthey were also strongly (112) oriented. Cu-rich films had larger grain sizes and less preferentialorientation. 
5. Characterization of thin films and their growth processes by methodsbased on cyclic voltammetry
Cyclic voltammetry is one of the most widely used electroanalytical methods forsemiquantitative studies in redox systems. It is based on varying the potential applied to theworking electrode of an electrochemical cell at a constant rate, and monitoring the current causedby electrochemical reactions taking place during the scan. The scan is typically chosen to startat such a potential value where no electrochemical reactions occur in the system. At apredetermined switching potential, the direction of the scan is reversed and the potential isscanned back to the initial value. The shape, location, sign, and magnitude of the current peaksor waves provide information about the electrochemical reactions.
5.1. Cyclic voltammetry combined with electrochemical quartz crystal microbalance
More detailed information about the reactions taking place in an electrochemical system can begained when cyclic voltammetry is used in combination with other methods, for instanceelectrochemical quartz crystal microbalance (EQCM).
The operation of the quartz crystal microbalance (QCM) is based on the converse piezoelectriceffect: an electric field applied across a piezoelectric material induces a mechanical strain in thatmaterial. The magnitude of the strain is proportional to the applied potential and its directiondepends on the polarity of the potential. Therefore, when an oscillating electric field is inducedperpendicular to the crystal surface, it produces a mechanical oscillation in the quartz crystal. Theresonant frequency of the oscillation depends on the mass and thickness of the crystal whichallows the use of the quartz crystal in the determination of very small mass changes. The quartzcrystal microbalance consists of a thin quartz crystal which has thin metal film electrodes on bothsides. The electrodes are used to induce the oscillation in the quartz crystal, and in theelectrochemical application (EQCM), one of the electrodes serves also as the working electrodein the electrochemical cell. [231, 232]
During the measurement, the potential of the EQCM electrode is changed and both the currentat the electrode and the frequency change of the quartz crystal are recorded simultaneously. Asa primary data, an EQCM measurement gives the electrode potential dependence of current andfrequency change (∆f) of the QCM crystal. Integration of the current gives the charge consumed(∆Q) that is related to the mass change of the deposit according to Faraday’s law (Eq.7)
∆Q = Fz∆m/M 
where F is the Faraday constant (96485.31 C mol-1), z the number of electrons consumed in thereaction, ∆m the mass change of the deposit during the reaction, and M the molar mass of thecorresponding chemical species.
The frequency change (∆f) may be converted to a deposit mass change ∆m by the Sauerbrey equation:
∆f = -2∆mf02/Α(µρ)2 = −Κ∆m 
where f0 is the fundamental frequency of the crystal, A the area of the electrode, and µ the shearmodulus (µ = 2.947x1011 g cm-1 s-2) and ρ the density ρ = 2.648 g cm-3) of quartz. All theconstants in the equation can be included into a single constant (K) which can be determinedexperimentally, using a deposition reaction that has a Faradaic efficiency of 100 %. As seen fromthe Equation (8), a mass increase causes a decrease in the resonant frequency and a mass decreaseresults in a higher frequency. The mass sensitivity of the EQCM can be calculated from the Kvalue if the electrode area is known. The theoretical mass sensitivity for a 5 MHz quartz crystalis 17.7 ng Hz-1 cm-2, or, expressed differently, 56.6 Hz cm2 µg-1 which means that a mass changeof 1 µg per square centimeter causes a frequency change of 56.6 Hz. The mass sensitivity for a10 MHz crystal is 4-fold (4.4 ng Hz-1 cm-2 or 226.4 Hz cm2 µg-1) since the sensitivity depends onthe square of the resonance frequency. Depending on the resolution of the frequency counter,mass changes as low as 10 ng cm-2 can be detected .
The high sensitivity of the EQCM makes it suitable for in situ mass measurements on amonolayer level or below. On the other hand, it can be used for studies on bulk processes toosince the Sauerbrey equation is valid as long as the resonant frequency change caused by massloading is less than 2 % of the fundamental frequency, that is, 0.1 MHz for a 5 MHz crystal.. EQCM has been used for various applications, including studies on underpotentialdeposition of metals, formation of surface oxides and self-assembled monolayers, adsorption anddesorption as well as monitoring of ion transport phenomena and electropolymerization. Bulkelectrodeposition and electroless deposition as well as corrosion of metals have been studied too.[231, 232, 234]
Due to the complex electrochemistry of chalcogens and their compounds, EQCM studies in thesesystems are of particular interest. Deposition and dissolution reactions occurring during cyclicvoltammetry measurements and/or growth experiments have been studied in severalsemiconductor and oxide systems including Te , Cd-Te [236, 237], Pb-Te , Cd-Se[239, 240], Pb-Se , Ag-Se  Cu-Se [243, II], Cu-In-Se [III], Cu-S , In-S , Fe-S , Pb-S  and Zn-O . EQCM measurements allow to distinguish betweenelectrochemical reactions leading to deposition or stripping and those occurring in the solution
phase . The depositing and stripping species can be identified, thus yielding informationabout the deposition and stripping mechanisms, even to the extent that enables in situcompositional analysis of compound semiconductor thin films either during growth [242, 243]or stripping [237, 239, 240]. Further, Faradaic efficiencies of reactions can be evaluated bycomparing ∆Q and ∆f data , and naturally the ∆f data alone can be used for monitoringgrowth rates.
For characterizing the electrochemical and other processes at the electrode surface, the primaryEQCM data may be treated by different ways. A simple and straightforward way is to combinethe Sauerbrey equation (Eq. 8) with the Faraday’s law (Eq.7). By defining the signs of z, ∆m, andM appropriately [II, III], one obtains
∆f = K∆QM/Fz = (K/F) (M/z)∆Q 
If the frequency change (∆f) is plotted as a function of the charge consumed (∆Q), then the slopeof such a plot (d∆f/d∆Q) may be used for the calculation of M/z values:
M/z = (d∆f/d∆Q) (F/K) 
The theoretical M/z is simply the change of the molar mass of the deposit divided by the numberof electrons involved in the reaction. The experimental M/z values obtained by this way do notinvolve any hypothesis about the reaction mechanisms but still represent directly the primarydata. On the other hand, a theoretical M/z value is easily calculated for any suggested reaction.An agreement between the observed and theoretical M/z values gives thus a quite solid proof forthe dominance of the suggested reaction while differences call attention for other mechanisms.[II, III]
Figure 5 [II] presents examples of ∆f vs. ∆Q plots for the deposition of Cu2-xSe at differentpotentials, as well as the corresponding M/z values calculated from the slopes of the plots. Thedifferent slopes obtained for different deposition potentials may indicate changing filmcompositions, morphologies, or growth mechanisms at the different potentials.
M/z = 50.04 g mol-1
M/z = 33.40 g mol-1
M/z = 18.57 g mol-1 (-0.1 V)
∆ Q / C
Figure 5. ∆f vs. ∆Q plots for the deposition of Cu2-xSe at -0.1 V, -0.3 V and -0.5 V vs Ag/AgCl
5.2 Cyclic photovoltammetry and photoelectrochemical characterization under choppedillumination
Similar to cyclic voltammetry, cyclic photovoltammetry and photoelectrochemicalcharacterization are semiquantitative techniques that give information of photoactivity andconductivity type of semiconducting films. In both techniques, the working electrode isilluminated during the measurement. Often chopped illumination is used but it is also possibleto make the measurements separately in the dark and under illumination and compare thedifference afterwards. Usually polychromatic illumination (white light) is used butmonochromatic illumination can be used too as long as the energy of light is higher than that ofthe band gap of the semiconductor. If the film is photoactive, a photocurrent is detected, i.e., thecurrent is higher under illumination than in the dark. The direction of the photocurrent givesinformation of the conductivity type of the film. Cyclic photovoltammetry can be used for in situdetection of formation of a photoactive deposit, and photoelectrochemical measurements forevaluating photoactivity as a function of, for instance, different post-deposition treatments.
When a semiconductor is immersed in a solution, an electric field develops at the solid/liquidinterface via charge transfer reactions between the two phases. The electric field enables theseparation of charge carriers, analogously to a pn-junction of a Schottky junction. Illuminationof the semiconductor causes a dramatic increase of the concentration of minority carriers, e.g.,electrons in a p-type semiconductor. The electric field drives the photogenerated minority carrierstowards the semiconductor/liquid interface, where they may participate electrochemical reactionsin the solution with a suitable redox species. Thus a p-type semiconductor is capable of reducingmore species under illumination than in the dark, causing an increase of cathodic current while
the anodic current remains unaffected. An n-type semiconductor acts the other way: anodiccurrent is enhanced under illumination as compared to dark, whereas cathodic current is notaffected. Semiconductor/liquid junctions are the basis of photoelectrochemical solar cells that areused for production of electricity or fuels. The photoelectrochemistry on semiconductorelectrodes has been studied a lot [249, 250].
In cyclic photovoltammetry, a cyclic voltammogram is measured in the deposition solution underillumination. Formation of a photoactive deposit during the measurement can easily be detectedby comparing the currents in the dark and under illumination. Thus the potential rangecorresponding to the formation of a semiconducting compound as well as the conductivity typeof the compound can be identified.  Cyclic photovoltammetry has been used for the reactionmechanism studies in a variety of semiconductor systems , also in the Cu-In-Se system[207, 252, 253, IV].
Photoelectrochemical (PEC) measurements, in turn, give information about the film propertiesafter deposition. The measurements are performed in an electrolyte solution that contains a redoxspecies the potential of which is in a suitable position with respect to the band edges of thesemiconductor so that charge-transfer reactions between the semiconductor and the solution arepossible. [249, 250] Photoelectrochemical measurements allow a simple and fast characterizationof the semiconducting properties of the film, and they have been used especially for comparativestudies between different post-deposition treatments.
PEC measurements on p-type CIS films are often performed in sulfate solutions, either sulfuricacid [106, 220, 254] or mildly acidic K2SO4 [222, IV] but other solutions such as the polysulfide(NaOH/Na2S/S) can be used too [116, 214]. In addition to conductivity type and the magnitudeof photocurrent, PEC measurements can be used for the determination of flat-band potential. Theband edge positions of CIS are strongly dependent on the electrolyte and on the surface chemistryof the film which may complicate the interpretation of the data, however [254, 255].
6.1. Deposition of films
The films were electrodeposited potentiostatically, i.e., at constant potential, using either anAutolab PGSTAT20 or a Metrohm 626 potentiostat with a three-electrode setup. A Ag/AgCl/3M KCl electrode was used as the reference electrode to which all the potentials in this work arereferred to, and a Pt plate or a graphite rod was used as the counter electrode. Substrates were 100nm Mo or ITO films sputtered on glass, and they were washed ultrasonically in water and ethanolbefore the depositions. The ZnO films were deposited using a standard three-electrode setup, andthe Cu2-xSe and CIS films using a two-compartment three-electrode arrangement where theanodic and cathodic compartments were separated with a salt bridge in order to prevent sidereactions at the anode. The salt bridge was filled with saturated KCl solution, and 0.1 M KClsolution served as the counter electrolyte in the anodic compartment. All films were depositedfrom unstirred solutions.
The Cu2-xSe and CIS depositions were carried out at room temperature from acidic (pH between2.4 and 3.1) solutions containing CuCl, SeO2, and in the case of CIS also InCl3. In order to enablefilm growth by the induced co-deposition mechanism, thiocyanate ions (SCN-) were used ascomplexing agents for the Cu+ ions to shift their reduction potentials to the negative direction sothat selenium deposits first and induces the formation of Cu2-xSe and CIS. The thiocyanate ionconcentration had to be very high (2-4 M) in order to prevent precipitation of the sparinglysoluble CuSCN. At such high SCN- concentrations the Cu+ ions were mainly present as[Cu(SCN)4]3- complexes . The concentrations of the Cu and In precursors were chosen tobe considerably higher than that of the Se precursor, in order to prevent the deposition ofelemental selenium.
The doped ZnO thin films were electrodeposited at 80 EC from aqueous 0.05 M zinc nitrate bathscontaining additionally either InCl3 or Al(NO3)3. The InCl3 concentration was varied between0.0005 M and 0.005 M and the Al(NO3)3 concentration between 0.001 and 0.01 M.
All solutions were prepared using ion-exchanged water and chemicals of minimum 98 % purity.
6.2. Characterization of films
Film morphology was studied by a Zeiss DSM 926 scanning electron microscope (SEM) at theElectron Microscopy Unit at the University of Helsinki. Approximate cation ratios and filmthicknesses were determined by a Link ISIS energy dispersive X-ray spectrometer (EDX) using
20 kV accelerating voltage. The results were calculated using a GMR Electron Probe Thin FilmMicroanalysis program . Density values of 5.99 g/cm3 for Cu2-xSe, 5.77 g/cm3 for CuInSe2,5.6 g/cm3 for ZnO and 10.2 g/cm3 for Mo  were used in the thickness calculations.
More accurate film compositions as well as the impurity contents were determined by ion beammeasurements that involved Rutherford backscattering spectrometry (RBS) and time-of-flightelastic recoil detection analysis (TOF-ERDA), performed at the Accelerator Laboratory of theUniversity of Helsinki. Ion beams of 4He+ at 6.5 MeV were used for RBS and 197Au9+ at 48 MeVTOF-ERDA measurements. The ion beams were generated by a tandem EGP-II accelerator.
The crystallinity of the films was examined by Philips MPD 1880 and Bruker AXS D8 powderX-ray diffractometers, using Cu Kα radiation. The step width was 0.02E and the time per step was1, 2, or 10 s.
The thicknesses of the ALD-grown ZnO films were determined by fitting their transmissionspectra according to . The transmission spectra were measured with a Hitachi U-2000 UV-vis spectrophotometer at a wavelength range of 370-1100 nm.
6.3. Characterization of film growth processes
Preliminary studies on film growth processes included cyclic voltammetry and cyclicphotovoltammetry that were performed using the Autolab PGSTAT20 potentiostat and the three-electrode setup described previously. In addition to Mo and ITO films, also previously depositedCu2-xSe and CIS films were used as the substrates. The cyclic photovoltammograms weremeasured under chopped polychromatic illumination provided by a 50 W halogen lamp. Moredetailed characterization was done by using the above mentioned techniques in combination withthe electrochemical quartz crystal microbalance (EQCM). The potential scan rate was 10 mV/sin all measurements, whether performed with or without the EQCM.
For the combined cyclic voltammetry and EQCM studies, the Autolab PGSTAT20 potentiostatwas equipped with EQCM (Institute of Physical Chemistry, Polish Academy of Sciences inWarsaw, Poland) . A standard three electrode configuration was employed where one of theelectrodes of the quartz crystal served as the working electrode. A Fluke timer/counter PM6680Bwas used for recording the frequency change of the quartz crystal. The quartz crystals wereunpolished 5 MHz AT-cut plano-convex crystals with evaporated Au film electrodes on bothsides, and they were operated at the fundamental mode. The crystals were mounted vertically ata PTFE holder  where the projected area of the Au electrode was 0.236 cm2.
The electrolytes used in the EQCM studies of Cu and In depositions contained 4 M KSCN and
0.05 M CuCl or 0.05 M InCl3, respectively. The solutions used for the studies on the binaryselenides contained additionally 0.001 M SeO2. The solution used in the studies on the ternaryCu-In-Se system contained 0.05 M CuCl, 0.05 M InCl3 and 0.001 M SeO2 in 4 M KSCN. In allsolutions that contained Cu or In precursors, 4 M KSCN was used as the complexing agent. Theelectrolyte for the Se deposition study contained 0.001 M SeO2 and 0.1 M KCl as the supportingelectrolyte. pH was 3 in all solutions except in the In and In-Se solutions where it was 2.
6.4. Post-deposition treatments
In order to make their properties to match better to those required for photovoltaic qualitymaterial, the CIS films were subjected to post-deposition treatments that included crystallinityimprovement by annealing as well as stoichiometry correction either by etching or by depositingan In2Se3 layer on the CIS film.
The annealing was done in a tube furnace under a N2 atmosphere either at 400 EC for 15 min orat 500 EC for 2.5 h. In either case, the films were allowed to cool down to room temperatureslowly under N2. Some of the CIS films were dipped in a saturated NaCl solution before or afterannealing, to study the effect of Na+ ions because they should have beneficial effects on filmmorphology, conductivity and defect distribution (see Chapter 2.1.1).
To improve the film stoichiometry, the excess Cu and Se were removed by etching the films in0.5 M KCN aqueous solution for different time periods (30 s-30 min). KCN etch is the traditionalway to remove the excess copper and chalcogen from chalcopyrite thin films [205, 212, 222].
An alternative attempt to correct the film stoichiometry without etching was made by depositingan In2Se3 film on the CIS film before annealing at 500 EC. In some cases, the CIS film waspreviously annealed at 400 EC. The In2Se3 films were electrodeposited according to Massaccesiet al.  at 80 EC except that InCl3 was used instead of In2(SO4)3. The deposition solutioncontained 0.1 M K2SO4, 0.01 M H2SO4, 0.002 M InCl3 and 0.001 M SeO2. The depositionpotential was -0.6 V and the deposition time ranged from 5 to 30 min, resulting in filmthicknesses between about 22 and 134 nm.
The effects of the post-deposition treatments on the photoactivity of the films were studied bymeasuring photoelectrochemical (PEC) scans in 0.5 M K2SO4 at pH 4.0-4.5. The PECcharacterization was carried out using the Autolab PGSTAT20 potentiostat and polychromaticillumination provided by a 50 W halogen lamp. The light was modulated with a timer relay andthe distance between the lamp and the working electrode was held constant, about 25 cm. A lightchopping sequence of 0.5 s on, 0.5 s off was used. The CIS films in the PEC studies were about400-500 nm thick and they were deposited at -0.5 V vs. Ag/AgCl.
6.5. Preparation of solar cells
Both substrate and superstrate solar cell structures were prepared (see Figures 3 and 4 in Chapter2.1). Most of the solar cells were prepared using 400-500 nm thick CIS films that were depositedat -0.5 V. The films were annealed and etched as described in the previous chapter. Some of thedevices were prepared using the annealed CIS+In2Se3 films that were not etched. In someexperiments, thicker CIS films of about 1 µm were used.
The CdS films were prepared by chemical bath deposition (CBD). The pretreated CIS films wereimmersed in solutions containing in most cases 1 M NH3, 0.001 M Cd(CH3COO)2 and 0.06 Mthiourea ((NH2)2CS) at 60 or 80 EC.  Some of the CdS films were deposited at 65 or 90 ECusing cadmium sulfate as the metal precursor according to . The thicknesses of the CdSfilms were either 50 or 150 nm. Some devices were prepared without the CdS film.
The ZnO layers were prepared either by electrodeposition, ALD, or sputtering. Theelectrodeposited as well as the ALD-grown ZnO films were prepared in our laboratory and thesputtered films were prepared either in Laboratoire d’Electrochimie et de Chimie Analytique,Ecole Nationale Supérieure de Chimie de Paris or in Hahn-Meitner-Institut (HMI) in Berlin.
All electrodeposited ZnO:In films used in the solar cells were deposited from solutions where theInCl3 concentration was 0.005 M, and the ZnO:Al films from solutions where the Al(NO3)3
concentration was 0.001 M. The deposition potential for the ZnO:In films was -1.2 V unless toldotherwise, and that for the ZnO:Al films -1.1 V. The undoped ZnO films used in some deviceswere deposited at -0.8 V from 0.05 M Zn(NO3)2 solutions at 80 EC . The thicknesses of theundoped and doped electrodeposited ZnO films were about 100 and 400 nm, respectively.
The ALD-ZnO films were prepared in a flow-type F120 ALD reactor (ASM-MicrochemistryLtd.) at 250 EC using dimethylzinc (DMZ), trimethylaluminum (TMA) and water as theprecursors. The temperature of the DMZ source was -20 EC, and TMA and water were used atRT. For the Al doped ZnO films, 3 % of the metal precursor pulses were TMA pulses. The pulseand purge lengths were 0.2 and 0.5 s for DMZ, 2 and 10 s for TMA and 1 and 3 s for water,respectively. The resistivities of the undoped and doped ALD-ZnO films were 2-4x10-2 and 5-10x10-3 Ω cm, respectively, and their thicknesses were 50 and 350 nm, respectively.
The superstrate structures were prepared by depositing first a CdS film on ITO and then a CISfilm on the CdS. The structure was annealed under N2 at 400 EC for 15 min. Au films (70 nm)were evaporated on the CIS for back contacts.
6.6. Electrical characterization
Information about the conductivity type of the CIS films was obtained by three methods: cyclicphotovoltammetry, photoelectrochemical measurements and thermoelectric probe measurements.The descriptions of the first two methods were given in Chapter 5.2. The thermoelectric probemethod allows the determination of conductivity type by the sign of thermal voltage generatedby a temperature gradient . The measurements were made using a CEM DT-3900 digitalmultimeter with one of the two tips at room temperature and the other cooled to the temperatureof liquid nitrogen.
Sheet resistances of the ALD-grown ZnO films were measured by the four point probe methodusing a Keithley 2400 Source Meter and Alessi C4S Four Point Probe head.
Current-voltage (I-V) characteristics of the devices were measured in dark and under illuminationof a 50 W halogen lamp, using the Keithley 2400 source meter. Source delay of 0.1 s and stepwidths of either 0.01 or 0.05 V were used.
For the devices prepared with the electrodeposited ZnO films, it was necessary to evaporate thin(10 to 100 nm) Al films for the front contacts. This was because of the low conductivity of theelectrodeposited ZnO films. The ZnO films prepared by the gas phase methods were conductiveenough so that no additional contacts were needed.
A Hewlett-Packard 4284A Precision LCR meter was used for the capacitance-voltagemeasurements. The LCR meter measures the complex impedance (the magnitude and phase angleof impedance) that is the total opposition of the device or the circuit to the alternating currentflow at the measurement frequency. The capacitance is then calculated using equivalent circuitmodes that contain a capacitor and a resistor, either in parallel or in series with each other. Themost appropriate of the two possible modes is chosen according to whether the parallel or theseries resistance of the circuit is more significant. For polycrystalline thin film solar cells, theparallel resistance seems to be more significant , and thus the parallel circuit mode was usedhere. The measurement frequencies were between 100 kHz and 1 MHz, and the amplitude of thealternating current was 5 mV. Measuring direction was usually from reverse to forward, and thevoltage step was between 0.01 and 0.1 V, in most cases 0.05 V. In order to ensure that thejunctions were rectifying, I-V curves were measured from the same contact dots.
The electrical front contacts for the measurements (when needed) were done by evaporating thin(about 10 to 100 nm) Al dots on the samples by electron beam evaporator IM9912 (InstrumenttiMattila Oy) with a Telemark 241 electron beam source. Contact area was either 0.052, 0.204, or3.14 mm2. The back contacts for the capacitance measurements were made by contacting a thinCu wire to the Mo substrate using In as a solder.
7. Results and discussion
This chapter summarizes the main results of this thesis. The results that are not included in thepublications, i.e., the capacitance results and most of the solar cell results, are discussed in moredetail here.
7.1. Cu2-xSe films
7.1.1. Film growth [I]
In order to achieve suitable conditions for induced co-deposition, the Cu+ ions were complexedwith SCN- ions to form strong complexes . The concentration of the SCN- ions had to bemuch higher than that of Cu+ ions in order to avoid the precipitation of insoluble CuSCN. Thecomplex formation equilibria depend also on the pH of the solution For instance, a SCN-
concentration of 4 M was required for Cu+ concentration of 0.05 M at the pH range used in thisstudy. Under these conditions, the Cu+ ions were mainly present as [Cu(SCN)4]3- . Thecomplexing shifted the reduction potentials of the Cu+ ions to the negative direction, so that thereduction of HSeO3
- occurred at less negative potentials than that of [Cu(SCN)4]3-. The depositionof Se thus induced the reduction of [Cu(SCN)4]3- ions at potentials less negative than where thedeposition of metallic Cu started.
The induced co-deposition mechanism allowed a wide potential range where the filmcomposition was nearly constant. The films deposited between -0.3 and -0.6 V contained about60-65 % Cu, corresponding to Cu2-xSe with x = 0.15-0.5. At potentials less negative than -0.3 V,the current density was very low, corresponding probably to the deposition of Se. At potentialsmore negative than -0.6 V, the current density increased due to the deposition of Cu-richmaterial, and at even more negative potentials metallic Cu was deposited. The growth rate of theCu2-xSe films was about 0.07-0.1 µm h-1.
The as-deposited films were amorphous but showed reflections of the cubic Cu2-xSe phase after annealing at 400 EC under N2 for 15 min. SEM studies revealed that the surface morphologyof most of the Cu2-xSe films was rough, containing rather large pores. Similar structures havebeen presented in the literature for Cu3Se2  and CuSe  films.
7.1.2. Growth processes studied by cyclic voltammetry and EQCM [I, II]
The electrochemical behavior of the Cu-Se system was studied first in a preliminary manner bymeasuring cyclic voltammograms on Mo films and on previously deposited Cu2-xSe films. Moredetailed characterization of the deposition processes was performed by using cyclic voltammetryin combination with EQCM. The reaction mechanisms were ascertained by growth experimentsperformed with the EQCM at constant potentials.
The reduction of HSeO3- to Se on the Au electrode was found to proceed via a 4e- net reaction
(Eq. 11) at the potential range between +0.12 and -0.38 V. At low overpotentials, i.e., in thepositive end of this potential range, the deposition of Se was found to proceed via a surface-induced process that resembles the underpotential deposition (UPD) of metals.
HSeO3-(aq) + 5 H+(aq) + 4 e- º Se(s) + 3H2O 
Theoretical M/z = 19.74 g mol-1
The formation of H2Se via the reduction of the deposited Se film (Eq. 12) was found to begin at-0.41 V which was verified also by measuring the scans on a previously deposited Se film in 0.1M KCl. The reduction potentials of the Se species were found to be strongly dependent on theelectrode surface.
Se(s) + 2 H+(aq) + 2 e- º H2Se(aq) 
Theoretical M/z = -39.48 g mol-1
The reduction of [Cu(SCN)4]3- to metallic Cu according to the reaction (13) started at -0.65 V,which is considerably more negative than the equilibrium reduction potential of Cu+ (+0.298 V), thus verifying the strong complexing ability of the SCN- ions towards Cu+. Thus thereduction potential of the [Cu(SCN)4]3- complex was prominently more negative than thoseobserved for either HSeO3
- (+0.12 V) or Se (-0.41 V).
[Cu(SCN)4]3-(aq) + e- º Cu(s) + 4 SCN-(aq) 
Theoretical M/z = 63.55 g mol-1
The reduction of [Cu(SCN)4]3- on a previously deposited Se film was found to begin at -0.25 V,i.e., at considerably more anodic potential than on the Au electrode. This is apparently due to theformation of Cu2-xSe according to the reaction (14).
Se(s) + 2 [Cu(SCN)4]3-(aq) + 2 e- º Cu2Se(s) + 8 SCN-(aq) 
Theoretical M/z = 63.55 g mol-1
The current flow ceased at about -0.4 V, indicating that the initial Se surface was now completelycovered with Cu2-xSe. The current began to flow again at about -0.63 V where the deposition ofmetallic Cu started. Figure 6 shows the cyclic voltammograms for [Cu(SCN)4]3- on Au and onSe.
-0.8 -0.6 -0.4 -0.2 0.0-1.5x10-3-1.0x10-3-5.0x10-4
E / V vs. Ag/AgCl
I / A
Figure 6. Cyclic voltammograms measured in a [Cu(SCN)4]3- solution on Au (solid line) and on Se(dotted line) surfaces
This result verifies that Se induces the reduction of [Cu(SCN)4]3- and thus the formation of Cu2-
xSe before the deposition of metallic Cu begins, and it was further supported by the fact that theformation of Cu2-xSe from a solution containing both [Cu(SCN)4]3- and HSeO3
- was observed tooccur between -0.23 and -0.65 V.
Thus, during the cyclic voltammogram measurement, Se deposited first according to reaction(11), followed by the formation of copper selenide. The formation mechanism of copper selenidechanged gradually from reaction (14) to reaction (15) as the previously formed Se film becamecovered with Cu2-xSe. The deposition of metallic copper began only at the more negativepotentials.
2 [Cu(SCN)4]3-(aq) + HSeO3-(aq) + 5 H+(aq) + 6 e- º Cu2Se(s) + 8 SCN-(aq) + 3H2O 
Theoretical M/z = 34.34 g mol-1
The observed M/z values were in excellent agreement with the theoretical ones, thereby
illustrating good Faradaic efficiencies and thus the absence of side reactions, and mostimportantly the validity of these reaction mechanisms.
In contrast to the case with cyclic voltammetry measurements, the M/z values obtained duringthe growth experiments at constant potentials were not equal: at -0.3 V the M/z value was 33.40g mol-1 corresponding to reaction (15) whereas at -0.5 V a larger value, 50.04 g mol-1, wasobtained, i.e. the apparent mass of the deposit increased faster at -0.5 V than at -0.3 V althoughthe current densities were equal. Since the film compositions (measured by EDX) were similarat both potentials, the difference has to be attributed to the roughening of the film surface duringthe film growth at -0.5 V. A similar explanation was given by Marlot and Vedel  too.Surface roughness is known to cause liquid trapping in surface cavities which in turn results inadditional mass increases .
The idea of morphology being responsible for the above difference was further supported by theobservation that when the deposition was started at -0.3 V and continued at -0.5 V, the M/z valueremained between 30 and 35 g mol-1 during the whole deposition [I]. This implies that when thedeposition starts at -0.3 V with a smooth morphology, the film surface remains smooth even ifthe potential is shifted to a more negative value that normally produces a rougher surface. At thesame time, the M/z value remains unchanged. This finding quite convincingly rules out also thepossibility that the M/z difference would be due to differing impurity amounts, like water orthiocyanate, at the different deposition potentials.
7.2. CuInSe2 films
7.2.1. Film growth [I, IV]
A typical example of the relative composition (measured by EDX) of the CIS films as a functionof the deposition potential is presented in Figure 7a. The film composition was constant and closeto the stoichiometric Cu:In:Se ratio of 1:1:2 over a wide potential range. All systems studiedbehaved similarly: neither the film composition, growth rate nor the potential range for thecompound formation was affected significantly by the solution composition, as long as tworequirements were met: the concentrations of the metal precursors in the solutions were muchhigher than that of the selenium precursor, and the concentration of the SCN- ions was highenough to keep all the Cu+ ions as [Cu(SCN)4]3- so that there were no free Cu+ ions in thesolution.
The film compositions remained essentially constant also when the concentration ratio of themetal precursors in the solution was changed between 0.1 and 2.5, as illustrated in figure 7b. Thisprovides further evidence that the induced co-deposition mechanism is operating in the system.
-0.7 -0.6 -0.5 -0.4 -0.3 -0.20
Deposition potential (V) vs. Ag/AgCl0.0 0.5 1.0 1.5 2.0 2.5
[Cu]/[In] ratio in the deposition solution
Figure 7. Relative amounts of Cu, In and Se in the CIS films by EDX a) as a function of the depositionpotential (Deposition solution: 0.05 M CuCl, 0.07 M InCl3, 0.001 M SeO2 and 4 M KSCN.) and b) as afunction of the Cu/In ratio in the deposition solution (Deposition potential -0.5 V vs. Ag/AgCl.)
The constant composition was Cu1.30In1.00Se2.20 according to RBS and Cu1.30In1.00Se2.18 accordingto TOF-ERDA, i.e, the films contained an excess of Cu2-xSe. According to TOF-ERDA, the filmscontained also a large amount of impurities, the main ones being oxygen, hydrogen, sulfur,carbon, and nitrogen. The oxygen and hydrogen impurites (both about 8 at.%) originate fromwater and hydroxyl residues from the deposition solution. Since the amounts of S, C, and N wereequal, about 6 at.% each, the films were deduced to contain thiocyanate ions. Similar to the Cu2-
xSe films, also the CIS films were amorphous as deposited. This may partly be due to the highamount of impurities hindering the crystallization.
Annealing at 400 EC under N2 for 15 min was enough to make the films crystalline with thecharacteristic chalcopyrite XRD reflections . Despite the large Cu2-xSe excess in the films,no reflections corresponding to Cu-Se phases were detected, possibly because the diffractionpeaks of the cubic Cu2-xSe phase  may overlap with the some peaks of the CIS chalcopyritephase .
The relative amounts of Cu, In, and Se in the films remained essentially the same after annealing,but the impurity contents decreased. The thiocyanate ions probably decomposed during annealingsince the carbon and nitrogen contents in the films decreased to about 1 at.% while the sulfurcontent remained higher, about 4 at.%.
Etching in 0.5 M KCN decreased the amounts of Cu and Se in all the films. In an agreement withliterature [212, 226], the order of the post-deposition treatments was found important. If the filmswere annealed before etching, their compositions approached the stoichiometric but filmmorphology or crystallinity were not affected. On the other hand, etching of the as-deposited
films resulted in partial removal of the film, and the remaining part showed larger decrease of theCu and Se contents. After annealing these samples showed several broad XRD peaks that couldnot be identified unambiguously. The only peaks possibly corresponding to the chalcopyritephase were the (112) and (204/220) reflections, and the remaining peaks were attributed to InySeor InySe-rich CIS phases.
7.2.2. Growth processes studied by cyclic voltammetry and EQCM [III, IV]
The combined cyclic voltammetry and EQCM studies confirmed the formation of CIS by theinduced co-deposition mechanism at potentials more positive than where Cu+ or In3+ alone arereduced. Although the reduction of In3+ began earlier on a Se surface than on a Au surface,implying formation of In-Se compounds at more positive potentials than where the depositionof metallic In occurs, no binary InySe compounds could be deposited at the potential range whereCuInSe2 formation was observed. Thus the formation of CIS is concluded to proceed via theformation of Cu2-xSe, and may be described as follows: Se deposits first (reaction 11) and inducesthen the formation of Cu2-xSe (reaction 14) at more positive potentials than where Cu+ or In3+
alone are reduced. The formation of Cu2-xSe then induces, at the same potential range, theunderpotential assimilation of In3+ and the formation of CIS (reaction 16).
Cu2Se(s) + 2 In3+(aq) + 3 HSeO3-(aq) + 15 H+(aq) + 18 e- º 2 CuInSe2(s) + 9 H2O 
The net reaction is
2 HSeO3-(aq) + [Cu(SCN)4]3-(aq) + In3+(aq) + 10 H+(aq) + 12 e-
º CuInSe2(s) + 4 SCN-(aq) + 6 H2O Theoretical M/z = 28.02 g mol-1
Figure 8 shows a cyclic voltammogram (solid line) and the simultaneous frequency change(dotted line), measured in the CIS deposition solution. The slope of the ∆f vs. ∆Q plot (Fig. 5cin III) corresponding to the CuInSe2 formation decreased during the cyclic voltammogram untilit settled to a constant value. This suggests that the CIS formation begins on the previouslyformed Se film and that the deposition mechanism changes during the cyclic voltammogramwhen the Se film becomes covered with CIS, analogous to the behavior observed in the Cu-Sesystem [II]. An M/z value of 23.19 g mol-1 was observed between -0.28 and -0.64 V. In contrastto the Cu-Se system, film depositions at constant potentials (-0.3 V and -0.5 V) yielded alsoessentially equal slopes. This may be due to smoother surface morphology of CIS as comparedto that of Cu2-xSe.
-0.8 -0.6 -0.4 -0.2 0.0-8.0x10-5
E / V vs. Ag/AgCl
I / A
∆f / H
Figure 8. Cyclic voltammogram (solid line) and the simultaneous frequency change (dotted line),measured in the CIS deposition solution.
The formation of p-type semiconducting films was confirmed by cyclic photovoltammetrymeasurements in the deposition solution on Mo and Au surfaces, in the latter case in combinationwith EQCM measurements. The current densities on the Au electrode were always higher thanon the Mo electrode which may result from the different work functions of the two metals.Ideally, the formation of a low-resistance, or ohmic, contact between a metal and a p-typesemiconductor requires the work function of the metal to be higher than that of the semiconductor. Therefore, as the work function of Au is higher than that of Mo , the current flow acrossthe Au/CIS junction may be facilitated because of lower contact resistance as compared to theMo/CIS junction.
When measured on previously deposited CIS films, the photoactivities started at more positivepotentials and were stronger than on bare electrodes. This is due to the improved light absorptionin a thicker semiconductor film than in a thinner one. Fig. 9 presents the cyclic voltammogramand the simultaneous frequency (mass) change, measured on a Au surface. The reason for thephotoactivity starting in this case already in the very beginning of the scan is that the scan in thefigure is a third successive scan. A weak photoeffect can be seen also in the frequency plotalthough it is much weaker than that observed in the cyclic voltammogram. Thus the film growthrate under illumination does not differ significantly from that in the dark. The maximum valueof Idark-Iph is about 7.4 µA which corresponds to a photocurrent density of about 30 µA/cm2. Themeasurements yielded similar M/z values as those obtained in [III].
-0 .6 -0 .5 -0 .4 -0 .3 -0 .2 -0 .1 0 .0-1 .2x10 -4
-1 .0x10 -4
-8 .0x10 -5
-6 .0x10 -5
-4 .0x10 -5
-2 .0x10 -5
0 .02 .0x10 -5
E / V vs . A g /A gC l
∆f / H
Figure 9. Cyclic photovoltammogram and the simultaneous frequency change under chopped illumination,measured in a solution containing 2 M KSCN, 0.01 M CuCl, 0.01 M InCl3, and 0.001 M SeO2.
7.2.3. Photoelectrochemical characterization [IV]
Photoelectrochemical characterization of the CIS films was performed in order to study theeffects of post-deposition treatments on their photoactivities. The as-deposited films were veryweakly p-type. Photoactivity was lost completely after annealing, regardless of the annealingtemperature. This may be due to the segregation of the detrimental Cu2-xSe phase to the surfaceor at the grain boundaries. On the other hand, it is possible that the as-deposited films containCuSCN as an impurity. CuSCN is a p-type semiconductor, and thus the lowering of photoactivitymay result from its decomposition upon annealing.
The photoactivities of the as-deposited and the annealed films improved markedly after etchingin 0.5 M KCN. The films were p-type regardless of the post-deposition sequence. The bestphotoactivity was achieved when the annealing treatment was performed before the etching, andthe optimum etch time was determined to be 1 min, resulting in a photocurrent density of 50µA/cm2. All the PEC scans showed high dark currents which is probably due to the metal-richcomposition [214, 222] or the presence of Cu2-xSe in the films.
The PEC experiments enabled also the modification of the deposition process to consume lessmetals (by a factor of five) and KSCN (by a factor of two) since the films deposited from themodified solution exhibited similar photoactivities to those deposited from the original one.When the CuCl concentration was lowered from 0.05 M to 0.01 M, the KSCN concentrationcould be lowered from 4 M to 2 M. Because of the lower KSCN concentration, the amounts ofsulfur and nitrogen impurities in the films decreased to about 2-3 at-%. The growth rate was notaffected since it was determined by the HSeO3
- concentration that was not changed.
The highest photocurrent densities, about 100 µA/cm2, were measured for the films prepared bydepositing an In2Se3 film on the CIS film and annealing the bilayer at 500 EC. Despite their Cu-poor compositions, these films were p-type too. Fig 10 shows an example of the PEC responseof a such film in 0.5 M K2SO4 solution.
-1.0 -0.8 -0.6 -0.4 -0.2 0.0-250
j / µ
E / V vs. Ag/AgCl
Figure 10. Photoelectrochemical response of a CIS + In2Se3 bilayer film in 0.5 M K2SO4. The bilayer filmwas prepared by depositing In2Se3 for 20 min on as-deposited CIS before annealing at 500 EC.
7.2.4. Capacitance-voltage measurements
One of the important properties of a semiconductor material is its charge carrier density. For asemiconductor to be useful as an absorber material in a solar cell, its carrier concentration hasto be, on one hand, high enough in order for the material to be conductive enough. On the otherhand, a too high carrier concentration causes unwanted recombination of the photogeneratedcharge carriers and thus deteriorates the conversion efficiency of the solar cell.
Capacitance-voltage (C-V) measurement is the most commonly used method for thedetermination of carrier densities in semiconductor materials. When the capacitance of a reverse-biased semiconductor junction is measured as a function of the applied reverse bias V, theapparent carrier density can be calculated from the slope of the (A/C)2 vs. V plot according to theequation
Ne d A C dVA
02ε ε ( / ) /
where NA is the acceptor concentration in a p-type material, e is the elemental charge, ε0 is the
permittivity of vacuum and εs the dielectric constant of the semiconductor material. 
Successful employment of the method requires the depletion layer approximation, i.e., that thereare no mobile charge carriers in the depletion region. Further assumptions are that all dopants areionized and that there are no minority-type dopants.  Deviations of real systems such aspolycrystalline diodes  from these assumptions may complicate the situation, and thereforeinterpretation of C-V data is not always straightforward, and the results presented here shouldbe considered just indicative.
Both Schottky junctions (glass/Mo/CIS/Al) and pn-junctions (glass/Mo/CIS/CdS/Al) werestudied, and similar results were obtained, in agreement with literature . The apparentcapacitance values were smaller at higher frequencies which may indicate the presence of trapsor interface states [267, 268].
The carrier concentrations of annealed, unetched films were very high; values between 3x1019
and 6x1019 cm-3 were obtained that are several orders of magnitude higher than those measuredfor high-efficiency CIS absorbers. These high carrier concentrations were probably due to thepresence of Cu2-xSe that is known to be a degenerate p-type semiconductor and has therefore ahigh carrier concentration.  High carrier concentrations are in fact very common toelectrodeposited CIS films; see, for example [163, 215]. On the other hand, carrier concentrationsin those electrodeposited CIS films that have resulted in relatively high conversion efficienciesare lower, about 1-2x1016 cm-3 [42, 164].
The KCN etching reduced the carrier concentrations by approximately a decade, to 1.3-10x1018
cm-3, but these values were still very high. This may be due to incomplete removal of copperselenide from the material. Another possible reason is that the etching treatment caused pinholes.
The carrier concentrations of the CIS + In2Se3 bilayer films were closer to those measured fromgood CIS samples, between 4x1016 and 5x1017 cm-3. This is in an agreement with the results ofPEC measurements that showed the highest photoactivities for the CIS+In2Se3 bilayer films.
7.3. Doped ZnO films [V]
The cathodic electrodeposition of oxides from nitrate solutions is thought to proceed via thereduction of nitrate ions according to reaction 19. The electrochemically generated hydroxideions then react with the metal ions in the solution to form a metal hydroxide deposit at thecathode (reaction 20). 
NO3- + H2O + 2 e- 6 NO2
- + 2 OH- 
Mn+ + n OH- 6 M(OH)n (M = metal)
Under suitable conditions, either already during the deposition or during post-depositionannealing, the hydroxide decomposes to the corresponding oxide:
M(OH)n 6 MOn/2 + n/2 H2O 
In the present experiments, the current flow started at less negative potentials when the Zn(NO3)2
solution contained also Al(NO3)3 or InCl3 as compared with the solution containing onlyZn(NO3)2. This suggests that the electrochemically generated hydroxide ions react more easilywith the Al3+ or In3+ ions than with the Zn2+ ions. This idea was supported by film compositions(Fig. 11). In the Zn-Al-O films, aluminum is the main metal in the deposit formed at low cathodicpotentials (more positive than -0.9 V). At more negative potentials, the amount of Zn in thedeposit increases and that of Al decreases. Between -1.0 and -1.6 V the Al/(Zn+Al) ratio in thefilms was 0.042 to 0.17 corresponding to 2-8 at.% Al concentration in ZnO which has generallybeen found suitable doping level. The Zn-In-O films behaved similarly: the films deposited atlow cathodic potentials consisted mainly of indium oxide or hydroxide, and In doped ZnO wasformed at more negative potentials. The In/(Zn+In) ratio in the films was 0.02 to 0.1 between -1.0and -1.2 V, corresponding to doping concentration of 1 to 5 at.%. These results are in anagreement with the fact that aluminum hydroxide and indium hydroxide are thermodynamicallymore stable than zinc hydroxide .
-1.8 -1.6 -1.4 -1.2 -1.0 -0.8 -0.6
Deposition potential (V) vs. Ag/AgCl
Figure 11. Relative metal ratios of Al doped ZnO films as a function of the deposition potential.Deposition solution contained 0.05 M Zn(NO3)2 and 0.001 M Al(NO3)3.
The situation for the ZnO:In films was somewhat more complicated since the amount of In in thedeposit started to increase again at even more negative potentials. This may be attributed to the
formation of ZnmIn2O3+m (m = 1,2,3,...) compounds that are known to exist in the ZnO-In2O3
system [271, 272]. All the XRD reflections measured from these films could, however, beidentified with those of the wurtzite ZnO . It is of course possible that part of the depositis in amorphous form. The increasing amount of In at the negative potentials was not observedwith lower InCl3 concentrations which suggests that the formation of ZnmIn2O3+m compounds isfeasible only when the amount of the In precursor in the solution is high enough.
The films where the main cation was Zn were crystalline as deposited, showing the characteristicZnO (wurtzite) XRD reflections  with a preferred (002) orientation (Fig. 12), as observedoften with electrodeposited ZnO films [248, 262] . The orientation was not affected by doping.Most of the films where the main cation was In, i.e. those deposited at potentials more positivethan -0.8 V, showed the reflection of In(OH)3 . No reflections were detected from the filmswhere the main cation was Al.
20 30 40 50 60 70 80
Zn(NO3)2 0.05 M and InCl3 0.005 M
Zn(NO3)2 0.05 M and InCl3 0.001 M
Zn(NO3)2 0.05 M and InCl3 0.0005 M
2 θ / o
Figure 12. XRD patterns of In doped ZnO films deposited on Mo at -0.9 V vs. Ag/AgCl with differentInCl3 concentrations.
7.4. Solar cells
The electrodeposited CIS films were used for the preparation of solar cells. The CIS films wereannealed and etched prior to the solar cell preparation as described in Chapter 6.5. Some deviceswere prepared using the CIS+In2Se3 bilayer films that were not etched. The CdS films wereprepared by chemical bath deposition. Three different preparation methods for the ZnO filmswere compared: electrodeposition, ALD, and sputtering. Superstrate structures were prepared toobut no photoresponses could be measured for them. This was probably due to the too high carrierconcentrations of the unetched CIS films (see Chapter 7.2.4).
7.4.1. Solar cells with electrodeposited ZnO
The rectification ratios of the solar cells with electrodeposited ZnO films were quite good, thatis, the devices clearly behaved as pn-junction diodes. The best rectification ratios were obtainedwith structures containing a thin (100 nm) undoped ZnO film between CIS and the doped ZnOfilm. In spite of the good diode behavior in the dark, the photoresponses measured for thesedevices were very weak. This is at least partly due to that the illumination had to be done througha thin Al film which was required for the front contacts because of the very low conductivity ofthe electrodeposited ZnO films.
Indium doped ZnO films resulted generally in higher forward currents and photoresponses thanthe aluminum doped films. This is in agreement with results obtained with spray pyrolysed films where the properties of the In doped ZnO films were found to be better than those of theAl doped films. This may be due to a more optimal doping concentration and thus betterconductivity of the In doped films, or to small differences in the structure or crystallinity of theIn and Al doped films.
Figure 13 shows current-voltage characteristics of two solar cell structures withelectrochemically prepared In or Al doped ZnO films, both measured in the dark. Nophotoresponses at all could be detected from structures that were prepared without CdS.
-1 .0 -0 .5 0 .0 0 .5 1 .0
j / m
V / V o lts
Figure 13. Dark I-V curves for two solar cell structures with electrodeposited ZnO films. Solid line:Mo/CIS/CdS/i-ZnO/ZnO:Al, dotted line: Mo/CIS/CdS/i-ZnO/ZnO:In.
The best open circuit voltage value, measured under 50 W halogen lamp illumination, was 0.405V, obtained for a Mo/CIS/CdS/ZnO:Al structure, where the ZnO:Al film was deposited at -1.1
V from 0.05 M Zn(NO3)2 and 0.001 M Al(NO3)3. Typical VOC values varied between 0.1 V and0.25 V. The short circuit current densities and the Pmax values were generally very low. Thevalues measured for the device with the best VOC value were 0.13 mA cm-2 and 0.015 mW cm-2,respectively, but the FF was 0.34 which is the best value obtained for the structures withelectrodeposited ZnO films. FF was typically about 0.25.
The highest short circuit current density was 8.65 mA cm-2, measured from a Mo/CIS/CdS/i-ZnO/ZnO:In structure where the ZnO:In film was deposited at -1.2 V from 0.05 M Zn(NO3)2 and0.005 M InCl3. The same device also yielded the highest Pmax value, 0.12 mW cm-2.
7.4.2. Solar cells with ALD-ZnO
The short circuit current densities for the devices with ALD-ZnO films were higher than for thosewith electrodeposited ZnO films. Typical values were between 2 and 4 mA cm-2. This is probablydue to the higher transparency and better conductivity of the ALD-ZnO films. Consequently, thePmax values were also higher than with the electrodeposited ZnO films. The open circuit voltagesand fill factors were similar to those obtained with electrodeposited ZnO films. Figure 14 showsa typical example of current-voltage characteristics for a device with ALD-ZnO, measured in thedark and under illumination.
-0.6 -0.4 -0.2 0.0 0.2 0.4 0.6
VOC = 0.18 V jSC = 3.77 mA cm -2
Pmax = 0.22 mW cm -2 FF = 0.32
j / m
V / Volts
Figure 14. Dark (solid line) and illuminated (dotted line) I-V curves of a device with ALD-ZnO film
The best photoresponse was measured from a Mo/CIS/CdS/i-ZnO/ZnO:Al structure with a thick(about 150 nm) CdS. The VOC, jSC, Pmax and FF for this device were 0.21 V, 5.47 mA cm-2, 0.34mW cm-2 and 0.30, respectively. The fact that the best response was obtained from a device with
a thick CdS film is probably a result of the low resistivity of the undoped ZnO layer (2-4x10-2
Ωcm). Because of this low resistivity, a thick CdS film was needed to prevent shunting betweenCIS and ZnO. This conclusion is further supported by the poor (short circuited) current-voltagecharacteristics obtained with devices without CdS.
7.4.3. Solar cells with sputtered ZnO
The solar cells with the sputtered ZnO films were prepared in cooperation either with EcoleNationale Supérieure de Chimie de Paris, or with the Hahn-Meitner-Institut (HMI) in Berlin. Inboth cases, the electrodeposited CIS films were prepared in Helsinki, and the ZnO bilayers wereprepared and the I-V measurements were made in Paris or in Berlin using light sources calibratedto give light intensity of 100 mW cm-2.
The results obtained from Paris were not markedly better than those obtained in our laboratorywith ALD-ZnO films. This may be due to the prolonged air-exposure of the Mo/CIS/CdSstructures before the cell completion. On the other hand, similar results were obtained also forMo/CIS samples that were annealed, etched and covered with CdS in Paris, just before the ZnOsputtering. The best open circuit voltage was 0.195 V, and the values were in general a bit lowerthan those measured from devices with ALD-ZnO. The short circuit current densities, in contrast,were similar to those measured from the devices with ALD-ZnO. The best value was 5 mA cm-2.Often a sample with high VOC yielded a low jSC and vice versa, for example, 0.195 V and 0.5 mAcm-2, and 0.035 V and 5 mA cm-2.
The best results were obtained from the glass/Mo/CIS samples completed in Berlin. The annealedCIS samples were CN--etched prior to the deposition of the CdS buffer and the ZnO bilayer bythe standard processes of HMI. The photoresponses were measured under standard AM1.5illumination and the best solar cell efficiency was 1.3 %. The VOC, jSC, FF, and Pmax of this samplewere 0.32 V, 10 mA cm-2, 0.39, and 1.3 mW cm-2, respectively. Even though the conversionefficiency is low compared to the highest values measured for electrodeposited CIS absorbers,about 5-7 % [42, 164, 169, 218], it demostrates that the electrodeposited CIS films can inprinciple be used in solar cells. Figure 15 shows I-V curves of two different devices withsputtered ZnO bilayers, measured under AM 1.5 illumination in Berlin. The difference betweenthe results obtained from Paris and from Berlin might be due to the two different CdS depositionprocesses.
-0 .6 -0 .4 -0 .2 0 .0 0 .2 0 .4 0 .6 0 .8-4 0-2 0
02 04 06 08 0
1 0 0
V O C 0 .3 1 V
jS C 5 .5 2 m A c m -2
F F 0 .3 2
η 0 .5 5 %
V O C 0 .3 2 V
jS C 1 0 .3 m A c m -2
F F 0 .3 9
η 1 .3 %j /
V / V o lts
Figure 15. I-V curves of two different devices with sputtered ZnO films, measured under AM 1.5illumination at HMI in Berlin. The solid line corresponds to a device where the CIS thickness was about0.5 µm whereas the dotted line corresponds to one with a thickness of about 1 µm.
Devices with electrodeposited CIS absorbers have generally shown VOC values between 0.33 and0.39 V, jSC values between 25 and 42 mA cm-2, and FF values of about 0.52-0.59, respectively[42, 164, 169, 218]. On the other hand, the 1.5 % efficient device of Sudo et al.  showed ahigh short circuit current density of 31.5 mA cm-2 in combination with a very low open circuitvoltage of 0.188 V. Low short circuit current densities in combination with low open circuitvoltages are not uncommon either for devices with electrodeposited CIS absorbers. For instance,the preliminary devices of Garg et al.  and Sahu et al.  showed jSC and VOC values ofless than 1 mA cm-2 and 0.188 V, respectively, and 0.056 mA cm-2 and 0.165 V, respectively.
Thus the VOC values measured in this study were comparable to or higher than those measuredfor other electrodeposited devices [42, 161, 163, 164, 166, 169, 218]. The main differencebetween the devices prepared in this study and the most efficient devices with electrodepositedCIS absorbers was that the short circuit current densities measured in this study wereconsiderably lower.
The results indicated that the main reason for the poor solar cell performance was undoubtedlythe insufficient quality of the CIS films, resulting partly from the too high carrier concentrationseven after etching. In addition, the CIS films were probably porous which may result from theescape of impurities during the annealing. Also the CN- etching may have caused pinholes. TheCIS films (thickness about 500 nm) used in these studies might also have been too thin forefficient light absorption. However, the results from thicker films were in general even worse –possibly because of incomplete removal of copper selenide from the thicker film.
Yet another problem might be the interface between Mo and CIS. The presence of a MoSe2
interlayer improves the adhesion between Mo and CIS . This layer has even been suggestedto be the prerequisite for the formation of a proper ohmic contact [39, 41]. The formation ofMoSe2 occurs under In- and Se-rich conditions at high temperatures [39, 40] and thus it is veryunlikely to be present in the samples studied in this work. In any case, the quality of the Mo backcontact is known to have a strong effect on the quality of electrodeposited CIS films .Further, the thickness of the Mo films may also have an effect: the Mo films used in these studieswere only 100 nm thick whereas usually about 1 µm thick films are used.
CuInSe2 and related chalcopyrite compounds are the most promising absorber materials forpolycrystalline thin film solar cells. CuInSe2 solar cells have shown the highest conversionefficiencies of all thin film solar cells. The record efficiency is 18.8 %, and several groups haveachieved efficiencies over 18 %. Further, the operational lifetimes of this type of solar cells arelong due to their extraordinary stability. CuInSe2 thin films can be prepared both from gas andliquid phases by a variety of methods, but the highest efficiencies have so far been obtained byabsorbers prepared by co-evaporation. In order to lower the production costs of photovoltaicmodules, alternative, low-cost deposition methods need to be developed. Electrodeposition is onealternative since it is a low-temperature liquid phase deposition method. The depositionequipment is relatively simple, and the advantages of the method include the potential forupscaling to large substrate areas and production volumes.
Electrodeposited CIS-based absorber films require generally annealing either under a Se-containing or an inert atmosphere prior to the cell preparation. Such approaches have resulted inconversion efficiencies between about 5 and 7 %. Even higher efficiencies, over 15.4 %, can beachieved if the stoichiometry of the electrodeposited precursor film is adjusted by adding In, Gaand Se by PVD prior to the cell preparation.
CIS-based films have been prepared by a variety of electrochemical techniques such as one-stepdeposition, sequential deposition of binary compounds, and deposition of elemental layersfollowed by annealing either under an inert or a reactive atmosphere. One-step electrodepositionis the most widely studied option. There are basically two alternative ways to control the filmcomposition: either by balancing the diffusion fluxes of the constituent ions to the cathode, or byrelying on thermodynamics. In the former case, the film composition is heavily dependent on thedeposition potential and on the concentrations in the deposition solution. Small, unavoidablevariations in concentrations and deposition potentials may therefore result in large changes in thefilm compositions which deteriorates reproducibility and may render upscaling to larger substrateareas problematic.
The latter option, in turn, utilizes induced co-deposition that has been used widely for binarycompounds, especially CdTe. In a binary system, the deposition of the more noble ion inducesthe underpotential reduction of the less noble ion and the formation of the compound at lessnegative potentials than where the less noble ion would reduce on its own. The reason for theunderpotential reduction of the less noble ion is the energy released in the compound formation.When the deposition solution contains a large excess of the less noble ion, induced co-depositionensures the formation of stoichiometric compound over wide concentration and potential ranges.These kind of processes are thus much less sensitive to electrolyte composition and depositionpotential than those based on the flux balance approach.
Despite its success in deposition of binary compounds, induced co-deposition had not beenutilized for the deposition of ternary compound semiconductors prior to this work. In the case ofCIS, this is partly because the formation of CIS occurs via Cu2-xSe, and the latter does not followthe induced mechanism. In the present work, suitable conditions for the induced co-depositionof Cu2-xSe and CuInSe2 were achieved by complexing the Cu+ ions by thiocyanate ions in orderto shift the reduction potential of metallic Cu to the negative direction. Under these conditions,Se reduced first, i.e., at more positive potentials than Cu. The reduction of Se induced theformation of Cu2-xSe at more positive potentials than where the bulk deposition of metallic Cubegan. Cu2-xSe, in turn, induced the formation of CuInSe2 at the same potential range, i.e., at morepositive potentials than where the deposition of metallic Cu or In began. The electrochemistryof the Cu-Se and Cu-In-Se systems was studied by cyclic voltammetry and electrochemicalquartz crystal microbalance measurements that verified the deposition mechanisms. Induced co-deposition allowed wide potential and concentration ranges for the formation of almoststoichiometric CuInSe2 films (Cu1.30In1.00Se2.20 according to RBS) as long as the concentrationsof the metal precursors were much higher than that of the selenium precursor, and theconcentration of the SCN- ions was high enough to keep all the Cu+ ions as [Cu(SCN)4]3- so thatthere were no free Cu+ ions in the solution.
The films were studied by a number of techniques: XRD, SEM, EDX, RBS, TOF-ERDA,photoelectrochemical and capacitance-voltage measurements. The as-deposited films wereamorphous and contained hydrogen, oxygen, sulfur, carbon, and nitrogen as impurities. Hydrogenand oxygen originated apparently from the aqueous deposition solution and the other impuritiesfrom the thiocyanate ligands. The films became crystalline upon annealing that also reduced theimpurity contents drastically. The relative amounts of Cu, In, and Se in the films remainedessentially the same after annealing.
Since photovoltaic-quality CIS films should be Cu-deficient rather than Cu-rich like the filmsdeposited in this study, two approaches were made to adjust the film compositions afterdeposition: etching in KCN solutions and addition of In2Se3. The effects of the post-depositiontreatments on the film properties were studied by EDX, photoelectrochemical and capacitancemeasurements that verified more stoichiometric composition and more suitable carrierconcentrations after the post-deposition treatments. However, the carrier concentration was stillmuch higher than those measured for high-efficiency absorbers.
Solar cells were prepared from films deposited and treated under the conditions bound to givethe highest photoactivities and lowest carrier concentrations. Doped ZnO films for the deviceswere prepared either electrochemically, by ALD, or by sputtering. For the first time, Al and Indoped ZnO films were prepared by electrodeposition. The electrodeposited ZnO films wereprepared from solutions containing Zn(NO3)2 and Al(NO3)3 or InCl3. The films were crystallineas deposited but did not result in good photoresponses due to their high resistivity. The current-
voltage characteristics measured in the dark showed, however, good rectifying behavior. Thiswas also the first time when electrodeposited ZnO:Al and ZnO:In films were used as frontelectrodes in solar cells.
The photoresponses with the ALD-ZnO films were better than with the electrodeposited ZnOfilms. Yet, the best photoresponses were obtained from the devices with sputtered ZnO bilayers,prepared at HMI Berlin. The highest conversion efficiency, measured under AM 1.5 illumination,was 1.3 %. Although the efficiency was low, the open circuit voltages of these devices werecomparable to those of higher efficiency devices with electrodeposited CIS absorbers.
 Suntola, T., in Proceedings of the PV CON ‘95, Kruger, South Africa, 1995. Solar Cells and Their Applications, Edited by L.D. Partain, John Wiley & Sons, Inc., N.Y.,1995. 600 p.  Bahaj, A.S., Renew. Energy, 27 (2002) 097-105.  Stone, J. L., Phys. Today, September 1993 22-29.  Contreras, M. A., Egaas, B., Ramanathan, K., Hiltner, J., Swartzlander, A., Hasoon, F., andNoufi, R., Prog. Photovolt.: Res. Appl., 7 (1999) 311-316.  Kröger, F. A., J. Electrochem. Soc., 125 (1978) 2028-2034.  Panicker, M.P.R., Knaster, M., and Kröger, F.A., J. Electrochem. Soc., 125 (1978) 566-572. Shah, A., Torres, P., Tscharner, R., Wyrsch, N. and Keppner, H., Science, 285 (1999) 692-698. Tsubomura, H., and Kobayashi, H., Crit. Rev. Solid State Mater. Sci., 18 (1993) 261-326. ASTM E927-91. Standard specification for solar simulation for terrestrial photovoltaictesting. ASTM G159-98. Standard tables for references solar spectral irradiance at air mass 1.5:Direct normal and hemispherical for a 37 E tilted surface (E891 & E892). Chapin, D.M., Fuller, C.S., and Pearson, G.L., J. Appl. Phys., 25 (1954) 676-677.  Goetzberger, A., and Hebling, C., Sol. Energy Mater. Sol. Cells, 62 (2000) 1-19.  Birkmire, R.W., Sol. Energy Mater. Sol. Cells, 65 (2001) 17-28.  Goetzberger, A., Luther, J., and Willeke, G., Sol. Energy Mater. Sol. Cells, 74 (2002) 1-11. Schock, H.-W., and Noufi, R., Prog. Photovolt.: Res. Appl., 8 (2000) 151-160.  Kojima, T., Koyanagi, T., Nakamura, K., Yanagisawa, T., Takahisa, K., Nishitani, M., andWada, T., Sol. Energy Mater. Sol. Cells, 50 (1998) 87-95.  Green, M.A., Emery, K., King, D.L., Igari, S., and Warta, W., Prog. Photovolt.: Res. Appl.,9 (2002) 55-61.  Powder Diffraction Files, Card 40-1487, International Centre for Diffraction Data,Pennsylvania, PA Powder Diffraction Files, Card 23-0207, International Centre for Diffraction Data,Pennsylvania, PA  Fthenakis, V. M., Morris, S. C., Moskowitz, P. D., and Morgan, D. L., Prog. Photovolt.:Res. Appl., 7 (1999) 489-497 and references cited therein. Siebentritt, S., Thin Solid Films, 403-404 (2002) 1-8.  Schmid, D., Ruckh, M., Grunwald, F., and Schock, H.W., J. Appl. Phys., 73 (1993) 2902-2909. Birkmire, R.W., and Eser, E., Annu. Rev. Mater. Sci., 27 (1997) 625-653.  Klenk, R., Thin Solid Films, 387 (2001) 135-140. Kwon, S.H., Park, S.C., Ahn, B.T., Yoon, K.H., and Song, J., Sol. Energy, 64 (1998) 55-60.
 Negami, T., Kohara, N., Nishitani, M., Wada, T., and Hirao, T., Appl. Phys. Lett., 67 (1995)825-827. Zhang, S.B., Wei, S.-H., Zunger, A., and Katayama-Yoshida, H., Phys. Rev. B, 57 (1998)9642-9656. Schock, H.W., and Rau, U., Physica B, 308-310 (2001) 1081-1085.  Zhang, S.B., Wei, S.-H., and Zunger, A., J. Appl. Phys., 83 (1998) 3192-3196.  Rau, U., Jasenek, A., Schock, H.W., Engelhardt, F., and Meyer, Th., Thin Solid Films, 361-362 (2000) 298-302.  Rau, U., Schmidt, M., Jasenek, A., Hanna, G., and Schock, H.W., Sol. Energy Mater. Sol.Cells, 67 (2001) 137-143.  Turcu, M., Pakma, O., and Rau, U., Appl. Phys. Lett., 80 (2002) 2598-2600. Shafarman, W.N., Klenk, R., and McCandless, B.E., J. Appl. Phys., 79 (1996) 7324-7328. Hanna, G., Jasenek, A., Rau, U., and Schock, H.W., Thin Solid Films, 387 (2001) 71-73.  Contreras, M.A., Tuttle, J., Gabor, A., Tennant, A., Ramanathan, K., Asher, S., Franz, A.,Keane, J., Wang, L., Scofield, J., and Noufi, R., in Proc. 1st World Conf. Photovolt. EnergyConv., Waikoloa, Hawaii (1994) p. 68-75. Dullweber, T., Lundberg, O., Malmström, J., Bodegård, M., Stolt, L., Rau, U., Schock,H.W., and Werner, J.H., Thin Solid Films, 387 (2001) 11-13.  Dullweber, T., Hanna, G., Shams-Kolahi, W., Schwartzlander, A., Contreras, M.A., Noufi,R., Schock, H. W., Thin Solid Films, 361-362 (2000) 478-481.  Wada, T., Kohara, N., Nishiwaki, S., and Negami, T., Thin Solid Films, 387 (2001) 118-122. Guillemoles, J.F., Kronik, L., Cahen, D., Rau, U., Jasenek, A., and Schock, H.-W., J. Phys.Chem. B, 104 (2000) 4849-4862.  Schmid, D., Ruckh, M., and Schock, H.W., Sol. Energy Mater. Sol. Cells, 41/42 (1996) 281-294. Guillemoles, J.-F., Cowache, P., Lusson, A., Fezzaa, K., Boisivon, F., Vedel, J., and Lincot,D. J. Appl. Phys., 79 (1996) 7293-7302. Schwartz, R.J., and Gray, J.L., Proc. 21st IEEE Photovolt. Spec. Conf., Kissimmee, FL, USA(1990) p. 570-574. Heske, C., Eich, D., Fink, R.,Umbach, E., van Buuren, T., Bostedt, C., Terminello, L.J.,Kakar, S., Grush, M.M., Callcott, T.A., Himpsel, F.J., Ederer, D.L., Perera, R.C.C., Riedl, W.,and Karg, F., Appl. Phys. Lett., 74 (1999) 1451-1453.  Nakada, T., and Kunioka, A., Appl. Phys. Lett., 74 (1999) 2444-2446.  Nakada, T., Kume, T., Mise, T., and Kunioka, A., Jpn. J. Appl. Phys., 37 (1998) L499-L501. Haug, F.-J., Rudmann, D., Bilger, G., Zogg, H., and Tiwari, A.N., Thin Solid Films, 403-404(2002) 293-296. Tringe, J., Nocerino, J., Tallon, R., Kemp, W., Shafarman, W., and Marvin, D., J. Appl.Phys., 91 (2002) 516-518. Jasenek, A., Rau, U., Weinert, K., Kötschau, I.M., Hanna, G., Voorwinden, G., Powalla, M.,Schock, H.W., and Werner, J.H., Thin Solid Films, 387 (2001) 228-230.
 Jasenek, A., and Rau, U., J. Appl. Phys., 90 (2001) 650-658. Yamaguchi, M., J. Appl. Phys., 78 (1995) 1476-1480. Kawakita, S., Imaizumi, M., Yamaguchi, M., Kushiya, K., Ohshima, T., Itoh, H., andMatsuda, S., Jpn. J. Appl. Phys., Part 2, 41 (2002) L797-799. Boden, A., Bräunig, D., Klaer, J., Karg, F.H., Hosselbarth, B., La Roche, G., in Proc. 28th
IEEE Photovolt. Spec. Conf., Anchorage, AK, USA (2000) p. 1038 -1041. Zabierowski, P., Rau, U., and Igalson, M., Thin Solid Films, 387 (2001) 147-150.  Köntges, M., Reineke-Koch, R., Nollet, P., Beier, J., Schäffler, R., and Parisi, J., Thin SolidFilms, 403-404 (2002) 280-286. Guillemoles, J.-F., Rau, U., Kronik, L., Schock, H.-W. and Cahen, D., Adv. Mater., 11(1999) 957-961. Hedström, J., Ohlsen, H., Bodegård, M., Kylner, A., Stolt, L., Hariskos, D., Ruckh, M., andSchock, H.-W., in Proc. 23rd IEEE Photovolt. Spec. Conf., Louisville, KY, USA (1993) p. 364-371.  Stolt, L., Hedström, J., Kessler, J., Ruckh, M., Velthaus, K-O., and Schock, H.-W., Appl.Phys. Lett., 62 (1993) 597-599.  Granath, K., Bodegård, M., and Stolt, L., Sol. Energy Mater. Sol. Cells, 60 (2000) 279-293. Bodegård, M., Granath, K. and Stolt, L., Thin Solid Films, 361-362 (2000) 9-16.  Lammer, M., Klemm, U., and Powalla, M., Thin Solid Films, 387 (2001) 33-36.  Contreras, M.A., Egaas, B., Dippo, P., Webb, J., Granata, J., Ramanathan, K., Asher, S.,Swartzlander, A., and Noufi, R., in Proc. 26th IEEE Photovolt. Spec. Conf., Anaheim, CA, USA(1997) p. 359-362.  Keyes, B.M., Hasoon, F., Dippo, P., Balcioglu, A., and Abulfotuh, F., in Proc. 26th IEEEPhotovolt. Spec. Conf., Anaheim, CA, USA (1997) p. 479-482.  Nakada, T., Iga, D., Ohbo, H., and Kunioka, A., Jpn. J. Appl. Phys., 36 (1997) 732-737.  Granata, J.E., Sites, J.R., Asher, S., and Matson, J., in Proc. 26th IEEE Photovolt. Spec.Conf., Anaheim, CA, USA (1997) p. 387-390.  Braunger, D., Hariskos, D., Bilger, G., Rau, U., Schock, H.W., Thin Solid Films, 361-362(2000) 161-166.  Heske, C., Eich, D., Fink, R., Umbach, E., Kakar, S., van Buuren, T., Bostedt, C.,Terminello, L.J., Grush, M.M., Callcott, T.A., Himpsel, F.J., Ederer, D.L., Perera, R.C.C., Riedl,W., and Karg, F., Appl. Phys. Lett., 75 (1999) 2082-2084.  Rau, U., and Schock, H.W., Appl. Phys. A: Mater. Sci. Process., 69 (1999) 131-147.  Niles, D., W., Ramanathan, K., Hasoon, F., Noufi, R., Tielsch, B.J., and Fulghum, J.E., J.Vac. Sci. Technol., A 15 (1997) 3044-3049.  Rockett, A., Britt, J.S., Gillespie, T., Marshall, C., Al Jassim, M.M., Hasoon, F., Matson,R., and Başol, B., Thin Solid Films, 372 (2000) 212-217.  Kimura, R., Nakada, T., Fons, P., Yamada, A., Niki, S., Matsuzawa, T., Takahashi, K., andKunioka, A., Sol. Energy Mater. Sol. Cells, 67 (2001) 289-295.  Wei, S.-H., Zhang, S.B., and Zunger, A., J. Appl. Phys., 85 (1999) 7214-7218.
 Rockett, A., Granath, K., Asher, S., Al Jassim, M.M., Hasoon, F., Matson, R., Başol, B.,Kapur, V., Britt, J.S., Gillespie, T., and Marshall, C., Sol. Energy Mater. Sol. Cells., 59 (1999)255-264.  Ruckh, M., Scmid, D., Kaiser, M., Schäffler, R., Walter, T., and Schock, H.W., in Proc. 1st
World Conf. Photovolt. Energy Conv., Waikoloa, Hawaii (1994) p. 156-159.  Kronik, L., Cahen, D., and Schock, H.W., Adv. Mater., 10 (1998) 31-36.  Cahen, D., and Noufi, R., Appl. Phys. Lett., 54 (1989) 558-560.  Kronik, L., Rau, U., Guillemoles, J.-F., Braunger, D., Schock, H.W., and Cahen, D., ThinSolid Films, 361-362 (2000) 353-359.  Rau, U., Braunger, D., Herberholz, R., Schock, H.W., Guillemoles, J.-F., Kronik, L., andCahen, D., J. Appl. Phys., 86 (1999) 497-505.  Caballero, R., and Guillén, C., Thin Solid Films, 403-404 (2002) 107-111.  Marudachalam, M., Hichri, H., Klenk, R., Birkmire, R.W., Shafarman, W.N., and Schultz,J.M., Appl. Phys. Lett., 67 (1995) 3978-3980.  Klenk, M., Schenker, O., Alberts, V., and Bucher, E., Semicond. Sci. Technol., 17 (2002)435-439.  Devaney, W.E., Chen, W.S., Stewart, J.M., and Mickelsen, R.A., IEEE Trans. ElectronDev., 37 (1990) 428-433.  Gabor, A.M., Tuttle, J.R., Albin, D.S., Contreras, M.A., and Noufi, R., Appl. Phys. Lett., 65(1994) 198-200.  Negami, T., Hashimoto, Y., and Nishiwaki, S., Sol. Energy Mater. Sol. Cells, 67 (2001) 331-335.  Hagiwara, Y., Nakada, T., and Kunioka, A., Sol. Energy Mater. Sol. Cells, 67 (2001) 267-271.  Chaisitsak, S, Yamada, A., and Konagai, M., Jpn. J. Appl. Phys., 41 (2002) 507-513.  Nakada, T., and Mizutani, M., Jpn. J. Appl. Phys., 41 (2002) L165-L167.  Contreras, M.A., Egaas, B., King, D., Schwartzlander, A., and Dullweber, T., Thin SolidFilms, 361-362 (2000) 167-171.  Contreras, M.A., Jones, K. M., Gedvilas, L., and Matson, R., Proc. 16th Eur. Photovolt.Solar Energy Conf., Glasgow, UK (James & James, London, 2001), p. 732-735. Shafarman, W.N., and Zhu, J., Thin Solid Films, 361-362 (2000) 473-477.  Niki, S., Yamada, A., Hunger, R., Fons, P.J., Iwata, K., Matsubara, K., Nishio, A., andNakanishi, H., J. Cryst. Growth, 237-240 (2002) 1993-1999.  Tiwari, A.N., Blunier, S., Kessler, K., Zelezny, V., and Zogg, H., Appl. Phys. Lett., 65(1994) 2299-2301.  Hermann, A.M., Gonzalez, C., Ramakrishnan, P.A., Balzar, D., Popa, N., Rice, B., Marshall,C.H., Hilfiker, J.N., Tiwald, T., Sebastian, P.J., Calixto, M.E., and Bhattacharya, R.N., Sol.Energy Mater. Sol. Cells, 70 (2001) 345-361.  Negami, T., Satoh, T., Hashimoto, Y., Shimakawa, S., Hayashi, S., Muro, M., Inoue, H., andKitagawa, M., Thin Solid Films, 403-404 (2002) 197-203.
 Powalla, M., and Dimmler, B., Thin Solid Films, 361-362 (2000) 540-546.  Dimmler, B., Gross, E., Menner, R., Powalla, M., Hariskos, D., Ruckh, M, Rühle, U., andSchock, H.W., in Proc. 25th IEEE Photovolt. Spec. Conf., Washington, D.C., USA (1996) p. 757-762.  Knapp, K., and Jester, T., Sol. Energy, 71 (2001) 165-172. Zank, J., Mehlin, M., and Fritz, H.P., Thin Solid Films, 286 (1996) 259-263.  Ramakrishna Reddy, K.T., Datta, P.K., and Carter, M.J., Phys. Stat. Sol. (a), 182 (2000) 679-685.  Adurodija, F. O., Song, J., Kim, S. D., Kwon, S. H., Kim, S. K., Yoon, K. H. and Ahn, B.T., Thin Solid Films, 338 (1999) 13-19.  Marudachalam, M., Birkmire, R.W., Hichri, H., Schultz, J.M., Swartzlander, A., and Al-Jassim, M.M., J. Appl. Phys., 82 (1997) 2896-2905.  Guillén, C., Martínez, M.A., and Herrero, J., Vacuum, 58 (2000) 594-601.  Yüksel, Ö.F., Başol, B.M., Safak, H., and Karabiyik, H., Appl. Phys. A, 73 (2001) 387-389. Chowles, A.G., Neethling, J.H., van Niekerk, H., Engelbrecht, J.A.A., and Watters, V.J.,Renew. Energy, 6 (1995) 613-618.  Bandyopadhyaya, S., Roy, S., Chaudhuri, S., and Pal, A.K., Vacuum, 62 (2001) 61-73.  Guillén, C., and Herrero, J., Sol. Energy Mater. Sol. Cells, 73 (2002) 141-149.  Sadigov, M.S., Özkan, M., Bakacsiz, E., Altunbaş, M., and Kopya, A.I., J. Mater. Sci., 34(1999) 4579-4584.  Chu, T.L., Chu, S.S., Lin, S.C. and Yue, J., J. Electrochem. Soc., 131 (1984) 2182-2185. Bekker, J., Alberts, V., and Witcomb, M.J., Thin Solid Films, 387 (2001) 40-43.  Chichibu, S.F., Sugiyama, M., Ohbasami, M., Hayakawa, A., Mizutani, T., Nakanishi, H.,Negami, T., and Wada, T., J. Cryst. Growth, 243 (2002) 404-409.  A. Garg, K.S. Balakrisnan and A.C. Rastogi, J. Electrochem. Soc. 141 (1994) 1566-1572. Rastogi, A.C., Balakrisnan, K.S., Sharma, R.K. and Jain, K., Thin Solid Films, 357 (1999)179-188.  Guillén, C., and Herrero, J., Thin Solid Films, 323 (1998) 93-98. Alberts, V., Klenk, M., and Bucher, E., Thin Solid Films, 387 (2001) 44-46.  Calixto, M.E., and Sebastian, P.J., J. Mater. Sci., 33 (1998) 339-345. Hodes, G., Engelhardt, T., Cahen , D., Kazmerski, L.L., and Herrington, C.R., Thin SolidFilms, 128 (1985) 93-106.  Kumar, S.R., Gore, R.B., and Pandey, R.K., Thin Solid Films, 223 (1993) 109-113.  Fritz, H.P. and Chatziagorastou, P., Thin Solid Films, 247 (1994) 129-133.  Kapur, V.K., Başol, B.M., and Tseng, E.S., Sol. Cells, 21 (1987) 65-72.  Prosini, P.P., Addonizio, M.L., Antonaia A. and Loreti, S. Thin Solid Films, 288 (1996) 90-94.  Altosaar, M., Mellikov, E., Kois, J., Guo, Y. and Meissner, D., in Proceedings of JointInternational Meeting of The Electrochemical Society, Inc. and The International Society ofElectrochemistry, Paris, France (1997) p. 1314-1315
 Lokhande, C.D., Bull. Electrochem., 4 (1988) 131-136.  Probst, V., Stetter, W., Riedl, W., Vogt, H., Wendl, M., Calwer, H., Zweigart, S., Ufert, K.-D., Freienstein, B., Cerva, H., and Karg, F., Thin Solid Films, 387 (2001) 262-267.  Kushiya, K., Thin Solid Films, 387 (2001) 257-261.  Kushiya, K., Tachiyuki, M., Nagoya, Y., Fujimaki, A., Sang, B., Okumura, D., Satoh, M.,and Yamase, O., Sol. Energy Mater. Sol. Cells, 67 (2001) 11-20.  Karg, F.H., Sol. Energy Mater. Sol. Cells, 66 (2001) 645-653.  Wada, T., Hashimoto, Y., Nishiwaki, S., Satoh, T., Hayashi, S., Negami, T., and Miyake,H., Sol. Energy Mater. Sol. Cells, 67 (2001) 305-310. Başol, B.M., Halani, A., Leidholm, C., Norsworthy, G., Kapur, V.K., Swartzlander, A., andMatson, R., Prog. Photovolt.: Res. Appl., 8 (2000) 227-235.  Keränen, J., Lu, J., Barnard, J., Sterner, J., Kessler, J., Stolt, L., Matthes, Th.W., andOlsson, E., Thin Solid Films, 387 (2001) 80-82.  Gillespie, T.J., Marshall, C.H., Contreras, M., and Keane, J., Sol. Energy Mater. Sol. Cells,59 (1999) 27-34.  Hermann, A.M., Mansour, M., Badri, V., Pinkhasov, B., Gonzales, C., Fickett, F., Calixto,M.E., Sebastian, P.J., Marshall, C.H., and Gillespie, T.J., Thin Solid Films, 361-362 (2000) 74-78.  Hermann, A.M., Gonzalez, C., Ramakrishnan, P.A., Balzar, D., Marshall, C.H., Hilfiker,J.N., and Tiwald, T., Thin Solid Films, 387 (2001) 54-56.  Park, S.C., Lee, D.Y., Ahn, B.T., Yoon, K.H., and Song, J., Sol. Energy Mater. Sol. Cells,69 (2001) 99-105.  Lee, D.Y., Yun, J.H., Ahn, B.T., Yoon, K.H., and Song, J., Mater. Res. Soc. Symp. Proc.,668 (2001) H8.8.1-6.  Ashida, A., Hachiuma, Y., Yamamoto, N., Ito, T., and Cho, Y., J. Mater. Sci. Lett., 13(1994) 1181-1184.  Klenk, M., Schenker, O., Alberts, V., and Bucher, E., Thin Solid Films, 387 (2001) 47-49. Merino, J.M., León, M., Rueda, F., and Diaz, R., Thin Solid Films, 361-362 (2000) 22-27. Sakata, H., and Ogawa, H., Sol. Energy Mater. Sol. Cells, 63 (2000) 259-265.  Akl, A.A.S., Ashour, A., Ramadan, A.A., and El-Hady, K.A., Vacuum, 61 (2001) 75-84. Joseph, C.M., and Menon, C.S., J. Phys. D: Appl. Phys., 34 (2001) 1143-1146.  Victor, P., Nagaraju, J., and Krupanidhi, S.B., Solid State Comm., 116 (2000) 649-653. Kuranouchi, S. and Yoshida, A., Thin Solid Films, 343-344 (1999) 123-126.  McAleese, J., O’Brien, P., and Otway, D. J., Chem. Vap. Deposition, 4 (1998) 94-96.  Jones, P.A., Jackson, A.D., Lickiss, P.D., Pilkington, R.D., and Tomlinson, R.D., ThinSolid Films, 238 (1994) 4-7.  Duchemin, S., Artaud, M.C., Ouchen, F. and Bougnot, J., J. Mater. Sci.: Mater. Electron.,7 (1996) 201-205. Artaud, M.C., Ouchen, F., Martin, L., and Duchemin, S., Thin Solid Films, 324 (1998) 115-123.
 Massé, G., Djessas, K., Monty, C., and Sibieude, F., Thin Solid Films, 414 (2002) 192-198. El Haj Moussa, G.W., Ariswan, Khoury, A., Guastavino, F., and Llinarés, C., Solid StateComm., 122 (2002) 195-199.  Bhattacharya, R.N., Hiltner, J.F., Batchelor, W., Contreras, M.A., Noufi, R.N., and Sites,J.R.,Thin Solid Films, 361-362 (2000) 396-399.  Bhattacharya, R.N., Batchelor, W., Ramanathan, K., Contreras, M.A., and Moriarty, T.,Sol. Energy Mater. Sol. Cells, 63 (2000) 367-374.  Bhattacharya, R.N., J. Electrochem. Soc., 130 (1983) 2040-2042.  Bhattacharya, R.N., Batchelor, W., Granata, J.E., Hasoon, F., Wiesner, H., Ramanathan,K., Keane, J., and Noufi, R. N., Sol. Energy Mater. Sol. Cells, 55 (1998) 83-94.  Garg, J.C., Sharma, R.P., and Sharma, K.C., Thin Solid Films, 164 (1988) 269-273. Reddy, K.T.R., Chalapathy, R.B.V., Slifkin, M.A., Weiss, A.W., and Miles, R.W., ThinSolid Films, 387 (2001) 205-207. Shirakata, S., Kannaka, Y., Hasegawa, H., Kariya, T., and Isomura, S., Jpn. J. Appl. Phys.,38 (1999) 4997-5002. Başol, B. M., Thin Solid Films, 361-362 (2000) 514-519. Eberspacher, C., Fredric, C., Pauls, K., and Serra, J., Thin Solid Films, 387 (2001) 18-22. Norsworthy, G., Leidholm, C.R., Halani, A., Kapur, V.K., Roe, R., Başol, B.M., Matson,R., Sol. Energy Mater Sol. Cells, 60 (2000) 127-134. Rau, U., and Scmidt, M., Thin Solid Films, 387 (2001) 141-146. Contreras, M.A., Romero, M.J., To, B., Hasoon, F., Noufi, R., Ward, S., and Ramanathan,K., Thin Solid Films, 403-404 (2002) 204-211.  Garg, P., Garg, A., Rastogi, A.C. and Garg, J.C., J. Phys. D: Appl. Phys., 24 (1991) 2026-2031.  Qiu, C.X. and Shih, I., Can. J. Phys., 65 (1987) 1011-1014.  Sahu, S.N., Kristensen, R.D.L., and Haneman, D., Sol. Energy Mater., 18 (1989) 385-397. Qiu, S.N., Li, L., Qiu, C.X., Shih, I., and Champness, C.H., Sol. Energy Mater. Sol. Cells,37 (1995) 389-393.  Rockett, A., and Birkmire, R.W., J. Appl. Phys., 70 (1991) R81-R97.  Sudo, Y., Endo, S., and Irie, T., Jpn. J. Appl. Phys., 32 (1993) 1562-1567.  Lincot, D., Froment, M., and Cachet, H., in Advances in Electrochemical Science andEngineering, Vol 6 , Edited by R.C. Alkire and D.M. Kolb, Wiley-VCH, Weinheim, Germany,1999, p. 165-235 Hashimoto, Y., Kohara, N., Negami, T., Nishitani, N., and Wada, T., Sol. Energy Mater.Sol. Cells, 50 (1998) 71-77. Qiu, S.N., Lam, W.W., Qiu, C.X., and Shih, I., Appl. Surf. Sci., 113/114 (1997) 764-767. Kylner, A., Rockett, A. and Stolt, L., Solid State Phenom., 51-52 (1996) 533-540.  Guillén, C., Martínez, M.A., Maffiotte, C., and Herrero, J., J. Electrochem. Soc., 148(2001) G602-G606.
 Kylner, A., J. Appl. Phys., 85 (1999) 6858-6865.  Friedlmeier, T.M., Braunger, D., Hariskos, D., Kaiser, M., Wanka, H.N., and Schock,H.W., in Proc. 25th IEEE Photovolt. Spec. Conf., Washington, D.C., USA (1996) p. 845-848.  CRC Handbook of Chemistry and Physics 82nd Ed., Edited by D.R. Lide, CRC Press, Inc.,Boca Raton, FL, 2001-2002. Canawa, B., Guillemoles, J.-F., Yousfi, E.-B., Cowache, P., Kerber, H., Loeffl, A., Schock,H.-W., Powalla, M., Hariskos, D., and Lincot, D., Thin Solid Films, 361-362 (2000) 187-192.  Bär, M., Muffler, H.-J., Fischer, C.-H., Zweigart, S., Karg, F., and Lux-Steiner, M.C., Prog.Photovolt.: Res. Appl., 10 (2002) 173-184.  Başol, B. M., Kapur, V. K., Norsworthy, G., Halani, A., Leidholm, C. R., and Roe, R.,Electrochem. Solid-State Lett., 1 (1998) 252-254.  Kushiya, K., Nii, T., Sugiyama, I., Sato, Y., Inamori, Y., and Takeshita, H., Jpn. J. Appl.Phys., 35 (1996) 4383-4388.  Ennaoui, A., Siebentritt, S., Lux-Steiner, M.Ch., Riedl, W., and Karg, F., Sol. EnergyMater. Sol. Cells, 67 (2001) 31-40.  Hariskos, D., Ruckh, M., Rühle, U., Walter, T., Schock, H.W., Hedström, J., and Stolt, L.,Sol. Energy Mater. Sol. Cells, 41/42 (1996) 345-353. Muffler, H.-J Bär, M., Fischer, C.-H., Gay, R., Karg, F., and Lux-Steiner, M.C., in Proc.28th IEEE Photovolt. Spec. Conf., Anchorage, AK, USA (2000) p. 610-613. Siebentritt, S., Kampschulte, T., Bauknecht, A., Blieske, U., Harneit, W., Fiedeler, U., andLux-Steiner, M., Sol. Energy Mater. Sol. Cells, 70 (2002) 447-457.  Guillemoles, J.-F., Canawa, B., Yousfi, E.B., Cowache, P., Galtayries, A., Asikainen, T.,Powalla, M., Hariskos, D., Schock, H.-W., and Lincot, D., Jpn. J. Appl. Phys., 40 (2001) 6065-6068.  Yousfi, E.B., Asikainen, T., Pietu, V., Cowache, P., Powalla, M., and Lincot, D., Thin SolidFilms, 361-362 (2000) 183-186.  Ohtake, Y., Kushiya, K., Ichikawa, M., Yamada, A., and Konagai, M., Jpn. J. Appl. Phys.,34 (1995) 5949-5955.  Ohtake, Y., Okamoto, T., Yamada, A., Konagai, M., and Saito, K., Sol. Energy Mater. Sol.Cells, 49 (1997) 269-275.  Ohtake, Y., Ichikawa, M., Okamoto, T., Yamada, A., Konagai, M., and Saito, K., in Proc.25th IEEE Photovolt. Spec. Conf., Washington, D.C., USA (1996) p. 793-796.  Tuttle, J.R., Berens, T.A., Keane, J., Ramanathan, K.R., Granata, J., Bhattacharya, R.N.,Wiesner, H., Contreras, M.A., and Noufi, R., Proc. 25th IEEE Photovolt. Spec. Conf.,Washington, D.C., USA (1996) p. 797-800.  Delahoy, A., Bruns, J., Chen, L., Akhtar, M., Kiss, Z., and Contreras, M., in Proc. 28th
IEEE Photovolt. Spec. Conf., Anchorage, AK, USA (2000) p. 1437-1440. Sugiyama, T., Chaisitsak, S., Yamada, A., Konagai, M., Kudriavtsev, Y., Godines, A.,Villegas, A., and Asomoza, R., Jpn. J. Appl. Phys., 39 (2000) 4816-4819.  Nakada, T., and Mizutani, M., in Proc. 28th IEEE Photovolt. Spec. Conf., Anchorage, AK,
USA (2000) p. 529-534.  Kushiya, K., and Yamase, O., Jpn. J. Appl. Phys., 39 (2000) 2577-2582.  Hariskos, D., Powalla, M., Chevaldonnet, N., Lincot, D., Schindler, A., and Dimmler, B.,Thin Solid Films, 387 (2001) 179-181. Cooray, N.F., Kushiya, K., Fujimaki, A., Sugiyama, I., Miura, T., Okumura, D., Sato, M.,Ooshita, M., and Yamase, O., Sol. Energy Mater. Sol. Cells, 49 (1997) 291-297.  Sang, B., Kushiya, K., Okumura, D., and Yamase, O., Sol. Energy Mater. Sol. Cells, 67(2001) 223-245. Chaisitsak, S., Sugiyama, T., Yamada, A., and Konagai, M., Jpn. J. Appl. Phys., 38 (1999)4989-4992.  Stolt, L., Hedström, J., and Skarp, J., in Proc. 1st World Conf. Photovolt. Energy Conv.,Waikoloa, Hawaii (1994) p. 250-253.  Olsen, L.C., Addis, F.W., Huang, L., Shafarman, W.N., Eschbach, P., and Exarhos, G. J.,in Proc. 28th IEEE Photovolt. Spec. Conf., Anchorage, AK, USA (2000) p. 458-461.  Gal, D., Hodes, G., Lincot, D., and Schock, H.-W., Thin Solid Films, 361-362 (2000) 79-83. Pandey, R. K., Sahu, S.N., and Chandra, S., Handbook of Semiconductor Electrodeposition,Marcel Dekker, New York, 1996. 289 p.  Saloniemi, H., Kanniainen, T., Ritala, M., and Leskelä, M., Thin Solid Films, 326 (1998)78-82. Saloniemi, H., Kanniainen, T., Ritala, M., Leskelä M., and Lappalainen, R., J. Mater.Chem., 8 (1998) 651-654. Thouin, L., Massaccesi, S., Sanchez, S., and Vedel, J., J. Electroanal. Chem., 374 (1994)81-88. Massaccesi, S., Sanchez, S., and Vedel, J., J. Electrochem. Soc., 140 (1993) 2540-2546. Thouin, L., and Vedel, J., J. Electrochem. Soc., 142 (1995) 2996-3001.  Pottier, T., and Maurin, G., J. Appl. Electrochem., 1 9 (1989) 361-367. Molin, A.N., Dikusar, A.I., Kiosse, G.A., Petrenko, P.A., Sokolovsky, A.I., andSaltanovsky, Yu.G., Thin Solid Films, 237 (1994) 66-71. Molin, A.N., and Dikusar, A.I., Thin Solid Films, 237 (1994) 72-77.  Oliveira, M.C.F., Azevedo, M., and Cunha, A., Thin Solid Films, 405 (2002) 129-134. Pourbaix, M., Atlas of Electrochemical Equilibria in Aqueous Solutions, Pergamon Press,New York (1966) Ganchev, M.G., and Kochev, K.D., Sol. Energy Mater. Sol. Cells, 31 (1993) 163-170.  Guillén, C., and Herrero, J., J. Electrochem. Soc., 141 (1994) 225-230. Xu, J.L., Yao, X.F., and Feng, J.Y., Sol. Energy Mater. Sol. Cells, 73 (2002) 203-208. Ueno, Y., Kawai, H., Sugiura, T., and Minoura, H., Thin Solid Films, 157 (1988) 159-168. Raffaelle, R.P., Forsell, H., Potdevin, T., Friedfeld, R., Mantovani, J.G., Bailey, S.G.,Hubbard, S.M., Gordon, E.M., and Hepp, A.F., Sol. Energy Mater. Sol. Cells., 57 (1999) 167-178.
 Tzvetkova, E, Stratieva, N., Ganchev, M., Tomov, I., Ivanova, K., and Kochev, K., ThinSolid Films, 311 (1997) 101-106. Edamura, T., and Muto, J., J. Mater. Sci., 5 (1994) 275-279. Kampmann, A., Sittinger, V., Rechid, J., and Reineke-Koch, R., Thin Solid Films, 361-362(2000) 309-313. Calixto, M.E., and Sebastian, P.J., Sol. Energy Mater. Sol. Cells, 63 (2000) 335-345. Sebastian, P.J., Calixto, M.E., Bhattacharya, R.N., and Noufi, R., Sol. Energy Mater. Sol.Cells, 59 (1999) 125-135. Khare, N., Razzini, G., and Bicelli, L.P, Thin Solid Films, 186 (1990) 113-128. Ugarte, R., Schrebler, R., Córdova, R., Dalchiele, E. A., and Gómez, H., Thin Solid Films,340 (1999) 117-124. Lokhande, C.D., J. Electrochem. Soc., 134 (1987) 1727-1729. Nomura, S., Nishiyama, K., Tanaka, K., Sakakibara, M., Ohtsubo, M., Furutani, N., andEndo, S., Jpn. J. Appl. Phys., 37 (1998) 3232-3237.  Chraibi, F., Fahoume, M., Ennaoui, A., and Delplancke, J.L., Phys. Stat. Sol. (a), 186(2001) 373-381.  Pern, F. J., Noufi, R., Mason, A., and Franz, A., Thin Solid Films, 202 (1991) 299-314.  Guillén, C., and Herrero, J., J. Electrochem. Soc., 141 (1995) 1834-1838. Friedfeld, R., Raffaelle, R.P., and Mantovani, J.G., Sol. Energy Mater. Sol. Cells., 58(1999) 375-385. Menezes, S., Electrochem. Solid-State Lett., 5 (2002) C79-C81. Baoming, H.M., Lister, T.E. and Stickney, J.L., in The Handbook of Surface Imaging andVisualization, Edited by Arthur T. Hubbard, CRC Press, Inc., Boca Raton, Florida, 1995, p. 75-91 Buttry, D. A., and Ward, M. D., Chem. Rev., 92 (1992) 1355-1378. Deakin, M. R., and Buttry, D. A., Anal. Chem., 61 (1989) 1147A-1154A.  Sauerbrey, G., Z. Phys., 155 (1959) 206-222. Buttry, D.A., in Electroanalytical Chemistry, Vol. 17, Edited by A.J. Bard, Dekker, NewYork, 1991, p. 1-85 Mori, E., Baker, C.K., Reynolds, J.R., and Rajeshwar, K., J. Electroanal. Chem., 252(1988) 441-451.  Matias, J.G.N., Juliao, J.F., Soares, D.M., and Gorenstein, A., J. Electroanal.Chem., 451(1997) 163-169.  Wei, C., Myung, N., and Rajeshwar, K., J. Electroanal. Chem., 347 (1993) 223-235. Saloniemi, H., Kemell, M., Ritala, M., and Leskelä, M., J. Electroanal. Chem., 482 (2000)139-148.  Wei, C., Bose, C.S.C., and Rajeshwar, K., J. Electroanal. Chem., 327 (1992) 331-336. Myung, N., Jun, J.H., Ku, H.B., Chung, H.K., and Rajeshwar, K., Microchem. J., 62 (1999)15-25. Saloniemi, H., Kemell, M., Ritala, M., and Leskelä, M., J. Mater. Chem., 10 (2000) 519-525.
 Neshkova, M.T., Nikolova, V.D., and Petrov, V., J. Electroanal. Chem., 487 (2000) 100-110.  Marlot, A., and Vedel, J., J. Electrochem. Soc., 146 (1999) 177-183. de Tacconi, N.R., Rajeshwar, K., Lezna, R.O., J. Phys. Chem., 100 (1996) 18234-18239. de Tacconi, N. R., and Rajeshwar, K., J. Electroanal. Chem., 444 (1998) 7-10. de Tacconi, N.R., Medvedko, O., and Rajeshwar, K., J. Electroanal. Chem., 379 (1994)545-547. Saloniemi, H., Kemell, M., Ritala, M., and Leskelä, M., Thin Solid Films, 386 (2001) 32-40.  Pauporté, T., and Lincot, D., J. Electroanal. Chem., 517 (2001) 54-62.  Tan, M.X., Laibinis, P.E., Nguyen, S.T., Kesselman, J.M., Stanton, C.E., and Lewis, N.S.,Prog. Inorg. Chem., 41 (1994) 21-144. Nozik, A. J., and Memming, R., J. Phys. Chem., 100 (1996) 13061-13078. Rajeshwar, K. and de Tacconi, N. R., in Studies in Surface Science and Catalysis, Vol 103,Edited by P.V. Kamat and D. Meisel, (editors), Elsevier, Amsterdam, 1996, p.321-351 Menezes, S., Mater. Res. Soc. Symp. Proc., 426 (1996) 189-194. Mishra, K.K., and Rajeshwar, K., J. Electroanal. Chem., 271 (1989) 279-294.  Guillén, C., Herrero, J., and Lincot, D., J. Appl. Phys., 76 (1994) 359-362. Siripala, W., Vedel, J., Lincot, D., and Cahen, D., Appl. Phys. Lett., 62 (1993) 519-521. Ahrland, S., and Tagesson, B., Acta Chem. Scand., A 31 (1977) 615-624. Waldo, R. A., Microbeam Anal. (1988) 310. Ylilammi, M., Ranta-aho, T., Thin Solid Films, 232 (1993) 56-62. Koh, W. Kutner, W., Jones, M.T., and Kadish, K.M., Electroanalysis, 5 (1993) 209-214. Massaccesi, S., Sanchez, S., and Vedel, J., J. Electroanal. Chem., 412 (1996) 95-101. Kylner, A., J. Electrochem. Soc. 146 (1999) 1816-1823. M. Izaki, and T. Omi, J. Electrochem. Soc., 143 (1996) L53-L55. Schroder, D.K., Semiconductor material and device characterization, Wiley, New York, 2nd
ed. (1998)  Mauk, P.H., Tavakolian, H., and Sites, J.R., IEEE Trans. Electron Dev., 37 (1990) 422-427. Powder Diffraction Files, Card 06-0680, International Centre for Diffraction Data,Pennsylvania, PA Schumacher, R., Borges, G. and Kanazawa, K. K., Surf. Sci. 163 (1985) L621-L626. Shih, I., Qiu, C.X., Qiu, S.N., and Huang, J.F., J. Appl. Phys., 63 (1988) 439-441. Santamaria, J., Gonzalez-Diaz, G., Iborra, E., Martil, I., and Sanchez-Quesada, F., J. Appl.Phys., 65 (1989) 3236-3241.  Noufi, R., Axton, R., Herrington, C., and Deb, S.K., Appl. Phys. Lett., 45 (1984) 668-670. Smith, R.M., and Martell, A.E., NIST Critically Selected Stability Constants for MetalComplexes Database, Version 4.0 (1997)  Minami, T., MRS Bull., 25 (2000) 38-44.
 Naghavi, N., Marcel, C., Dupont, L., Rougier, A., Leriche, J.-B., and Guéry, C., J. Mater.Chem., 10 (2000) 2315-2319. Powder Diffraction Files, Card 36-1451, International Center for Diffraction Data,Haverford, PA Powder Diffraction Files, Card 16-0161, International Center for Diffraction Data,Haverford, PA Nunes, P., Fortunato, E., Vilarinho, P., and Martins, R., Int. J. Inorg. Mater., 3 (2001)1211-1213. Martínez, M.A., and Guillén, C., Surf. Coat. Technol., 110 (1998) 62-67.